# MODELLING OF SOME EQUILIBRIUM THERMODYNAMIC PROPERTIES OF

### Transcript of MODELLING OF SOME EQUILIBRIUM THERMODYNAMIC PROPERTIES OF

MODELLING OF SOME

EQUILIBRIUM THERMODYNAMIC PROPERTIES

OF POLYMER SYSTEMS

Alexander Stroeks

MODELLING OF SOME

EQUILIBRIUM THERMODYNAMIC PROPERTIES

OF POLYMER SYSTEMS

~

Schematic representation of a central cell with all adjacent sites occupied.

MODELLING OF SOME

EQUILIBRIUM THERMODYNAMIC PROPERTIES

OF POLYMER SYSTEMS

Proefschrift

ter verkrijging van de graad van doctor aan de Technische Universiteit Eindhoven, op gezag van de Rector Magnificus, prof. dr. J.H. van Lint, voor

een commissie aangewezen door bet College van Dekanen in bet openbaar te verdedigen op

dinsdag 21 mei 1991 om 16.00 uur

door

Alexander Antonius Marie Stroeks Geboren te Heerlen

druk: wibro dissertatiedrukkerij, helmond"

Dit proefschrift is goedgekeurd door

de promotoren :

en de copromotor :

Prof.dr.R.Simha

Prof.dr.P J.Lemstra

Dr.E.Nies

Het in dit proefschrift beschreven onderzoek werd uitgevoerd onder auspicien van de

Stichting Scheikundig Onderzoek in Nederland (SON) met financiele steun van de

Nederlandse Organisatie voor Wetenschappelijk Onderzoek (NWO).

De natuur gedoogt dat gij haar bespiedt, niet dat gij haar ontraadselt.

Pythagoras

Contents

Contents

Chanter 1 Introduction

1.1 General Introduction

1.2 Objective of the present investigation

1.3 Outline of the thesis

Chanter 2 Theoretical considerations

2.1 The liquid state

2.2 Equihbrium statistical mechanics

2.3 Simha-Somcynsky theory for low molar mass fluids

2.4 Simha-Somcynsky theory for polymers

2.5 A modified hole theory for polymers and low molar mass

fluids

2.6 Basic thermodynamic equations

2.6.1 Equation of state

2.6.2 Hehnholtz free energy

2.7 Generalization for multicomponent fluids

2.8 Basic thermodynamic equation for multicomponent systems

2.9 Phase behaviour

2.10 Analogy with other equation of state theories

2.11 Cell models

2.12 The Flory-Orwoll-Vrij theory

2.13 The Sanchez-Lacombe theory

1

4

4

7

9 11

17

18 20

20

22

22

25

26

28

29

30

33

i

ii Contents

Chapter 3 Equation of state behaviour of pure components

3.1 Introduction 37

3.2 Comparison of equation of state models; a literature survey 37

3.3 Comparison Simha-Somcynsky / Holes-Huggins model 39

3.3.1 Universal PVT surface 39

3.3.2 Experimental data 42

3.4 Molecular parameters for studied systems according to SS

and HH theories

3.5 Conclusions

Polymer Solution Section

47 50

Chapter 4 Computation of Phase Equilibria : Comparison of Approximate

and Exact Methods

4.1 Introduction

4.2 Phase behaviour of the system polyethylenefn-hexane

4.3 Conclusions

Chapter 5 Phase Behaviour : Influence of Pressure, Temperature,

Composition and Molar Mass

5.1 Introduction

5.2 The system polystyrene/cyclohexane

5.2.1 Selected experimental data

5.2.2 Determination of molecular parameters

5.2.3 Phase behaviour under atmospheric conditions

5.2.4 Pressure influence on phase behaviour

53

54

64

65

65

65

66

67

72

Contents

5.3 The system polystyrenefmethylacetate 84

5.3.1 Introduction 84

5.3.2 Selected Experimental Data 84

5.3.3 Determination of molecular parameters 86

5.3.4 Phase behaviour under atmospheric conditions 88

5.3.5 Pressure influence on phase behaviour 89

5.4 Conclusions 95

Chanter 6 Thermodynamic Excess Functions and Correlations with Phase

Behaviour

6.1 Introduction and some general principles 97

6.2 The system Polystyrene I Cyclohexane 100

6.2.1 Link between excess volume and pressure influence

on phase behaviour 100

6.2.2 Confrontation of theory with experimental excess

volumes

6.3 The system Polystyrene I Methylacetate

6.4 Conclusions

Chapter 7 The Flory Huggins parameter

7.1 Introduction

7.2 Definitions for computation of Xscac parameters

7.3 Xsca1 and its contributions

7.4 Comparison of theoretical Xsca1-values with experiment

7.5 Conclusions

104 112

114

115

117

119

126

131

iii

iv

POLYMER BLEND SECTION

Chapter 8 Phase Behaviour : Influence of Pressure, Temperature,

Composition and Molar Mass

8.1 Introduction

8.2 Model computations for a hypothetical blend

8.3 Phase behaviour of the system polystyrene/

poly(paramethylstyrene)

8.3.1 Introduction

8.3.2 Experimental

8.3.3 Experimental results

8.3.4 Theoretical study of phase behaviour

8.4 Conclusions

Contents

135

136

144

144

145

147

150

153

Chapter 9 Thermodynamic Excess Functions and Correlations with Phase

Behaviour

9.1 Introduction

9.2 Hypothetical model blend

9.3 The system polystyrene I poly(paramethylstyrene)

9.4 Conclusions

Chapter 10 References

Future Outlook

Summary

Samenvatting

Nomenclature

Dankwoord

Curriculum Vitae

155

157

159

161

163

168

169

173

177

182

183

Introduction 1

1. Introduction

1.1 General Introduction

It is easy to elucidate that miscibility aspects play an important role in the

development of synthetic polymer materials. Miscibility and its consequences are

encountered in various stages of polymer product development, varying from the

synthesis of polymers, the processing of polymer materials and the

characterization of these products.

Miscibility behaviour may have a large impact on the ultimate properties of

polymer materials. This is certainly the case for polymer blends. To meet the

growing demands concerning the ultimate set of properties of polymer materials,

two or more polymers are mixed. Depending on the application of the material

the morphology may range from a completely homogeneous (miscible) material

to a two or multiphase (immiscible) system. During processing polymer blends

are subjected to extreme conditions; elevated temperatures and pressures are

reached and high shear forces may occur. All these factors influence the

miscibility of the system and consequently its ultimate properties. For the

development of polymer blends it is therefore of great importance to gain more

insight in the relation between processing conditions and polymer demixing

phenomena.

Also in the area of polymer synthesis knowledge of polymer miscibility is

essential. A vast majority of all synthetic polymer materials is produced by either

solution or bulk polymerization. During the polymerization process the polymer

product may segregate depending on reaction conditions but also depending on

the polymer molar mass. Consequently a polymer-rich second phase is formed

which is for many practical reasons mostly unwanted and has to be avoided. This

can be achieved by the use of another solvent or combinations of solvents in the

2 Chapter 1

case of solution polymerization. In the case of bulk polymerization, the reactor

conditions have to be changed which might have consequences for the reactor

design. These examples illustrate that also in polymer synthesis, miscibility

problems are frequently encountered and a detailed understanding of polymer

miscibility seems desirable and even necessary in order to solve these problems.

In general, miscibility is determined by the equilibrium thermodynamic

functions of state. In view of the time scale of the kinetic processes in

comparison to the time scale of the experiment, the equilibrium situation is most

easily reached for polymer solutions. For polymer blends however, true

equilibrium is not always obtained. Knowledge of the equilibrium situation is still

valuable though, because it forms the driving force for the kinetically controlled

processes and therefore will determine to a great extent the ultimate structure

of the system.

For 25 years it has been known that equation of state properties determine

equilibrium thermodynamic properties of polymer systems. This was

demonstrated unambiguously by the cell model of Prigogine [1] and later by the

equation of state theory of Flory, Orwoll and Vrij [2-5]. This latter lattice model

had a tremendous impact on the thermodynamic research related to polymer

systems. Since then many equation of state theories have been proposed on this

subject. These theories have provided the relevant parameters which are

responsible for e.g. LCST (Lower Critical Solution Temperature) demixing

phenomena, frequently encountered in polymer systems and for the influence

exerted by pressure on miscibility behaviour. The older Flory-Huggins theory [6-

9], which ignores equation of state properties, completely fails to predict LCST

phase behaviour.

Introduction 3

The classical equation of state theories can be subdivided in three main

classes.

In a first category we find the cell theories, e.g. the earlier mentioned cell

model of Prigogine [1 ], the Flory-Orwoll-Vrij theory [2-5], the approach of Walsh

and Dee [10,11] and the recent approach of Kammer [12]. In all these lattice

theories the compressibility and thermal expansion of the polymer system are

explained solely by changes in cell volume.

In a second class the lattice fluid theory of Sanchez and Lacombe [13-15], the

approach of Panayioutou and Vera [16] and the lattice gas model of Koningsveld

and Kleintjens [17-19] are situated. In these theories volume changes of the

polymer systems are modelled by allowing a variation of empty sites on the

lattice while the cell volume is assumed to be constant.

Finally we have the hole theories where the basic ideas of the above two

groups of theories are incorporated. Allowance is made for cell size variation

whereas a change in the number of vacancies on the lattice is also taken into

account. An example of such a theory is the Simha-Somcynsky theory [20]. This

theory has been developed in the late 1960's for the description of

thermod}'namic equilibrium properties of pure components. This theory is

particularly successful in the description and prediction of properties related to

equation of state behaviour [21-25]. Therefore it provides a solid basis for the

theoretical study of equation of state behaviour of multicomponent polymer

systems. With the introduction of extra mixing rules [26], based on the ideas of

Prigogine (1], the equation of state behaviour of polymer solutions as well as of

polymer blends was described in a fruitful manner [27,28]. From this point it was

logical to proceed in the direction of enumeration of phase behaviour of polymer

multicomponent systems. For the Simha-Somcynsky theory, the first study was

given by Simha and Jain [29]. As a start, these authors set out to investigate as

an example the LCST phase behaviour in a particular solution, namely

polyethylene in n-hexane. In this study, the compositional derivatives of the free

4 Chapter 1

energy of mixing, required for the description of phase behaviour, were

approximated by polynomial fits to the theoretical free energy. Most important

conclusions from this work are that the Simha-Somcynsky theory is indeed

capable in describing LCST phase behaviour and that this behaviour is strongly

dictated by the theoretical free volume fractions of the pure components. It was

basically this study which opened the way for a further and more detailed

analysis of polymer phase equilibria in the framework of the Simha-Somcynsky

theory and related theories. At this point we have reached the objective of this

thesis.

1.2 Objective of the present investigation

The objective of this work is the study of miscibility behaviour and related

properties of polymer systems in the framework of the hole theories. This study

is aimed to provide more insight in the theoretical factors which govern polymer

miscibility.

1.3 Outline of the thesis

In chapter 2 the theoretical background of the Simha-Somcynsky theory and

its relation with other equation of state theories are discussed. Furthermore a

theoretical modification of this theory will be presented.

In chapter 3 the process of the extraction of pure component model

parameters from equilibrium equation of state data is presented. The Simha

Somcynsky theory and its modified version are compared to other equation of

state theories in their ability to describe pure component equation of state data

[30].

As mentioned earlier in this chapter, Jain and Simha gave the first description

Introduction 5

of miscibility behaviour of polymer systems in the framework of the Simha

Somcynsky theory. A polynomial fit of the Gibbs free energy of mixing was used

to compute the compositional derivatives which govern phase behaviour. In

chapter 4 this procedure is compared with exact and more general computations

of these derivatives. Consequences for the computed phase behaviour of the

solution polyethylenefn-hexane are discussed [31].

In chapter 5 the Simha-Somcynsky theory and its modified version are

confronted with detailed experimental miscibility information of the solution

polystyrenefcyclohexane (32-35]. Especially the complicated and subtle influence

of pressure on miscibility will be thoroughly examined. Furthermore the modified

version of the theory is used to investigate miscibility behaviour of the

polystyrenefmethylacetate solution. Again the influence of pressure plays an

important role in this study.

Chapter 6 deals with the relation between pressure influence on miscibility

and thermodynamic excess functions. Experimental excess volume data of the

solution polystyrene/cyclohexane, together with demixing information of chapter

5, serve to illustrate this relation.

In chapter 7 x-parameters, generated with the Simha-Somcynsky theory and

the modified version, are presented for the solution polystyrene/cyclohexane.

A comparison is made with x-parameters from literature [36-39], which are

determined from light scattering experiments. The contributions of the different

theoretical factors to the x-parameter are elucidated.

Chapter 8 deals with phase behaviour of polymer blends as described by the

original and the modified version of the Simha-Somcynsky theory. In first

instance phase behaviour is investigated for a hypothetical model blend. The

influences of molar mass of the constituents and pressure effects on the phase

diagrams are studied systematically. Furthermore the miscibility behaviour of the

polymer blend polystyrene /poly(paramethylstyrene) under atmospheric conditions

6 Chapter 1

is determined experimentally [40]. The Differential Scanning Calorimetry (DSC)

and the phase optical microscopy techniques served to detect phase separation.

The experimental results were used to test the modified version of the Simha

Somcynsky theory ..

Theoretical predictions concerning the excess functions of the hypothetical

model blend and the blend polystyrenefpoly(paramethylstyrene) are presented

in chapter 9.

This thesis is partly based on a collection of publications which have been

published in various journals [30-35,40).

Tbeoretic:al considerations 7

2. Theoretical considerations

2.1 The liquid state

To describe the disordered liquid state different theoretical approaches have

been considered. The efforts for polymer systems closely mimic the

developments presented for small polymer systems. On the most primitive

statistical mechanical level one can distinguish between the radial distribution

function theories and the approaches based on the partition function. For small

molecule systems the RDF theories have proven to be very successful [41]. It is

only quite recently that these theories are applied for polymer systems.In this

respect the work of Curro and Schweizer [42,43] deserves a lot of credit. The

work presented in this thesis is based on the partition function approach which

was developed earlier and in the polymer field has a longstanding scientific

history. In an attempt to describe the disordered liquid state in the partition

function concept two extreme approaches are possible.

One can start from a gas which can be represented as a set of particles

moving around in space quite independently because of the low particle density.

A liquid can be regarded as a pseudo-gas system with a significantly increased

density. Focussing on a single particle, this means the number of particles in the

direct surrounding space will increase substantially as a result of this

densification process. This effect restricts the mobility of the particle and

introduces a kind of short-range ordering which is characteristic for a liquid but

is missing in a gas.

An alternative way of imagining the liquid state is the crystal-like approach.

A crystal can be pictured as a set of particles with each particle vibrating with

a small amplitude around its equilibrium position. This oscillation process takes

place in an environment formed by all the neighbouring particles. Mter melting

the crystal the density of the system will decrease slightly as a result of a small

8 Chapter 2

increase in interparticle distance. The mobility of the particles will be enhanced

in such a way that the concept of small vibrations is not valid any more.

However, the specific heat of a liquid just above its melting point is about the

same as that for the crystal [44]. This fact supports the idea of the particle still

moving 'in a restricted space formed by its neighbouring species.

On the basis of experimental data on simple liquids, is it possible to give

preference to the gas· or to the crystal-like approach in the discription of the

liquid state? Or stronger, is it even possible to reject one of these options? To

give an answer to these intriguing questions the illustrative neutron-scattering

experiments on liquid krypton by Clayton and Heaton [45] will serve. For the

present discussion a description of the experimental setup or the refined

interpretation of the scattering data will be omitted. Only the basic outcome of

their work will be presented. From scattering experiments on liquid krypton at

various temperatures they concluded that the nearest neighbour interatomic

distance increased only slightly with temperature whereas the number of nearest

neighbours decreases substantially (see table 2.1).

Table 2.1 Neutron scattering results on liquid krypton

Temp Density Nearest neighbour Number of nearest

(K) (atoms/A') distance (A) neighbours

117 0.0176 4.02 8.5

133 0.0166 4.04 8.0

153 0.0154 4.08 7.0

183 0.0130 4.10 6.5

210 0.0075 4.20 4.0

The slight increase of the nearest neighbour distance with temperature supports

the crystal-like concept whereas the decrease of number of nearest neighbours

underlines , the gaseous character of a fluid. On the basis of these basic

Theoretical considerations 9

experimental results a molecular theory for a fluid should involve both distinct

ideas about the nature of the fluid.

A theory, in which both ideas are contemplated, is the Simha-Somcynsky hole

theory [20]. This theory is based on statistical mechanics as will be shown. It was

formulated in the late sixtees by Simha and Somcynsky and can be applied to

low molar mass species as well as to polymers. Going the way from statistical

mechanics to the ultimate working equations, several assumptions are made. In

first instance a brief introduction in rigorous statistical mechanics is presented.

Subsequently the Simha-Somcynsky theory and the relevant assumptions are

discussed for low molar mass components. Later on a generalization will be

made towards polymers. The extension towards multicomponent systems will be

considered in detail.

2.2 Equilibrium statistical mechanics

A system of prescribed temperature and volume is considered with r different

accessible quantum states. The partition function or sum-over-all-states Z is

defined by either of two equivalent expressions :

Z = }; exp(·ErfkT) }; & exp(·ErfkT) (2.1) r r

with k Boltzmann's constant and T the absolute temperature. In the first

expression Er is associated with the energy of the system in a quantum state with

quantum numbers {j} = j 1, j2, •••• On the other band , in the second expression

Er is the energy representing the r energy level. This level is degenerated in

& states. The partition function is closely related to the Helmholtz free energy

A of the system :

A= -kT In Z (2.2)

10 Chapter 2

and presents the key in the derivation of all other thermodynamic properties of

the system. The energy Er consists of different contributions due to different

degrees of freedom. Translational degrees of freedom which determine the

positions and motions of the mass-centres of the molecules are predominant in

this respect. In classical statistical mechanics the translational partition function

for a system of N identical molecules reads [1]:

with

(2.4)

where Pi is the momentum corresponding to the centre of mass of the i'th

molecule, ri its position, U the potential energy of the whole system, h Planck's

constant and m the mass per molecule. The integration is performed over the

momenta and positions of all individual molecules. The integration over

momenta in the partition function may be performed so that Z1r may be written

in the form:

ztr = ~3~N! J exp (-k~ ) dr1 ... drN = :: (2.5)

with ~2 = h2/(211'mkT).

The factor 1/>.3N represents the contribution from the kinetic energy to the

partition function. zconf is the configurational partition function and reflects the

potential energy distributions .. Z1r forms the starting point in the derivations of

the thermodynamic properties one is interested in.

Theoretical considerations 11

2.3 Simha-Somcynsky theory for low molar mass fluids

The above given expression for the partition function is a general one and it

is applicable to the solid, fluid or gaseous phase of monatomic components. To

obtain the partition function for a liquid the volume V of the system is split up

into a number of cells. With the scattering results of Clayton and Heaton in

mind, allowance is made for the presence of empty cells or holes. Let y denote

the fraction of occupied cells. Furthermore the molecules in the cells have a

certain mobility to wander around in their individual cells. It is assumed that the

cells are sufficiently small, so there is a negligible probability of finding two

molecules within the same cell. The cells however are large enough to

accomodate one molecule, i.e. s = 1 where s represents the number of occupied

cells per molecule.

Focussing on one particular occupied cell, two extreme situations may occur.

All the adjacent cells can be occupied whereas in the other extreme all are

vacant (situations sketched in fig.2.1a and b).

ace-----,~ / ' I \

tJ( ~ )~ [f----t~

D

Fig.2.1 Schematic representation of a central cell with all adjacent sites occupied (a) or vacant (b)

12 Chapter 2

Let's first concentrate on situation a. To a reasonable approximation (the

Einstein or Griineisen approximation) we can picture the central molecule

wandering in that force field which would be present if all the neighbouring

species were at their equilibrium cell positions (see fig.2.2).

Fig.2.2 Schematic representation of a central cell with all neigbouring species at their equilibrium

cell position

When the central wanderer is at position r relative to the centre or origin 0 of

the cell, it has a relative potential energy E(r)-E(O). So now the partition

function for a N molecules system reads :

{ _ E(O) )f (_ E(r1 ..... N) -E(O) ) exp \ kT exp\ kT

(2.6)

with the integral defined as the cell partition function or cell free volume vr.

The potential energy E(r) consists of all individual pair interactions between the

Theoretical considerations 13

central particle and its neighbours. All these species can be regarded as being

point-centres. When the interaction is purely dispersive, i.e. no specific

interactions occur, this pair interaction can be represented by a 6-12 Lennard

lones potential :

t(r) = t* [ (v* fwt- 2(v* fw)2] = t* [ (r* /r)12

- 2(r* /rt] (2.7)

with t * and v* the energy and volume belonging to the minimum in the

Lennard-lones curve (see fig.23), w the cell volume, defined by w = yV /N, and

r* and r the one-dimensional analogues of v* and w.

The cell free volume is determined by the motion of the central segment in its

cell. The wanderer is restricted to move around in its cell in the potential field

of the neighbouring segments. This cell potential field is a complicated function

of the location of the neighbouring segments and the exact intermolecular

potential law. For the Lennard-Jones potential the cell free volume can be

studied exactly. However to simplify the mathematics involved in the expression

1.5 ....-------.....-----------.

1.0

0.5

• ~ 0.0 t---~---rv-----===-1

-0.5

-1.0 -1.5 ...._ ___ ...._ ___ ........ ___ ........ ___ __..

0.0 0.5 1.0 1.5 2.0

Fig.2.3 Scaled Leonard-Jones interaction potential

14 Chapter 2

for the cell partition function, one does not adhere to the exact Lennard - Jones

relation but it is approximated by a square well. Consequently the cell is

simplified to a cage with a constant cell potential which becomes infinite at the

cell wall at a distance 2·1/6 r•. The situation is sketched below.

Flg.2.4 Schematic representation of the central cell free volume with all adjacent sites occupied

The partition function for the above sketched system of N molecules reads :

1 ( E(O)) z = exp - ~ J dr1 •• drN tr .fNN! sphere

1 [wl/3 _ 2·1/6 v•t/3] 3 (2.8) ).3NN!

In the other extreme, with all adjacent cells vacant, the wanderer is not restricted

in its movement by neighbour elements and can move over the entire cell.

Because of the lack of interaction the cell potential energy is independent of the

position in the cell. This situation is sketched in fig.2.5.

Theoretical considerations 15

D D

Fig.Z5 Schematic representation of the central cell free volume with all adjacent sites vacant

In this case the partition function becomes:

exp (- EkT(O) ~ I

2 dr1 .. drN cell

(2.9)

In a fluid system, the situation will be somewhere between the two extremes.

The main problem one faces for the moment is the evaluation of the effective

free volume accessible to the wanderer. It is a somewhat arbitrary manoeuvre

but one can introduce the linear average for the free lengths (one-dimensional

free volume) over the occupied fraction y. This procedure leads to the following

expression for the cell partition function or cell free volume vr:

(2.10)

16 Chapter 2

In reduced quantities the cell partition function reads :

(2.11)

with w = w/v*.

Assuming that the molecules are independent the partition function reads:

The factor g represents the statistical number of arrangements related to the

permutations of vacant and filled cells. Simple combinatorics states:

g = N!/[(yN)! ((1-y)N)!] (2.13)

The energy for the system at rest Eo is related to the total number of pair

contacts in the system and the energy belonging to such a contact :

Eo = ~Nz £* [ A(v* f'wt- 2B(v* /w)2] (2.14)

Due to the long-range character of the interaction potential, the contribution

of interactions between non-nearest neighbours is not negligible. In particular,

the attractive energy constant·B in eq. 2.14 is significantly greater than unity.

Unfortunately, the exact contributions of these non-nearest neighbour

interactions depend on the specific lattice used. Following Simha and Somcynsky

[20] the values A= 1.011 and B = 1.2049 are used valid for a face-centered cubic

lattice [46].

So far the partition function for a low molar mass component has been

established and for each term in this function a detailled expression has been

presented. In the next section a generalization will be made to polymers.

Theoretical considerations 17

2.4 Simha-Somcynsky theory for polymers

The derivation of the partition function for polymers closely parallels the

procedure given for low molar mass components. For the latter it was assumed

that one molecule occupies one cell. A polymer however is considered as an

open chain consisting of s segments. This s-mer may be treated as a set of s

point-centres each subjected to the external forces exerted by the neighbouring

segments at their rest positions. The mean distance between neighbouring point

centres is considered approximately the same whether they belong to the same

molecule or not. The basic problem is now to obtain an explicit form for the cell

partition function. Each s-mer contains contributions from inter- and

intramolecular forces. Because intermolecular forces are of a different order of

magnitude compared to the intramolecular, it is possible to separate the total of

3s degrees of freedom of a molecule in the internal and external degrees of

freedom which respectively depend on intramolecular valency and intermolecular

forces. Only these external degrees of freedom contribute to the translational

partition function. When the total number of external degrees of freedom per

molecule equals 3c, there are 3(s-c) internal degrees present. As Prigogine

showed [1], the partition function for this system can be approximated as :

with t and 1/1 the reduced cell partition functions per three external and internal

degrees of freedom respectively. The term l/1(s-<)N />.3(><)N does not contribute to

the compositional derivatives of the translational partition function because only

intramolecular forces are involved in this term. So one obtains:

(2.16)

with (2.17)

Bearing in mind the connectivity of a molecular chain, the total number of

18 Chapter 2

external contacts per molecule equals y(s(z-2)+2). For the total energy of the

system at rest one obtains:

E0 = lhyN (s(z-2)+2) £* [ A(v* fwt- 2B(v* fw)2] (2.18)

with z the coordination number and with the segmental cell volume defined by

w=yV/Ns. (2.19)

The combinatorial term has to be altered because the statistics for a sys,tem

containing s-mers and holes is far more complex than for the s = 1 case. Flory

[47] estimated the number of arrangements for this complex case by placing the

segments sequentially on a lattice. The possibility of placing a segment at a given

lattice site is determined by the probability that this particular lattice site is

vacant. This probability is related to the occupied site fraction y. This method

leads to the following ultimate expression for g:

g = 2-N NN Nh·Nh [(z-1)/e](s-t)Nh (sN + Nh)(N+Nh} y-<N+Nh} (1·y)-<t-y)(sN+Nb)/y

(2.20)

with Nh the number of vacant cells.

2.5 A modified hole theory for polymers and low molar mass fluids

In the suggested modification , the Simha-Somcynsky structure parameter y, i.e.

the fraction of occupied sites is replaced by a more appropriate structure

parameter, i.e. the external contact fraction q. This fraction is a measure for the

number of intermolecular contacts a system of s-mers can make. This alteration

has consequences for the combinatorial factor, the cell partition function and for

the expression for Eo which are discussed in the following. The Flory expression

is replaced by the Huggins expression in the combinatorial part of the partition

Theoretical considerations 19

function. In deriving the combinatorial factor g Huggins [6,48,49] used the

scheme similar to that of Flory. The fundamental difference however lies in the

definition of the probability tliat a lattice site is vacant. Whereas Flory relates

this probability to the occupied fraction y, according to Huggins it is identified

with the contact fraction q defined by

q = N[s(z-2)+2)] / [N[s(z-2)+2] + zNh] (2.21)

The contact fraction and the site fraction y are interrelated by :

q = (1-c:t)y/(1-ay) (2.22)

where a = -y(1-1/s) and 1 = 2/z.

The Huggins procedure adds one extra term to the original Flory expression for

g :

g(Huggins) = g(Flory) * (1-ay)<t-ay)/1Y (2.23)

and gives a significant improvement as indicated by Monte-Carlo simulations on

lattices [50-53] and by the description of experimental data [54]. This is the

main motivation for the introduction of this refined entropy expression into the

Simha-Somcynsky hole theory.

Furthermore in the expression for E0 the site fraction y is replaced by the

contact fraction q :

Eo= 1/2q_N (s(z-2)+2) £* [ A(v*/wt- 2B(v*/w)2] (2.24)

This substitution is also adopted in the averaging procedure of the free length

in the cell partition function. Instead of averaging over y one averages over q,

so the reduced cell partition function becomes :

(2.25)

20 Chapter 2

This modified version is referred to in literature as the Holes and Huggins or

Holey Huggins theory [30]. In the low molar mass case (s= 1), this Holes and

Huggins version reduces to the original Simha-Somcynsky formulation, see

relation 2.22. With the introduction of these modifications it is hoped that a

more consistent description of thermodynamic properties is obtained. In the

following chapters the predictive and descriptive power of both theories is tested

by confronting them with equilibrium thermodynamic properties of real systems.

2.6 Basic thermodynamic equations

2.6.1 Equation of state

The partition function opens the way for the determination of the equilibrium

properties one is interested in. In order to evaluate these properties for a N

molecules system basically seven parameters have to be quantified first:£*, v*,

s, c, z, y and the volume V with the relevant parameters expressed per mole

segments. The coordination number z is set equal to 12. To solve y and V as a

function of the pressure p and temperature T the equation of state and the

minimization condition serve. The latter condition is a reflection of the tendency

of the system to obtain a minimum free energy defining the equilibrium value

ofy:

(of/(Jy)N,V,T = (olnZ/(Jy)N,V,T = 0 (2.26)

The equation of state reads:

p = -(8F/8V)N,T = -(8F/8V)N,T,y + (8F/fJy)N,T,v(8y/8V)N,T (2.27)

and becomes: p = -(oF/8V)N,T,y (2.28)

The equation of state is expressed in reduced macroscopic quantities V,

Theoretical considerations 21

f and p. These are related to the microscopic variables as follows :

V = V /V* = V /(Nsv*) (2.29)

f = T/T* = cRT/((s(z-2)+2) t*) (2.30)

p = p/p* = psv*/((s(z-2)+2) t*) (2.31)

The expressions for the minimization condition and the equation of state in

reduced form now become :

(s/c) [(s-1)/s + In (1-y)/y -In (1-ay)/('YY) -<k/1] = (317-l+ay)/((1-q)(l-ay)) +

(2.32)

(1-a)y [2B(yV}-2-3A(yV)4 +4ay(A(yV)"''-B(yV)"2)]/(2T(l-ay)2)

and

PY7T = (1-q)-1 + 2(1-a)y (yVf2 [A(yVf2 -B]/((1-ay)T) (2.33)

with 11 = 2-116 (1-<k)Y (yVf1'3 /(1-ay) (2.34)

These relations reduce to the expressions obtained in the Simha-Somcynsky

theory if a equals zero or s equals one.

There are two alternative routes for the determination of the molecular

parameters t*, v*, s and c. In the original Simha-Somcynsky theory [20] c is

related to s through the so called semi-flexibility rule 3c = s + 3. This relation

was first derived by Prigogine [1] for semi-flexible chain molecules. In this case

the parameters are determined by fitting experimental equilibrium equation of

state data to the equations 2.32 and 2.33. An alternative approach is to link s to

the molecular structure. The parameter s can be chosen at forehand in such a

way that one monomer repeat unit in a polymer molecule occupies exactly one

cell site. The three molecular parameters left are again determined by a fit of

experimental equation of state data. This latter procedure is used henceforth

unless otherwise stated.

22 Chapter 2

2.6.2 Helmholtz free enelliY

The Helmholtz free energy per mole of occupied lattice sites is given by:

A/(NsRT) = lny/s + (1-y)ln(1-y)/y -(1-ay)ln(1-ay)/('YY)

(2.35)

with Nathe number of Avogadro. Some volume independent contributions (eq

2.20) to the combinatorial entropy have been omitted in the expression for the

Helmholtz free energy because one is only interested in a relative rather than

an absolute value of the Helmholtz free energy. Standard equilibrium

thermodynamics links all other thermodynamic properties to this Helmholtz free

energy.

2. 7 Generalization for multicomponent systems

This paragraph is devoted to the description of multicomponent systems within

the framework of the presented theories. The approach that is taken relies on

the principle of corresponding states which is a useful guide in the estimation of

the density of fluid systems. In the present context it can be formulated that all

substances obey the same equation of state in terms of reduced variables. These

variables can be expressed in terms of critical constants or in terms of molecular

parameters, e.g. f.*, v*, s and c. The molecular parameters of a mixture partly

depend on the molecular parameters of the pure components. A composition

dependent averaging procedure may be introduced which is separately applied

to each kind of segment in the system. One can even go a step further and take

an average over all kinds of pairs in the system. This process is illustrated by

Theoretical considerations 23

focussing for the moment on one segment in a two-component system. The

wanderer can be either a component A or B segment. This wanderer feels a

force field in which A-A and A-B or B-A and B-B interactions play a role. This

field can be replaced by some kind of average force field depending on the

fractions of the constituents A and B. Consequently this composition dependent

fluctuations are neglected which is reasonable, provided the pair interactions in

the system are not too different. So the average interaction energy for a pair of

segments at a distance r in the mixture may be written as [26,29]:

(2.36)

with XA the site fraction of component A defined by :

(2.37)

The energy contributions can be expressed in terms of Lennard-lones potentials

leading to:

(2.38)

From these two relations <£*> and <v*> are deduced:

[ X 2 £ * v *2 + 2X X c. * v *2 + X 2 c. * v *2 ]2

AAAAA ABABAB BBBBB <£*> = (2.40)

24 Chapter l

The cross interaction parameters £ AB * and r AB * can be expressed as a function

of the average of the pure component parameters :

£ , _ X (c. , £ *)1/2 AB - AA BB

When X and Y equal unity, the interaction are purely dispersive.

The other molecular parameters s and c are defined as follows :

with the segment fraction defined by

(2.42)

(2.43)

(2.44)

(2.45)

(2.46)

Based on corresponding state arguments the average molecular mass per

segment M0 is averaged as well and becomes [26]:

The macroscopic scaling parameters <p*>, <V*> and <T*> become

composition dependent by the introduction of the averaged microscopic

parameters in eq. 2.29-2.31. The combinatorial part of the partition function will

become more complex for multicomponent systems because a statistical mixing

process takes place between more than one component and vacancies. Because

only purely dispersive interactions are accounted for in the theory without any

specific interactions, this mixing process is assumed to be completely random.

For a two component system the total number of arrangements is increased by

a factor !fJA/sA ln~pA + ~psfs8 ln~p8 .

Theoretical considerations 25

2.8 Basic thermodynamic equation for multi-component systems

The scaled working equations for a mixture and for a single component fluid

are formally identical. The main difference. ,however is the introduction of the

composition averages for the molecular parameters in these working equations.

Apart from this difference the equation of state and the minimization condition

( eq.2.34 and 2.35) do not change. In the expression for the Helmholtz free

energy an extra term appears from the mixing of more than one component. For

a binary mixture this energy per mole of segments becomes :

Aro/(N<s>RT) = I()AjsA lni()A + l()a/sa lnl()a + (1-y)/y ln(1-y)

+ In (y)/ <s> -(1-<a>y)/(1'1) ln(1-<a>y)

- <c.> In (v* yV (1-17)3)

+ (1-a)y <c.> [A(yV)4 -2B(yV)"2]/(2(1-ay)T)

+ 3/2 <c5 > In (211'<M0 >RT/(N8h)2) (2.48)

The volume V and the occupied fraction y of the mixture are quantified as a

function of p and T by simultaneously solving the minimization condition and the

equation of state for the mixture.

In paragraph 2.6 it is shown that basically seven parameters characterise a one

component fluid uniquely within the framework of the theory. In the description

of a two-component system two additional parameters are introduced, i.e. f. AB *

and v AB *. Whereas the pure component parameters are estimated by fitting

experimental equilibrium equation of state data, the two mixing parameters are

evaluated from the fit of an experimental critical point as will be shown in the

next section. This is one of the procedures that is available to fit the mixing

parameters and will be used as a standard procedure throughout this thesis.

26 Chapter 2

2.9 Phase behaviour

Generally, in the pressure-temperature-composition space of a binary system

a two-phase region or miscibility gap exists bounded by the binodal condition.

This condition requires equality of the chemical potentials of the constituents in

the two phases. The miscibility gap is subdivided in a metastable and. unstable

region by the spinodal condition :

(2.49)

with the Gibbs free energy of mixing :

with Gm the Gibbs free energy of the mixture. In the stable and metastable

regions Jsp is positive whereas in the unstable region this derivative is negative.

Binodal and spinodal coincide at the critical state which is situated at the top of

both curves for a strictly binary system. Here in addition the critical condition

has to be fulfilled :

(2.51)

The critical state (fPc.., Tc,) at atmospheric pressure serves to fit the mixing

parameters £AB * and v AB *.

In first instance Jain and Simha [29] approximated the theoretical values of

AGm by fourth order polynomials in the concentration. This facilitates to a great

extend the differentiation procedure necessary to evaluate phase behaviour.

Because second and third derivatives are involved, it is clear that small errors

in the estimation of AGm may lead to considerable errors in the computation of

phase behaviour. At a later stage the mathematical exact first and second

derivatives of AGm were derived in order to avoid these possible errors. The

Theoretical considerations 27

minimization condition, the equation of state and the Gibbs free energy of

mixing are complex functions of the principle variables "B> y, p, T and V. To

make the derivatives, which are functions of the principle variables manageable,

some extra auxiliary variables are introduced. The working equations are

functions of these auxiliary variables, viz. :

the Helmholtz free energyA/(N<s>R1)=A(~pA>y,T,Q,n,<s>,<c>,<Mo>,<v"' >)

the equation of state : EOS = EOS(y,T,Q,71,<s>,<c>)

and the minimization procedure : MICO = MICO(y,T,Q,I'J, < s >, < c >)

where EOS and MICO represent eq. 2.32 and 2.33 in the multicomponent form

implicitly. The compositional derivatives, which determine the phase behaviour,

can be expressed in terms of the auxiliary variables [31]. For the first derivative

of a function E, e.g. one of the three above given functions, one obtains :

with Ii one of the n1 auxiliary variables.

The second derivative reads:

(:~J p,T (2.52)

(ai.) (a1. ) aq~~ p,T ~ p,T

(2.53)

The derivatives for the thermodynamic functions with respect to the auxiliary

variables are summarized in [31] together with the compositional derivatives of

these variables. Appropriate combination of the expressions produces the desired

thermodynamic properties, e.g. chemical potentials and spinodals. The third

28 Chapter 2

compositional derivative, which determines the critical state, was not derived

analytically but was computed numerically starting from the analytically derived

second derivative. As stated before, y and V are determined by solving the

equation of state and the minimization condition simultaneously. The first and

second derivatives of y and V are determined by solving the set of equations

formed by the first and second derivative of the equation of state and

minimization condition. Once y,V and the derivatives have been obtained, all

tabulated expressions and consequently thermodynamic properties can be

computed in a straightforward way.

Chapter 4 is devoted partly to differences in AGm that occur when either the

analytical or the approximate method is used for the computation of AGm for a

polymer/solvent system. The consequences for the computed phase behaviour

are discussed as well.

2.10 Analogy with other equation of state theories

A unique feature of the Simha-Somcynsky theory and the Holes and Huggins

theory is the way the free volume is treated. First of all the total free volume is

obtained from the free lattice sites and cell free volume contributions.

Furthermore the division of the cell free volume in a solid-like and a gas-like

part sets these theories clearly apart from the other existing equation of state

models. These other models are discussed below because computations have

been performed also with other equation of state theories and to elucidate the

position of the Simha-Somcynsky and the Holey Huggins theories amongst these

other theories.

These other models can be divided into two classes. The first class is formed

by the cell models in which vacant cell sites are not admitted. The free volume

exclusively originates from the free space available to each wanderer in its

individual cell. Representative for this approach are Prigogine's cell model [1],

the Flory, Orwoll, Vrij theory [2-5], Pattersons approach [55-59], the modified

version of the cell model by Walsh and Dee [10,11] and the recent approach of

Theoretical considerations 29

Kammer et al [12].

The second class is formed by the vacancy models. The wanderer are froozen

in at their equilibrium positions and free volume is determined by vacant cells ·

only. Examples are the theories of Sanchez and Lacombe (13-15], Koningsveld

and Kleintjens [17-19] and the approach of Panayiotou and Vera [16].

In the next section these models are discussed briefly and especially the

Flory-Orwoll-Vrij theory and the model of Sanchez-Lacombe are examined

more extensively. The reason for this is that computations on real systems have

been performed also with these two theories. This opens the possibility to

compare the different models not only on a pure theoretical level but also to test

their power in describing and predicting thermodynamic properties of real

systems.

2.11 Cell models

If no allowance is made for vacant cells, i.e. y = 1, the Sirnha-Somcynsky theory

boils down to the crude version of the smoothed potential cell model as defined

by Prigogine [1]. Walsh and Dee [10] adapted this potential cell model for pure

components. Their aim was to obtain a better equation of state description for

pure polymers at equilibrium conditions. An extra fit parameter was added to

the cell partition function which can be seen as a correction for the hard core

volume:

(2.54)

The value for q corresponds to an increase of the hard-core volume of

approximately 25% in comparison with the original cell model. Although one has

to recognize there is no solid theoretical basis for the introduction of this fit

parameter the equation of state description of homopolymers is enhanced.

30 Chapter 2

Recently Kammer [12] modified the cell theory of Prigogine [1] for the

description of miscibility behaviour of copolymer systems. The square well

approximation, leading to an explicit expression of the cell partition function, is

not used in this approach. Instead the cell partition function is expressed in

terms of properties of the pure components. An expansion is applied in powers

of reduced pressure and reduced reciprocal temperature. The cell theory that has

found wide application in the field of polymer physics, is the theory of Flory,

Orwoll and Vrij [2-5]. It is compared in this thesis with the SS and HH theory

in its capability to describe the phase behaviour of the polymer solution

polystyrene/ cyclohexane.

2.12 The Flory-Orwoll-Vrij theory

A theory that bas found wide application is the Flory-Orwoll-Vrij [2-5] theory.

The reason for this is its relative mathematical simplicity combined with its

capability of successfully describing physical properties. The most important

distinctions between this theory and the Simha-Somcynsky model are

summarized below.

1. The equilibrium energy is assumed to be of a van der Waals form instead of

a Leonard-Jones type :

Eo - Cfw (2.55)

with C a constant.

2. The term 2-116 in the cell partition function vanishes because this term is

derived from the Leonard-Jones potential energy equation. The occupied fraction

y equals unity so the cell partition function reads :

(2.56)

Theoretical considerations 31

3. The hard core volumes v* are chosen in such a way that they are equal for

all components in a mixture.

4. A surface area per segment ri is introduced. For a binary system the fraction

of the total surface area for molecules of type A becomes :

(2.57)

5. Averaging rules are not defined for microscopic parameters but instead for the

scaling parameters p* and T*. For a binary system the mixing rules are

introduced :

(2.58)

(2.60)

(2.61)

with XAB the Flory-Huggins imeraction parameter defined by :

(2.62)

with ApA the chemical potential difference between solution and pure A

The translational partition function for a mixture reads :

(2.63)

with the equation of state :

32 Chapter 2

(2.64)

withp = pj<p*>, T = T/<T*> and V = V/(Nsv*) (2.65)

To e~timate the pure component parameters in the Flory-Orwoll-Vrij theory, it

is not common to fit a whole pVT-surface. Mostly a one-point fit is used. This

means knowledge of a single molar volume at a given temperature and

atmospheric pressure together with the corresponding thermal pressure and

thermal expansion coefficient is sufficient to quantify these parameters.

From the equation of state one derives at zero pressure :

(2.66)

(2.67)

(2.68)

with the thermal pressure coefficient 1 = (1Jp/8T)v and the thermal expansion

coefficient a = (alnV /8T)p. In the Flory-Orwoll-Vrij ~eory it is a prerequisite

that the hard core molar volumes vi* (expressed in m3 /mole) are equal. By

adjusting the molar mass per segment of the pure components this condition can

be fulfilled. The number of external degrees of freedom for a pure component

follows from :

(2.69)

and the surface area per segment :

r. = 2p. * v. *2/C I I I (2.70)

The interaction parameter XAB and cAB are determined from miscibility

behaviour.

Theoretical considerations 33

2.13 The Sanchez-Lacombe model

The vacancy models form a second class of equation of state models. An

example of this type is the Sanchez-Lacombe theory [13-15]. In this model the

segments are frozen in at the equilibrium positions on their respective cells and

have consequently no free volume in the cell to move over. In contrast to the

cell models, this means the Boltzmann factor in the partition function is not split

up in a rest term containing Eo and a cell partition term reflecting the deviation

from this value at rest. In the Sanchez-Lacombe theory the configurational

partition function for a pure component is defined by :

Acont = f f g exp [-(E+pV)/kT] dV dE (2.71) VE

with E the internal energy of the system. Please note this partition function is

defined in such a way that it leads directly to the Gibbs free energy G. In the

lattice formulation with the fraction of occupied sites f = s~/(s~ + Nh) the

total number of configurations of the system becomes approximately :

(2.72)

This is analoguous to the combinatorics applied in the Simha-Somcynsky theory.

H random mixing is assumed, the chance that two adjacent sites are occupied

equals e. Denoting the corresponding interaction energy between these sites £,

the total intermolecular energy is :

(2.73)

A typical feature of the Sanchez-Lacombe theory is the fact that the number of

segments attributed to a polymer molecule in the pure component state may

change in the mixture. Just as in the Flory-Orwoll-Vrij theory it is a prerequisite

34 Chapter 2

that the hard core volumes v* for segments of different components are equal

in the mixture. In the following a binary mixture is considered. If a type i

molecule occupies s;0 sites in the pure state, it occupies s; sites in the mixture,

where

s. = s.0 v.*f<v* > I I I (2.74)

with the hard core volume averaged over the volume fraction :

<v* > - '" <lv * + '" 0v • - TA A TB B (2.75)

where (2.76)

The average chain length < s > follows straightforwardly from :

(2.TI)

The total number of configurations for a binary system is approximately given

by:

with fo = N0/(N0+sANA +s8Ns), fA = sANAf(N0+sANA +s8N8) and

fB = 1-fA-fo (2.79)

If random mixing is assumed, the intermolecular energy becomes :

(2.80)

(2.81)

(2.82)

Theoretical considerations

The volume fraction A in the mixture is defined by :

The equation of state for the mixture now becomes :

1/1J2 + p + T[ln(1-1/V) + (1-1/<s>)1/V] = o

with the reduced equation of state parameters :

V = V/<V*> = V/(Ns<v*>)

T = T/<T*> = kT/<E:*>

p = p/<p*> = p<V*>/<r.*>

The Gibbs free energy for the mixture now becomes :

(2.83)

(2.84)

(2.85)

(2.86)

(2.87)

35

G/(<s>N<r.*>) = -1/V + pV + T[(V-1)1n(1-1/V)-1/<s> lnV (2.88)

36 Chapter 2

Equation of State Behaviour of Pure Components 37

3. Equation of State Behaviour of Pure Components

3.1 Introduction

In chapter 2 some statistical mechanical models have been presented for low

molar mass systems as well as for polymers. In each model particular

suppositions were made characterizing the model. In this chapter the molecular

parameters of the pure components are presented for these models. These

parameters are quantified by confronting the theoretical equations of state with

equilibrium equation of state data for various components. The quality of the fit

a certain model gives, is taken as an indication for the adequacy of the

approximations involved in this model. In this chapter only pure component

parameters are presented. So the appropriateness of the mixing rules involved

in the different models is not discussed. The SS and HH model are compared

with the Sanchez-Lacombe theory [13-15], the Flory-Orwoll-Vrij theory [2-5] and

Prigogine's cell model [1]. The results of Dee and Walsh [10,11] will serve to

make this comparison. Furthermore the differences between the SS and the HH

theory are discussed as well.

3.2 Comparison of equation of state models ; a literature survey

In fitting dilatometric data to the theoretical equation of state only

equilibrium data in the fluid phase or melt state are of interest. This is because

in the derivation of these equations the fluid phase is considered to be in

equilibrium. Under these conditions the specific volume is a function of the state

variables only. For polymers equilibrium can be maintained in the melt and

solution states. The glassy state however is a non-equilibrium state, i.e. the

38 Chapter 3

specific volume depends also on formation history parameters such as the rate

the glass was formed or the pressure during the formation. For the present

purposes only equation of state data in the molten state are considered.

Zoller [60] and Dee and Walsh [10,11] have investigated extensively pVT

data' of the most common polymers in the melt and analysed these data in the

framework of the various equation of state theories. These authors compared the

Sanchez-Lacombe (SL) theory, the Flory-Orwoll-Vrij (FOV) theory, Prigogines

cell model (CM), Walsh's and Dee's modified version of the cell model (MCM)

and the Simha-Somcynsky theory in the ability to fit p VT-data of polymers. Both

authors concluded that the Simha-Somcynsky theory gives one of the best

representations of the data over an extended range of pressures and

temperatures with deviations usually smaller than 0.003 cm3 fg for pressures up

to 200 MPa and temperatures as large as 250 oc. The results of Walsh serve to

illustrate this, see table 3.1. Equilibrium pVT-data of polyethylene (PE),

polystyrene (PS), polydimethylsiloxane (PDMS) and poly(hydroxypropyl)ether of

bisphenol A (PO) were fitted, applying the equations of state of the various

theories. A non-linear least squares fit was used, minimizing the value of s2, with

(3.1)

with the summation performed over all data-points, with N the number of data

points, Pi,exp is the measured pressure at a specified volume and temperature

and Pi,theory is the value of the pressure predicted by the relevant equation of

state for the i'th data point. The modified cell model gives numerically the best

fit although one has to take into account that one additional adjustable

parameter is introduced to achieve this (see also chapter 2). When one compares

the results of the Simha-Somcynsky theory with the cell-model, only a slight

improvement in pVT-description is observed. This does not imply however that

thermal expansion and compressibility properties can be mainly described by

changes in cell free volume in the Simha-Somcynsky theory. In paragraph 3.3 it

will be elucidated that the number of vacancies varies significantly with changing

temperature and pressure. Its impact on the total equation of state behaviour is

Equation of State Behaviour of Pure Components 39

quantitatively larger than the change in the cell volume upon a temperature or

pressure change. The use of solely changes in the number of vacancies in the

case of the Sanchez-Lacombe theory, gives a less satisfactory fit comparable to ·

the other presented models.

Table 3.1 s2 of pVf-fits for polyethylene (PE), polystyrene (PS), poly(dimethylsiloxane) and poly

(bydroxypropyl)ether of bispbenol A (PO) according to the indicated models

P-range (bar)

T-range (K)

SL

FOV

CM

ss MCM

PE

0-2000

425-535

16.97

9.25

1.942

1.49

0.85

PS

0-1800

395-595

30.6

11.1

1.64

0.975

0.51

PDMS

0-2000

300-510

102.2

42.6

5.66

4.67

4.71

PO

0-1800

360-575

36.06

10.89

3.15

1.1

0.89

3.3 Comparison Simha-Somcynsky I Holes-Huggins model

3.3.1 Universal pVT surface

In this section the ability of the original Simha-Somcynsky theory and the

Holes-Huggins theory to describe pVT-characteristics is compared [30]. One can

compare the theories on a general basis with the relations expressed in reduced

variables for an imaginary molar mass (s value has to be specified)

independently of any actual system. In fig.3.1 reduced isotherms are presented

40 Chapter 3

l> 1.08 4)

i > 1.03 "0

3 ~ "0

.! 0.98

0.93 0.00 0.05 0.10 0.15 0.20

N

Reduced Pressure P

Flg.J.l Reduced volume versus reduced pressure at indicated reduced temperatures according to

SS (- - -) and HH (--) theories

1.00 ... T•0.021

0.96 )\

c 0 ;:: 0 • 0.92 .. 1&.

4) -en 0.88

0.84 0.00 0.05 0.10 0.15 0.20

Reduced Pressure P

Fig.J.Z Occupied site fraction y versus reduced pressure at indicated reduced temperatures

according to the SS (- • ·) and HH (--) theories

Equation of State Behaviour of Pure Components 41

0.97 ....-----------.,

I 0.96

0.96

I P•O.tO

0.94

---------------0.98 L..-________ __._ __ ___,

0.026 0.036 0.046 0.066

"' Reduced Temperature T

F'la-3.3 Reduced ceO volume versus reduced temperature at indicated reduced pressures according

to SS (- - -) and HH (--) theories

for the SS and the HH theories. At higher reduced temperatures differences

between the theories emerge. Clearly, the theories have different universal pVT

surfaces. In fig.3.2 it is observed that the parameter y in the same p VT interval

is substantially larger for the SS theory; i.e. a denser structure is predicted. The

reduced cell volume as a function of temperature and pressure is almost

identical in both theories, as indicated in fig.3.3. Although only slightly

dependent on temperature, the cell volume changes significantly with pressure.

At low reduced temperatures the occupied fraction y approaches unity and the

contact fraction q tends to the fraction y. Consequently both treatments can be

practically superimposed at low temperatures.

42 Chapter 3

3.3.2 Experimental data

Because differences are obseiVed for the universal pVT-surfaces, it is of

interest to see if differences are also noticeable in the description of

experimental data. As was already outlined in chapter 2, the pure component

can be modelled in different ways. Here the relative chain length is taken equal

to the degree of polymerization s = M/Mo where M is the molar mass of the

polymer and Mo the molar mass of a physical repeat unit, unless otherwise

stated. In fig.3.4 experimental pVT-data for PS are shown [24]. Differences

between the SS and the HH theories are numerically small and are not visible

in this figure. Also differences in computed thermal expansion and

compressibility coefficients are very small. Nevertheless the polymer is modelled

differently in both theories. For the sake of comparison, the molecular and

scaling parameters for some polymers are compiled in table 3.2. These were

extracted from experimental equation of state data [24,61,62] · using a

multiparameter estimation program (PEP) [63] developed at DSM, the

1.03 ,...-------------. 1

a 1.01 ..... .. e 0 -> 0.99 .., i > 0.97

~ '() .., i 0.95

0.93 380 400 420 440 460 480

Temperature T (K)

Fig.3.4 Volume -temperature behaviour at indicated pressures (bar) for polystyrene: experimental

data (24] (•) and theoretical deseription according toSS(·--) and HH (--)theories.

Equation of State Behaviour of Pure Components 43

Netherlands. For the systems considered in table 3.2 the scaling parameters p*,

V* and T* are larger for the SS than for the HH theory. Consequently, the

polymer is situated in different regions of the universal pVT-surface. The

differences in the scaling parameter values are related to differences in

molecular parameters. In the SS theory the interaction parameters E * and v* are

larger, indicating a deeper and wider potential bowl than for the HH theory. On

the other band, the flexibility parameter c, is smaller, indicating that fewer

TaWe 3.Z Molecular and scaliDg parameters acc:ording to the SS and HH theory for polystyrene

(PS), polyethylene (PE), poly(p-chlorostyrene) (PpCJS) and poly(o-methylstyrene)

(PoMeS)

Polymer t•

(J/mole)

A. SS theory

PS 6968.8 99.54

PE 3356.2 29.68

PpCJS 9981.0 108.63

PoMeS 8508.1 114.78

B. HH theory

PS 6690.9 98.46

PE 3162.9 29.62

PpCIS 9535.5 107.87

PoMeS 8181.9 113.52

,. (bar)

0.7694 7002.6

0.5508 11309.6

13361 9189.1

0.9591 7416.0

0.8531 67%.6

0.5834 10679.8

1.4356 8840.8

1.0611 7210.8

0.9572

1.0581

0.7838

0.9712

0.9468

1.0560

0.7783

0.9606

T*

(K)

10899.2

733().9

8985.8

10674.2

9438.1

6522.4

7989.7

9278.4

44 Chapter 3

degrees of freedom are volume-dependent in the SS theory. From the changes

in the molecular parameters one can anticipate a denser structure for the SS

theory compared to the HH theory which is confirmed by the computations. It

is worthwile to observe that C5 can become larger than unity, indicating that the

monomer segments are not rigid spheres but have some degrees of freedom

depending on volume. The quality of the fit of the HH theory is somewhat

better than the fit obtained with the SS theory, although numerical differences

are small.

So far we have only considered the pVT-description of individual pure

components and their molecular- and scaling parameters. The final goal however

is to describe and predict equilibrium thermodynamic properties of mixtures. In

order to do this these pure component parameters are essential, together with

the two mixing parameters hi the computation of the average segmental energy

< E * > and volume < v* > for which the mixing rules 2.40 and 2.41 serve. These

mixing rules may only be applied when the hard core volumes differ not too

much as Prigogine pointed out [1]. He estimated a tolerable difference in v* of

approximately 10%. Of course this is only a guide-line because it is impossible

to give an absolute limit. This limit for the difference in hard core volumes may

pose a problem for a polymer blend for which the hard-core volumes of the

monomer repeat units are very different. The same problem might arise in the

case of a polymer solution when the molar volume of the solvent is again

different compared to the polymer repeat unit volume. In these cases one of the

two pure component descriptions has to be adapted in such a way that the

molecular parameters come closer, i.e. one of the segment sizes has to be

increased or decreased. How does this change affect the quality of the pVT·

description? To answer this question pVT-data of PS are fitted making use of

the HH theory while changing the segmental size. In fig.3.5 results are displayed

of a pVT-fit of PS-data obtained from Quach and Simha [24]. The fit was

performed using PEP. The segment size of PS was varied around the size of a

monomer repeat unit and the quality of each fit was expressed in s2, defined by

Equation or State Behaviour or Pure Components 45

where the summation is performed over the data points and where the standard

deviations are set to aP = 0.5%, av = 0.04% and aT= O.lK respectively. In this

fit 28 datapoints were used over an extended temperature and pressure regime.

s2 is only slightly dependent on the chosen value for the segmental molar mass.

So for the quality of the pVT-fit it does not really matter what segmental molar

mass is chosen. As shown in fig. 3.6a, b and c the scaling parameters E *, v* and

C5 are linear functions of the segmental molar mass .

.to ..------------.

35

... .so t~-----------, -21

2 0 ....___._ _ _.______. _ _,__.______.

70 80 90 100110120130

Segm. molar maas (g/mol)

Flg.3.5 Quality of the pVT-fit, expressed in the parameter s2, for PS (24] as a function of the PS

segmental molar mass

46 Chapter 3

10 15 - a b 0 .... 0

9 E E ..... 13 ..... ., . - .§

8 11

7

9 6

5 7

.. 5 70 80 9 0 1 00 11 0 1 2 0 13 0 70 80 90100110120130

Segm. molar mass (g/mol) Segm. molar mass (g/mol)

·1.20 r-------------, c

1.00

0.60

0.40 ~...-_.__ ......... _.___.____,........_____.

70 80 90 100110120130

Segm. molar mass (g/mol)

Fig.3.6 The molecular parameters C.* (a), v* (b) and c, (c) for PS as a function of the segmental

molar mass

Equation of State Behaviour of Pure Components 47

3.4 Molecular parameters for studied systems according to SS and

HH theories

In table 3.3-3.7 molecular parameters are displayed for the components that are

studied in this thesis. The references, where the equation of state data are taken

from, are displayed for each system. Pure component parameters for the system

PS/CH in the framework of the Flory-Orwoll-Vrij and the Sanchez-Lacombe

theories are included as well.

Table 3.3 Molar mass and molecular parameters according to the SS-theory for PE [21,61] and CH

[64]. The semi-flexibility rule 3c=s+3 was used.

Sample

CH

PE

E*(J/mole)

2932.5

2737.4

4.9050*10..5

3.2924*10'5

M,(kg/mole)

0.0344

0.0317

Table 3.4 Molecular parameters for PS [24] and CH [65] according to the SS and HH theories

Sample E*(J/mole) v*(m3/mole) cs M,(kgfmole)

PS

ss 6968.8 9.8538*10.5 0.76939 0.104

HH 6690.9 9.8464*1(T5 0.85312 0.104

CH 6543.4 9.3596*10..S 1.8 0.084

48 Chapter 3

Table 3.5 Molecular parameters for PS [24] and MeAc [66] according to the HH theory

s;Wple E*(J/mole) v*(m3 /mole) cs Mo(kg/mole)

MeAc 5243.3 6.6813*10"5 1.5480 0.074

PS 6690.9 9.8464*10"5 0.85312 0.104

5545.5 8.1539*10-s 0.68805 0.086

Table 3.6 Molecular parameters for model blend according to the SS and HH theories, the semi

flexibility rule 3c = s + 3 is used

Component

A

B

E*(J/mole)

3500

4000

v*(m3 /mole) Mo(kg/mole)

5*10"' 0.050

5*10-S 0.050

Table 3.7 Molecular parameters for PS [24] and PpMeS [67] according to tbe HH theory

Sample

PS

PpMeS

E*(J/mole)

6690.9

7114.7

v*(m3/mole) cs

9.8464*10"5 0.85312

9.8422*10-5 0.89964

Mo(kg/mole)

0.104

0.1005

Equation of State Behaviour of Pure Components

Table 3.8 Molecular parameters for PS and CH according to the Sanchez-Lacombe theory

Sample

PS

CH

f*(J/mole)

6110.1)6

4125.66

Mo(kgfmole)

0.0191

0.0097

Table 3.9 Characteristic parameters at 298 K for PS and CH according to the FOV theory

Sample

PS

CH

a (1/K)

5.72*1!r

1.217*10"3

"( (N/(m~))

1.381*1~

1.067*10-3

49

50 Chapter 3

3.5 Conclusions

In this chapter the SS theory is compared with the Sanchez-Lacombe theory,

the Flory-Orwoll-Vrij theory and with the conventional and a modified version

of the cell model in their ability to describe equation of state behaviour of some

common polymers under equilibrium conditions.

The modified cell model (MCM) gives numerically the best fit although one

has to recognize that one additional parameter is introduced to improve the

description.

Amongst the other theories, the SS theory generates superior pVT-fits with a

minimum of independent adjustable parameters. This is an indication for the

validity of the approximations involved in this model.

The HH theory produces a somewhat better quantitative descriptions of

equilibrium equation of state behaviour of polymers in comparison with the SS.

theory. Differences are noticeable if one considers a real polymer system. The

HH theory suggests a less dense structure, i.e. a larger fraction of holes on the

lattice. This is realized by a slightly shallower bowl of the interaction potential.

However, the most important factor responsible for the introduction of extra

holes is the increased number of external degrees of freedom.

51

Polymer Solution Section

52

Computation of Phase Equilibria 53

4. Computation of Phase Equilibria : Comparison of·

Approximate and Exact Methods

4.1 Introduction

Since the pioneering work of Flory [8,9] and Huggins [6,7] a large number of

publications has been devoted to the study of Upper (UCST) and Lower Critical

Solution Temperature (LCST) behaviour in relation to different thermodynamic

and molecular parameters. Basically, for non-polar systems, thus excluding

systems with strong orientational dependent interactions, the UCST demixing

is a result of entropic contributions to the free energy favouring miscibility at

high temperatures and unfavourable energetic interactions ultimately causing the

system to demix at sufficiently low temperatures [68]. The entropically driven

LCST demixing is essentially due to a mismatch between the equation of state

properties of the mixture constituents [68]. The discussion of strong orientational

interactions can only be successful when different theoretical concepts are

applied [1,69], Therefore, in this dissertation only non-polar systems are

considered.

The SS and HH theories not only provide a sound theoretical framework to

discuss the phase behaviour under atmospheric conditions but allow also the

evaluation of miscibility at elevated pressures. In this section (chapters 4-7) of

the dissertation polymer solutions are considered whereas the next section is

devoted to the study of polymer blends (chapters 8,9).

As was already outlined in chapter 2, the compositional derivatives of the

Gibbs free energy of a multicomponent system were in first instance computed

in an approximate manner by Jain and Simha [29]. In order to obtain some

54 Chapter 4

initial results they fitted quartic polynomials in the concentration to the

theoretical free energy. As a first test-case for this procedure the system

polyethylene(PE) /n-hexane(nH) was selected mainly because the equations of

state of both pure components had been studied in detail. In this chapter

recomputed chemical potentials and higher derivates are presented for the

PE/nH system making use of the exact expressions for the compositional

derivatives necessary to discuss phase behaviour. In these computations only the

original Sirnha-Somcynsky theory was used. In a comparison with the theoretical

results of Jain and Sirnha [29] emphasis will be on the LCST phase behaviour

of the system . In the exact computations a wider range of PE molar masses is

considered than previously. The theoretical effect of pressure on the miscibility

behaviour is discussed in detail.

4.2 Phase behaviour of the system polyethylene / n-hexane

In this chapter monodisperse PE/nH systems are considered with the PE

molar mass varying between 8 to 1000 kg/mole. The pure component parameters

are summarized in table 3.3, the molar mass characteristics of the PE samples

are displayed in table 4.1. The cross interaction parameters were quantified in

the same way Jain and Sirnha [29] did, i.e. vAB * = ((vPE*1/3 + vnH.I/3)/2)3

, [Y = 1]

and f. AB * = f.nH *. The pure component parameters however are slightly different

compared to those in the approximate computations. Hence the calculations of

the polynomial representations were repeated for purposes of comparison with

the exact results.

Figure 4.1 depicts the variation of the chemical potential difference of the

solvent AP.nn as a function of the mole fraction of polymer PE1 at atmospheric

pressure at 450 K for the exact and the approximate computations. The mole

fraction was. chosen as the composition variable for the sake of comparison with

the original Jain and Simha results. The differences between the two sets and the

location of the maxima are pronounced, especially at higher concentrations of

Computation of Phase Equilibria 55

o 2 4 8 x, 10• 8 10

Fig.4.1 Exact(--) and approximate(---) curves (a) for the chemical potentials vs. composition

for the system PE1/nH. (b) shows part of plots in more detail.

440

420

400 .._._,_......._ _ _,_ _ __,_ __ .___..__....L... _ _J

0 2 6

Fig.4.2 Exact calculated binodal (--), spinodal (- - -) and critical conditions ( •) at different

indicated pressures for the system PE1/nH. Part of the approximate spinodal(- • -)

at atmospheric pressure is also shown.

56 Chapter 4

the polymer. In (ig.4.2 the computed spinodal curves at three pressures are

displayed. The differences from the polynomial spinodal at 1 bar (the dash-dot

line) are pronounced. These deviations indicate that the quartic polynomial fit

of the oompositional derivatives of the Gibbs free energy is not accurate enough

to c?mpute phase behaviour in a detailed way. As a test of the analytical

derivations and numerical calculations it is noted that binodals and spinodals

make contact at their extrema, in accordance with thermodynamic principles.

Moreover, these extrema are also computed to represent the critical state, as

they should.

Table 4.1 Molar mass characteristics for PE samples

Sample code M (kg/mol)

PE1 8

PEz 10

p~ 50

PE4 100

PE5 177

PE6 500

p~ 1000

In fig.43 the variation of the critical coordinates for polymer PE1 is presented.

Both composition and temperature increase with pressure. However, whereas the

former tends to become practically constant above approximately 600 bars, the

latter increases significantly, indicating the enhanced miscibility at elevated

pressures. As has been recognized in the literature, this is a consequence of the

fact that pressure tends to reduce the differences in the thermal and pressure

properties of the low- and high-molar mass constituents [70,71]. Jain and Simha

[29] concluded that this difference can be expressed solely in terms of the site

Computation of Phase Equili~ria

8 .----.-----r----,-----r---~18

1-7

e

I s I

I

/ /

/ /

/

----..........---

8 8 P1o• (bar)

18

14

10

57

Fig.4.3 Pressure dependence of critical temperature(---) and composition(·--) upto 1000 bar

for the system PEtfuH.

free volume fractions h = 1-y of the constituents, at least over a moderate range

of pressures. Specifically, at the critical point (LCST), the free volume difference

(YPE-YnH) remains invariant to a very good approximation, although YPE and You

increase with pressure. This means an iso-free volume principle applies, i.e. a

certain value of the free volume difference has to be exceeded before LCST

demixing sets in. That this conclusion also stands on the basis of the exact

derivatives, is illustrated in table 4.2. The second column Jists the difference (yPE

YnH) at the critical temperatures seen in the fourth column. AT in table 4.2

represents the difference between the actual and an estimated critical

temperature. The estimate is obtained from the iso-postulate and the value of

(YPE-YnH) at 1 bar. Below about 200 bars, the difference is acceptable. In fig.4.4

the temperature dependence of the free volume difference (ypE-YnH) is shown as

a function of reduced temperature at various pressures. The divergence from the

common intercept at the respective critical temperatures remains small over the

presented range of temperatures. In the case of the PE/n-H solution, the

58 Chapter 4

Table 4..2 The critical temperature Tcn., free volume difference (yPE-YIIH) and excess free volume

h ... as a function of pressure for the system PEtfnH. The temperature difference !J.T

is defmed in the text.

p

[bar]

1

50

100

200

500

1000

21

20

19

Yrll-YDH ·h... at consolute state

0.186883 0.021924

0.186738 0.022291

0.186546 0.023789

0.186034 0.023151

0.184003 0.023680

0.184400 0.022633

5 10

Tcril

[K.]

402.25

413.32

424.84

448.60

526.80

723.64

15 20 (T-T., .. ) (K)

25

!J.T [K]

0.00

0.19

0.56

1.70

9.34

21.66

Fig.4.4 Site free volume difference y2-y1 versus reduced temperature at different indicated pressures

for the system PEtfnH.

Computation of Phase Equilibria 59

volumetric mixing parameter Y equals unity which means that changes in cell

size upon mixing are not in order now. Under this condition the above iso-free ·

volume postulate is applicable. In later chapters it will be explained that this

postulate is not general; under conditions in which cell sizes change upon mixing

the postulate is not applicable any more.

It is well known that LCST type of demixing is initiated by a difference in

free volume quantities of the pure constituents [70,71]. As is shown this can be

expressed in terms of the free volume difference. Alternatively the excess free

volume function hexc serves to demonstrate the free volume influence on

miscibility properties:

(4.1)

with XpE and XnH the mole fraction of polymer and solvent respectively.

Approximate master curves can be constructed on the basis of this excess

function as shown in figure 4.5. Table 4.2 indicates that similar conclusions can

be reached for hexc· A minimum in (yPE-YnH) and an oscillation in hexc can be seen

for which no explanation can be offered. However it is not the result of

numerical inaccuracies in the determination of the critical temperatures.

The spinodal and binodal curves in fig.4.1 can be transformed into a scaled

representation in terms of T-Tcrit and x-"ct;1 as presented in fig.4.6. Approximate

master curves for the spinodals extend over a range of about 20K above Tent·

For the binodals however, superposition is less satisfactory. The miscibility curves

become more narrow with enhanced pressure which is most pronounced for the

binodals. An extension to higher pressures leads to closed-loop miscibility gaps

although at physical unrealistic temperatures for this system. With increasing

pressure this type of phase diagram disappears and yields a new and very broad

miscibility gap at low temperatures. Under these conditions however the pVf

regime, from which the pure component parameters were fitted, is passed which

might lead to errors in the pVf-description in this high pressure regime.

20

10

5

0

0

Ill iii ii\

\II l\ l\ \\

\ .. \ "

Chapter 4

2 4 6 y .,.10' 8

Fig.4.5 The calculated excess free volume for binodal spinodal(---) aod critical (•)

conditions at different indicated pressures for the system P~/nH.

20

10

I 0

-1 0

100bar Ill );

50bar--1/

/It,) bar

I I

I I

I

2 3 4 5 (x,-x,., .. ho•

Fig.4.6 Representation of calculated (T-Tcrit) versus (x-x,;,) for binodal (-),spinodal(---) and

critical conditions (•) at indicated pressures for the system PEtfnH.

Computation of Phase Equilibria 61

Furthermore from a theoretical point of view one might argue that the square

well approximation to the cell potential is no longer adequate for a quantitative

treatment. Because of these reasons a discussion of the predicted high pressure

phase behaviour is not in order now.

Analogous results have been derived for all other molar masses listed in table

4.1. As expected, location and shape of spinodal curves change. However,

superposition of these for a given molar mass and varying pressures is again

accomplished. For high molar masses computations of binodals in terms of mole

fractions give numerical problems. Hence the existence of master curves could

not be verified. The important results concerning the iso-free volume principle

still stand as is displayed in table 4.3, where critical coordinates and free volume

differences are listed. The variation of the free volume difference is relatively

small over the wide range of molar masses between 8 and 1000 kg/mole. This

suggests that an iso-result derived here for the critical conditions of a binary

system, might also be applied for the critical and treshold temperatures of

polydisperse solutions.

In the next section the dependence of the critical coordinates with molar mass

is examined. It is instructive to make a comparison with the Flory-Huggins

theory [6-9] although this theory can not account for LSCf phenomena at all.

The variation of the critical volume fraction 'PPE,c with chain length is in close

agreement with the well known result of this theory, i.e.

(4.2)

Making use of this relation a Shultz-Flory plot can be constructed using

computed critical temperatures for different PE-molar masses at a series of

pressures, see fig.4.7. The intercepts are the reciprocal a-temperatures. The

Flory-Huggins theory predicts, in the absence of equation of state contribution

to the Gibbs free energy, linear relationships in the Shultz-Flory plot. The

Simha-Somcynsky theory gives significant departures from this linearity

62 Chapter 4

Table 4.3 Critical conditions and free volume differences for indicated molar masses and pressures

Sample

code

PE1

PE2

p~

PE4

PE5

PE6

PE,

p

[bar)

1

50

100

200

1

50

100

200

1

50

100

200

1

50

100

200

1

50

100

200

1

50

100

200

1

50

100

200

[K)

402.25 0.186883

413.32 0.186738

424.84 0.186546

448.60 0.186034

396.605 0.183495

407.852 0.183242

417.862 0.182927

439.919 0.182143

373.229 0.169563

381.431 0.168964

389.724 0.168273

405.976 0.166662

368.550 0.166768

376.364 0.166121

384.233 0.165378

399.547 0.163661

365.874 0.165164

373.475 0.164491

381.113 0.163722

395.922 0.161951

362.738 0.163270

370.099 0.162572

377.477 0.161776

391.728 0.159953

361.430 0.162477

368.694 0.161768

375.967 0.160963

389.985 0.159116

Computation of Phase Equilibria

on the low molar mass side where enhanced LeST-miscibility is observed.

Furthermore the predicted Shultz-Flory curves at different pressures are not

superimposable for the lower molar masses of PE. These differences in

miscibility behaviour are not restricted to the consolute state, but extend to the

complete phase diagram. All these phenomena must be related to the reduced

difference in thermal and pressure characteristics between solute and solvent

with decreasing molar mass of the former.

?77

~" ' 0 --\..

2157

237

217 L..._ ___ ...L._ ___ __._ ___ __, __

0 4 8(2/.ta+t/aho•

12

Fig.4.7 Shultz-Flory plot at indicated pressures (bar) for the critical temperatures shown in table

4.2. The solid points are calculated critical temperatures, the lines are drawn to indicate

extrapolations.

64 Chapter 4

4.3 Conclusions

Computations of miscibility-related properties of the first test-case PE/nH

lead to the following conclusions :

1. Rather large deviations occur between chemical potentials and spinodals

computed by the approximate and the exact method. These deviations can be

attributed to the fit of quartic polynomials in composition to the Gibbs free

energy as is done in the approximate version and their use in obtaining higher

derivatives.

2. Critical conditions are characterized by an invariant (iso) free volume

difference, or alternatively by an invariant excess free volume fraction over a

moderate pressure range. Within reasonable limits the variations of this latter

function along binodals and spinodals can be represented by universal curves.

3. The equation of state contribution to the free energy influences primarily the

critical temperature for low molar masses.

Phase behaviour

5. Phase Behaviour : lnftuence of Pressure,

Temperature, Composition and Molar Mass

S.l Introduction

65

In this chapter the SS and HH theories are confronted with phase equilibria

data of the polymer solutions polystyrene(PS)/cyclohexane(CH) and

PS/Methylacetate(MeOAc). In the case of PS/CH also the Flory-Orwoll-Vrij [2-

5] theory and the Sanchez-Lacombe model [13-15] are examined in their ability

to describe and predict miscibility. A comparison of these models is presented.

The influence of pressure, temperature, composition and molar mass on phase

behaviour is examined.

5.2 The system polystyrene/ cyclohexane

5.2.1 Selected Experimental Data

The system PS/CH is selected mainly because a wealth of accurate experimental

information concerning phase behaviour from different laboratories is available.

Another reason is the absence of specific interactions in this system. A selection

of experimental data is used to test the SS and the HH theories. The available

molecular characteristics and supplier information for solvent and polymer are

shown in table 5.1 at the end of this paragraph. All polymer samples are

synthesized anionically which garantees low Mw/Mn polydispersity ratios. For

three different PS fractions, UCST spinodals and critical data [54] are presented

ChapterS

in tables 5.2 and 5.3 and shown iri fig.5.1. Experimental LCST cloud point data

[73] for different PS/CH sets are shown in table 5.4 and fig.5.2. In table 5.5 the

effect of pressure on the upper critical solution temperature is tabulated in the

range between 0 and 300 bar. These data were obtained by Wolf et al [72] for

a PS molar mass of 600 kg/mole. Saeki et al [73] also studied the pressure

influence on upper critical solution temperatures of PS/CH solutions ranging

from 37 to 2700 kg/mole and over a moderate pressure regime from 1 to 50 bar.

These data are summarized in table 5.6.

5.2.2 Determination of Molecular Parameters

The pure component parameters from table 3.4 are used for the computation of

phase equilibria for PS/CH according to the SS and HH theory. The mixing

parameters X and Y are determined from the consolute condition for the system

PS M3/CH1, see table 5.7. These values of the cross parameters are very close

to one which is an indication for the dispersive character of the interactions.

Thus having established all necessary parameters one is in a position to predict

any desired equilibrium thermodynamic property. The requisite expressions for

the evaluation of spinodals are expressed in chapter 2.

The phase behaviour of the PS/CH system is also evaluated by the Flory-Orwoll

Vrij theory. The pure component parameters are obtained from equation of state

data of Hocker, Shih and Flory [74] for CHand H6cker, Blake and Flory [75]

for PS (see chapter 3). The energetic mixing parameter X12 was determined from

the upper critical solution temperature of the system PS(520 kg/mole )/CH : X12

= 1.72*107 J/m3• The entropic mixing parameter 0 12 was set equal to zero. It

was assumed that the number of external degrees of freedom per segment

depends linearly on composition, i.e. c12 equals zero (see chapter 2). This makes

a comparison with the SS and the HH theory more realistic because in these

theories the same assumption is made.

Phase behaviour 67

For the Sanchez-Lacombe theory the pure component parameters were obtained

from literature [13,76], (see chapter 3). The experimental upper critical solution

temperature of PS(520 kg/mole)/CH is used to fit the mixing parameter £ 12*. Note that in the SS and HH theories two mixing parameters are fitted from a

critical temperature and composition whereas in the Sanchez-Lacombe and in

the Flory-Orwoll-Vrij theory one mixing parameter is determined from a critical

temperature.

5.2.3 Phase Behaviour under Atmospheric Conditions

In fig5.1 predicted critical coordinates and spinodals are compared with

experimental results [54,77]. For the HH theory the calculated change of critical

temperature and composition with molar mass of PS is too small. For the SS

theory the agreement with respect to predicted critical temperatures is better but

not in quantitative agreement either. It has been shown that small changes of the

mixing parameters E AB * and v AB * with molar mass can correct the deviations

between theoretical and experimental critical coordinates [32]. For the present

discussion we will not go into detail concerning these issues because 1)

introducing these corrections the molecular cross parameters become molar mass

dependent which is an empirical correction and 2) we want to predict

thermodynamic properties with a minimum of adjustable parameters for the sake

of argument and simplicity. It is interesting to note however that in a recent

article Schleifer traces these deviations back to the ignoration of any

conformational changes upon mixing [78]. Differences between theoretical and

experimental spinodal branches at the low polymer concentration side are

related to dilute-solution effects. The presented theories are derived for uniform

segment densities. In dilute solutions large fluctuations in the local segment

density exist, thus violating the uniform segment density approximations. Also the

right hand side of the calculated spinodal branches is somewhat too narrow in

comparison with experimental data. These differences can be reconciled if small

changes in the flexibility parameter [32] are tolerated, which can be interpreted

as a slight temperature dependence. Again, for the sake of clarity we will

68

~

.E 1-

ao5

aoo M3

M2

295

290 M1

285

280 ~~U----L--~----~-l~~~

0.00 0.06 0.10 0.16 0.20 0.25 0.30

w,..

Chapter 5

Flg.S.l Experimental UCST spinodal (o) [54) and critical data (D) [77] for the systems PS Ml, M2

and M3 in CHl. Predicted critical coordinates (•) and spinodal curves according to SS

(- - -) and HH (-) theories

~

.E 1-

5 20 ,---------------------------.

510 • • • • ... ... ... ... ... ...

500

• • - • • Q:) 0 tAM ~ 490 I:[) a

480

470

460

460 ~--~---L--~----~---L----0.00 0.05 0.10 0.15 0.20 0.25 0.30

w,..

Fig.5.2 Experimental LCST cloud point data [73) for different molar masses (M5 (e), M9(.a.),

MlO(•), Mll(o), M7(.t.) and M12(0)) and predicted spinodal curves according to the SS

theory

Phase behaviour

:.:: .&

1-

520

610

600 • • • Cb 0

490 t:A""" rJ/1 1110

480

470

460

450 '-------''---------'---'----'----'----' 0.00 0.05 0.10 0.15 0.20 0.25 0.30

w ..

69

Fil-5.3 Experimental LCST cloud point data [73] for different molar masses (MS ( • ), M9( • ),

MlO(->, Mll(o), M7(•) and M12(0)) and predicted spinodal curves according to the HH

theory

proceed with the pure component parameters estimated from the fit-procedure

of p VT -data and with mixing parameters quantified by fitting just one

experimental critical point. In fig.5.2 and 5.3 the predicted spinodals and

experimental LCST phase behaviour (i.e. binodals) for the data of Saeki et al

[73] are compared. Although one can not compare these data directly the

agreement is satisfactory, particularly if one realizes that with the set of

molecular parameters estimated from a energetically driven phenomena situated

at a temperature of about 300K, an entropy driven demixing 180K higher is

predicted with this accuracy. Also here the change of the critical coordinates with

molar mass is slightly underestimated. This is comparable to the situation

observed for the UCST behaviour. Comparison of the spinodal curves predicted

by either the SS or the HH theory reveals differences between these models. For

the HH theory the LCST miscibility gaps are predicted at higher temperatures,

in better agreement with experimental data. Furthermore the predicted spinodals .

according to the HH theory are considerably broader than the corresponding SS

spinodals.

70 ChapterS

It is well recognized that LCST demixing is governed by free-volume differences

between the constituents [31,70,71]. In the hole theories discussed here this

quantity is explicitly defined in terms of the structure parameter h ( = 1-y), i.e.

the free site fraction. The improved miscibility predictions according to the HH

theory are realized because of a smaller difference in this quantity, as presented

in fig.5.4. The observed shift of the LCST of approximately 50K is larger than

the shift one would anticipate from fig.5.4 in which only pure component free

volume characteristics are considered. So the iso-free volume concept does not

solely explain the observed difference of LCST phase behaviour according to the

two theories. Apparently there are also other factors responsible, these will be

considered in detail in chapter 7.

The predicted UCST spinodal phase behaviour according to the Flory-Orwoll

Vrij theory is presented in fig.5.5 for three molar masses of PS in comparison

with experimental spinodal points and critical conditions. The spinodals are too

narrow compared with the experimental ones and the critical points are shifted

towards the low polymer concentration edge of the phase diagram. The

temperature shift of the spinodals with molar mass is overestimated. With all

parameters kept constant, LCST phase behaviour is predicted approximately

lOOK too low, as is shown in fig.5.6. One has to keep in mind that the pure

component parameters were determined from dilatometric data at zs·c. To

describe pVT-data in the high temperature regime in accurately, these

parameters must be revaluated. This is one of the drawbacks of the Flory

Orwoll-Vrij theory. In order to obtain a reasonable fit ofpVT data, parameters

have to be adjusted as a function of temperature. If one accepts this temperature

dependence a reasonable description of phase behaviour can be obtained but a

direct comparison with the SS and HH results is more difficult because in these

theories no temperature dependence of the parameters whatsoever is introduced.

Quite unexpectedly UCST phase behaviour can not be described making use of

the Sanchez-Lacombe theory for the PS/CH system. Only LCST type of

Phase behaviour

0.30

0.20

0.10

0.00 '-----''-----''-----''-----''--__,j

300 350 400 450 500 550

TIn K

Flg.5.4 Site free volume difference of the pure constituents PS and CH versus temperature

~

.E

...

310 .....-----------.

290 0

270

2 50 IIJ-L---''-----''-----''-----''-----ll

0.00 0.05 0.10 o. 15 0.20 0.25

Weight fraction PS

71

Fig.S.S Experimental UCST spinodal (0) [54) and critical data (•) [77) for the systems PS Ml, M2

and M3 in CHl. Predicted spinodal curves according to FOV theory

72 Chapter 5

520 ,....------------,

• • • • ... ... ... ... ... ... 500 ~~0- • •

480

~ 460 .5 ... 440

420

400

3 8 0 '------"'--------'"----J..__--J.__---1

0.00 0.05 0.1 0 0.15 0.20 0.25

Weight. fraction PS

Fig.S.6 Experimental LCST cloud point data [73] for different molar masses (M5 (e), M9(•),

MlO(•), Mll(o), M7(4) and M12(D)} and predicted spinodal curves according to the FOV

theory for the systems PS (Ml,M2,M3)/CH.

demixing is achieved when one fits the experimental upper critical solution

temperature of the system PS(M =520 kg/mole )/CH. Thus the Sanchez-Lacombe

theory fails to describe the occurance of both UCST and LCST type of demixing.

5.2.4 Pressure InOuence on Phase Behaviour

The experimental findings of Wolf and Geerissen [72], concerning the pressure

influence on UCST for the PS M4/CH system, are compiled in fig5.7. As

indicated by the previous results, one may expect deviations between

experimental and theoretical data under atmospheric (conditions, due to the

Phase behaviour 73

8 I I I I I I I I I I I

2 I I I I I I

~ I I I

.5 I I I I

t I I I

1- I I •. I

I

1- I I I I I

0

-1 L-~--~--~--J---L-~~~

o so 100 uso 200 210 8oo aso

p in bar

Fig.5.7 Differences between critical temperatures at elevated and atmospheric pressure versus

pressure. Experimental data (72) (e) and predicted pressure dependence according to SS

(- - -) and HH (-) theories.

so~-------------------------.

----40

80

20

10

~· 0 ~--~~------. ... .---------1

•• • -10 L_------~---------L------~

0.50 1.50 2.110 8.50

log M (M in kg/mole)

Fig.5.8 Pressure coefficient ( 8T / 8p )c vs. the logarithm of molar mass. Experimental data of Saeld

et al (e) [73) and Wolf et al (•) [72]. Predicted pressure coefficient according toSS

(- - - ) and HH (--) theories

74 Chapter 5

selection of the mixing parameters. Furthermore Wolf and Geerissen [72] have

shown that for solvents of llifferent suppliers, somewhat different critical

temperatures are obtained. Therefore the pressure dependence of the critical

temperature is presented in reduced form, i.e. relative to the temperature at 1

bar. The SS theory predicts a continuous increase with pressure. The modified

hole theory however gives an excellent prediction of the observed effect. Slope

and change in sign are predicted quantitatively. The results of the pressure

studies of Saeki et al [73], combined with those of Wolf and Geerissen [72], are

presented in fig.5.8. The initial slope at 1 bar (aT I ap )t is negative for sufficiently

high molar masses of PS. With decreasing molar mass (BT/8p)t becomes zero

and turns positive for· even lower molar masses. So in the low pressure regime

pressure improves miscibility for low molar masses of PS, at a molar mass of

nearly 100 kg/mole phase behaviour app~ars invariant to pressure and at higher

molar masses increasing pressure deteriorates miscibility. This trend is indeed

predicted by HH but not by. the SS theory, see fig.5.8. The computed and

measured values of (aT/ ap )t differ by approximately a constant amount for all

molar masses. Consequently the computations suggest a change of sign at lower

molar mass as found experimentally. One has to realize however that all these

predictions are based on mixing parameters determined from one single critical

temperature and composition at atmospheric pressure for PS(M=520

kg/mole)/CH. These results demonstrate quite clearly that the HH theory gives

a very good prediction of these subtle pressure effects. For completeness, the

change of critical composition with pressure for UCST and LCST phase

behaviour is presented in fig.5.9. According to eq.6.4 these changes are related

to the fourth compositional derivative of the Gibbs free energy. This is one of

the rare phenomena that probes the compositional dependence of the free

energy in such an intrinsic manner. However, presently no systematic

experimental study for polymer solutions is available. These calculations reveal

differences between the SS and the HH theory and experimental information

could give an extra indication of their relevance.

Although there is no experimental information to our knowledge about the

pressure influence on LCST demixing, predictions by the SS and the HH theory

Phase behaviour

CD A.

I i

0.55

0.50

1 0.45

• 0 -

0.40 L-------'------'-----L-----'

0 100 200 300 400

P in bar

75

Fig.5.9 Predicted pressure dependence of the critical composition according to the SS (- - -) and

HH (--) theories for the system PS M3/CH

260

200 I

I I

!II: I 160 I

.5 , , 0 / l /

1- / I 100 / .. /

1- / /

/ /

/ / so /

/ /

/ /

/ /

0 ....

0 100 200 300

p in bar

Fig.S.lO Difference between critical temperature at elevated and atmospheric pressure vs. pressure

according to the SS (- - -) and HH (--) theories

76

... • :e

1.00.------------,

0.80

:\il::: 0.60 ----------.6 __

..... _____________ _ 0.40

0.20

0.00 ~-----------1 0.50 1.60 2.60 3.60

Jog M (M In kg/mole)

Chapter 5

Fig.S.ll Pressure dependence (aTjap). versus the logarithm of molar mass according toSS

(-- -) and HH (-) theories

are shown in fig.5.10. The effect is considerably larger than the effect on UCST

demixing. In fig.5.11 the molar mass dependence of (aT/ap)c under atmospheric

conditions is presented. The predicted pressure effect is larger for the HH theory

and miscibility will be enhanced with pressure moving towards lower molar

masses of PS. Again, for the moment these effects can not be verified with

experimental facts.

The influence of pressure upon the upper critical solution temperature according

to the Flory-Orwoll-Vrij [2-5] theory is presented in fig.5.12. The predicted large

enhancement of the miscibility with pressure is not in agreement with the

experimental facts so the Flory-Orwoll-Vrij theory fails to predict the pressure

influence on miscibility for the PS/CH system. The effect of pressure on LCST

demixing is not investigated.

It was mentioned previously that the Sanchez-Lacombe [13-15] theory does not

predict UCST phase behaviour for the system PS/CH. Consequently the

influence of pressure can not be discussed.

Phase behaviour 77

1

• 0 •

• • • • ~ -1

.s: 0 -2 l

1-I ...

-3 1-

-4

-5 0 100 200 300 400

p in bar

Flc-5.12 Difference between critical temperatures at elevated and atmospheric pressure vs. pressure

for the system PS M4/CH. Experimental data (72] ( •) and predicted pressure dependence

according to the FOV theory

78 Chapter 5

'lilllle 5.1 Available Molecular Characteristics and Supplier Information for Selected Samples

Sample

PSMl

PSM2

PSM3

PSM4

PSMS

PSM6

PSM7

PSM8

PSM9

PS MlO

PS Mll

PS M12

PS M13

CHI

CH2

CH3

1WM., (kg/mol)

51

166

s:w 600

37

110

670

1450

97

:wo 400

670

2700

1.04

1.08

1.19

<1.10

<Ul6

<1.06

<1.15

<1.10

<1.06

<1.06

<1.06

<1.10

<1.10

spectrochemical quality

Merck

Supplier

Pressure Chemical

Pressure Chemical

Pressure Chemical

Pressure Chemical

Pressure Chemical

Pressure Chemical

Pressure Chemical

Pressure Chemical

Pressure Chemical

Pressure Chemical

Pressure Chemical

Pressure Chemical

Pressure Chemical

Phase behaviour 19

Tallie 5.2 Spinodal Data for PS Fractions M1, M2 and M3 in Cyclohexane [54]

wi'S.IIpia

PS M1/CH1

219.55 .0258 288.45 .'1JY1.9

284.15 .0435 287.35 .ITIS6

287.35 .0764 288.25 .0894

288.25 .0903 288.95 .1194

288.95 .1204 289.05 .1404

289.05 .1415 288.95 .1707

288.95 .1721 288.45 .2013

PSM2/CH1

289.95 .0186 29555 .1496

294.25 .0407 296.05 .0617

296.05 .0620 296.35 .0817

296.35 .0821 296.45 .1008

296.45 .1012 296.25 .1230

296.25 .1243 295.55 .1489

PSM3/CH1

291.55 .0175 300.45 .0635

299.65 .0289 300.15 .0832

300.45 .0450 299.55 .1046

80 Chapter 5

Table 5.3 Critical Coordinates for PS Fractions Ml, M2 and M3 in Cyclohexane [77]

Solution

PS M1/CH

PS M2/CH

PS M3/CH

288.85

296.60

301.15

.146

.099

.064

Table 5.4 Experimental LCST Ooud Point Data for PS/CH Solutions [73]

TinK WPS TinK

PSM12/CH2

489.13 .0180 488.81 .0351

488.60 .0224 491.08 .0605

PS M7/CH2

491.78 .0070 491.77 .0362

492.10 .0143 491.93 ..()655

491.74 .0275 492.39 .o733

PS Mll/CH2

497.27 .0023 495.01 .0279

495.36 .0218 494.49 .0810

Phase behaviour

Table 5.4 Continued

PSM10/CH2

4'YI3l .0306 496.82 .1039

496.93 .0565 4'Y1.38 .1327

496.89 .fD72 498.12 .1524

PSM9/CH2

503.81 .0247 501.83 .1041

502.52 .0503 501.97 .1229

502.02 .0753 502.21 .1520

PSM5/CH2

51L44 .(1537 510.42 .1589

510.86 .0806 512.44 .2276

510.70 .1060 513.11 .2325

Table S.S Experimental Critical Temperatures vs. Pressure for PS M4/CH Solution

pin bar

1

37

88

UCSTinK

301.34

301.11

300.95

PSM4/CH3

152 300.96

pin bar

187

260

300

Data are extracted from the original f.gure in reference (72].

UCST inK

301.12

301.43

301.68

81

82 ChapterS

Table 5.6 Experimental Critical Te1p.peratures vs. Pressure for indicated Solution (73]

pin bar UCSTinK pin bar UCSTinK

PS M5/CH2

1 285.41 30 285.49

10 285.43 40 285.53

20 285.46 50 285.56

PS M6/CH2

1 294.38 30 294.36

10 295.36 40 294.35

20 294.35 50 294.35

PSM7/CH2

1 300.97 30 300.81

10 300.91 40 300.79

20 300.86 50 300.75

PS M8/CH2

1 303.27 30 303.10

10 303.21 40 303.04

20 303.15 50 302.98

Phase behaviour 83

'l'llllle 5.7 Cross interaction parameters for the system PS/CH as determined from the consolute

state of solution PS M3/CH1

ss HH

X

.99630807

.99134879

y

1.()0638489

1.00691909

84 Chapter 5

5.3 The system polystyrene/methylacetate

5.3.1 Introduetion

The system polystyrene(PS)/methylacetate(MeOAc) is selected because both

UCST and LCST type of phase behaviour appear. Furthermore the pressure

influence on these two types of phase behaviour is knQWD from literature. From

an energetic and entropic point of View however the system PS/MeOAc is not

an ideal model system to study in the. framework of the SS and HH theories. In

these theories the energetic interaction between two segments is described by

means of a Leonard-Jones potential. In applying this potential one assumes that

only dispersive interactions are involved and this assumption is questionable for

the PS/MeOAc solutions. The ester group of the solvent may interact in a

preferential way with the phenyl group of the polymer which makes the Leonard

Jones description inappropiate. Also the random mixing assumption might be

violated by this possible specific interaction. Despite these remarks the

PS/MeOAc system is investigated with the HH theory to see what is achievable

with this model.

5.3.2 Seleeted Experintental Data

Molar mass characteristics and supplier information of PS and MeOAc are

reported in table 5.8. UCST cloud points have been measured by Kubota, Abbey

and Chu [79] for PS M20/Me0Acl and are presented in fig.5.13 together with

cloud points and spinodal data measured by van Dijk and Wakker [80] for PS

M21/Me0Ac2. These data are tabulated in table 5.9 and 5.10. LCST cloud

points are determined by Myrat and Rowlinson [81] for solutions with varying

molar mass of polystyrene (PS M22-27/Me0Acl), see table 5.11 and fig.5.14.

UCST and LCST cloud point temperatures and pressure influence on these

Phase behaviour 85

310

•• • 0 0

290

~

.e ... 270

250 ~----~~~~--~~ 0.00 0.10 0.20 0.30

Weight fraction PS

Flg.5.13 Experimental spinodal (0) [80] and cloud point data( .. ) [79), (e) (80) for the systems PS

M20 and PS M21 in MeOAd/2. Predicted spinodals according to the HH theory

430

~

.e 410

...

390

3 7 0 ~------==--'-------'--------1 0.00 0.10 0.20 0.30

Weight fraction PS Fig.5.14 Experimental cloud points (81) for the systems PS M22·27 / MeOAcl. Predicted spinodals

according to the HH theory.

86 Chapter 5

temperatures are determined by Zeman and Patterson [82] for pressures from

1 to 300 bar. These cloud point temperatures are all very close to the critical

temperatures of the respective solutions. The authors assume that the pressure

influence on these critical temperatures is identical to the influence on the cloud

point temperatures. The experimental findings concerning this pressure influence

are displayed in fig.5.15.

5.3.3 Determination of molecular parameters

The HH theory is used for the computation of phase behaviour of the system

PS/MeOAc because it has been shown in the previous paragraphs of this chapter

that this theory gives superiour results compared to the original theory in the

case of PS/CH. To fit the pure component parameters, equilibrium pVT-data

were used. For PS, data of Quach and Simha [24] served to obtain the molecular

parameters whereas in the case of MeOAc data of Kumagai and Iwasaki [66]

were applied ranging from -20 oc to 40 oc and pressures upto 1600 bar.

The choice of the segment size for PS is not so straightforward as it is for the

system PS/CH. The reason for this is the small value of the volume parameter

for methylacetate in comparison with the value for the styrene repeat unit, see

table 3.5 where all scaling parameters are compared. With these values for the

pure component parameters, no realistic phase behaviour can be produced which

is due to the applied mixing rules in the theory. As Prigogine already pointed out

especially the hard core volumes of the pure component should not differ much

although no strict limit can be given for this difference. With the values of table

3.5 in mind this means the size of the PS segments should be decreased. This is

a quite arbitrary manoeuvre. We have selected a value for the segmental molar

mass of PS of 86 g/mole which corresponds to a volumetric parameter of

8.1539*10-5 m3/mole. This value was selected on the basis of the experimental

available demixing information. After fitting the maximum point (see table 5.9)

in the UCST binodal of Kubota, Abbey and Chu [79], which gives the mixing

parameters listed in table 5.12, the LCST demixing is described in a satisfactory

way as will be presented in the next section of this chapter. If another value is

Phase behaviour

310

+

300

~

.e 290 + 1- • •

280

• • • 2 70 .____.__....______......__ .......... ___ __.

0 100 200 300

p in bar Fig.5.15 Pressure influence on cloud point temperatures [82] for the solutions PS M 29-34 I

Me0Ac3. Predicted pressure dependence of UCST of the corresponding solutions

accortling to the HH theory 500r-~-----------~

450

... . . + •

•• • " ..

" ... • •••

+ •

•

•

3 50 ....___._ _ _.__~.....__ ......... __ ......___.

0 100 200 300

p in bar Fig.S.l6 Pressure influence on cloud point temperatures [82] for the solutions PS MlS-31,34

I Me0Ac3. Predicted pressure dependence of LCST of the corresponding solutions

according to the HH theory

87

88 Chapter 5

chosen for the segmental molar mass, the LCST phase behaviour is calculated

at slightly different temperatures. Thus, although for the equation of state

behaviour a change in segmental molar mass is unimportant (see chapter 3), for

the miscibility behaviour it is of importance. Also the pressure influence on

UCST and LCST phase behaviour is predicted reasonably well with this value

for the segmental molar mass, see paragraph 5.3.4. So the demixing information

formed the basis for the selection of the value of the PS segmental hard core

volume. In this context one can not speak any more about a pure prediction but

about a description of the demixing characteristics for this system. The values of

the mixing parameters in table 5.12 deviate. largely from unity which may be

interpreted as an indication for the non-dispersive contributions to the total

intersegmental interaction.

5.3.4 Phase behaviour. under atmospheric conditions

The theoretical UCST spinodals are presented in fig.5.13 together with the

experimental cloud points of Chu et al [79] and the cloud points and spinodals

of Wakker [80] et al. The theoretical spinodal representing the system of Chu

et al. seems too broad on the high polymer concentration site in comparison with

the experimental cloud points. In predicting the other molar mass spinodals, all

pure component and mixing parameters are kept constant. The shift of the

spinodal temperatures with molar mass going from system PS M20 to M21 is

largely underestimated, see fig.5.13. The predicted spinodal is much too broad

compared to experiment. With the interaction parameters obtained from UCST

demixing, LCST phase behaviour is described approximately 40-50 K too low,

see fig.5.14 where a comparison is made with the experimental information of

Myrat and Rowlinson [81 ]. Also in this high temperature region, the spinodal

temperature shift with molar mass is again underestimated. Furthermore most

spinodals are shifted to higher concentrations of PS compared to experiment.

Phase behaviour

5.3.5 Pressure inftuence on phase behaviour

The experimental findings of Zeman and Patterson [82] concerning the initial

pressure influence on upper critical solution temperatures are shoWn in fig.5.15

as a function of molar mass of PS. In the low pressure regime increasing

pressure enhances the miscibility of PS/MeOAc ,i.e .. (aTjap)c is negative,

whereas with increasing molar mass of PS (BT/ap)ctends to more negative

values. The HH theory indeed predicts negative values.Jor (BT/Bp)c and also

the observed trend with molar mass is there, although the effect is less

pronounced. Zeman and Patterson [82] observed that ~with increasing pressure

the factor (BT/op)c goes to less nega,tive values and se~ms to become zero at

approximately 300 bar, see fig.5.15. This tendency is predicted in an accurate

way by theory (see fig.5.15), the observed temperature discrepancy is of course

related to the underestimation of the temperature shift. with molar mass. The

pressure effect on LCST phase behaviour is more pronounced as for the UCST

case, see fig.5.16. Increasing pressure enhances miscibility in a way which is

molar mass independent but also more or less pressure independent, i.e. the

value of (iJT/ap)c is not very sensitive for changes in pressure (see fig.5.15 and

5.16). This first effect is expressed in fig.5.17 where the initial pressure

dependence is plotted vs. the molar mass of PS and in fig.5.18 which represents

the shift of lower critical solution temperatures vs. pressure for indicated

PS/MeOAc solutions. The initial pressure dependence is somewhat

underestimated by theory (see fig.5.18) but it is almost molar mass independent

in accordance with experiment. The observed theoretical invariance of (aT I ap )c

with pressure is also in agreement with the experimental findings of Myrat and

Rawlinson [81] (fig.5.16).

The Flory-Orwoll-Vrij [2-5] and the Sanchez-Lacombe [13-15] theories have not

been used to investigate phase behaviour of the system PS/MeOAc.

90 Chapter 5

0.00

-0.02 • .. • .ll ...... :X: -0.04 .E

-· i -0.06 ...... ~ •

.... ~ •

-0.08 •

-0.10 1.50 2.50 3.50

log M (M in kg/mole)

Fig 5.17 Experimental (•) and theoretical t--) pressure coefficient (8T/8p). for UCST versus

the logarithm of the PS molar mass

... • .ll ...... :X:

.!: • a.

"0 .... .... ~

0.50 r-----------, •

0.40

0.30

0.20

0.10

• • •• • •

0.00 L..-------'-----....1

1.50 2.50 3.50

log M (M in kg/mole)

F"tg 5.18 Experimental (.) and theoretical (--) pressure coefficient ( BT I ap ). for LCST versus

the logarithm of the PS molar mass

Phase behaviour '1

Table 5.8 Available Molecular Characteristics and Supplier Information for Selected Samples

Sample

PSM20

PSM21

PSM22

PSM23

PSM24

PSM25

PSM26

PSM27

PSM28

PSM29

PSM30

PSM31

PSM32

PSM33

PSM34

MeOAcl

Me0Ac2

Me0Ac3

1(}3M,

(kg/mol)

179

756

48

'59

65

99

195

270

51

en 160

498

670

860

1800

Supplier

1.07 NBS

1.04 Polymer Lab.

1 Monsanto

1 Manchester University

1.18 Manchester University

1.04 Manchester University

1.10 Monsanto Co.

1.09 Monsanto Co.

<1.10 Pressure Chemical

<1.10 Pressure Chemical

<1.10 Pressure Chemical

<1.10 Pressure Chemical

<1.10 Pressure Chemical

<1.10 Pressure Chemical

<1.10 Pressure Chemical

Unkown

Aldrich

British Drug Houses

92 Chapter 5

TaWe 5.9 Experimental UCST cloud points for PS M20/Me0Acl according to Kubota. Abbey and

Chu (79]

TinK

281.30

284.03

285.66

286.96

Maximum point:

.00195

.0158

.03389

.()6981

287.45 .10

TinK

287.36

286.99

286.61

284..56

Data are extracted from original figure in reference [79].

.()9211

.1140

.01323

.1650

Table 5.10 Experimental UCST and LCST Spinodal and Cloud Points for the System PS

M21/Me0Ac According to van Dijk and Willer [80]

0.00503

0.0160

0.0325

0.0647

0.1030

T-inK

UCST

296.10

300.66

301.45

299.06

295.40

291.7 414.0

401.18 299.1 404.7

401.25 301.3 401.3

401.25 297.7 403.3

294.3 405.3

Phase behaviour 93

Table 5.11 Experimental LCST Cloud Point Data for Indicated PS/MeOAc Solutions according

to Myrat and Rowlinson (81)

TinK ·TinK

PS M22/Me0Acl

440.33 .0040 427352 .0498

435.59 .0098 427.23 .0679

434.9 .0116 427.41 .0753

433.59 .0152 427.76 .0902

431.65 .0182 427.89 .0982

430.01 .0249 428.09 .1014

428.78 .0324

PS M23/Me0Acl

435.34 .0070 427.88 .0325

434.67 .0075 426.73 .0517

429.35 .0221 426.94 .0882

PS M24/Me0Ac1

431.11 .0065 425.50 .0219

428.68 .0127 422.76 .0584

427.32 .0117 422.98 .0696

PS M25/Me0Acl

407.98 .0102 406.19 .0376

407.54 .0139 401.95 .0724

410.69 .1177

PS M26/Me0Ac1

412.34 .0056 409.23 .0684

410.72 .0115 409.58 .0882

409.64 .0186 410.05 .1206

408.17 .0292 410.44 .1224

Chapter 5

Tallie 5.11 Cootinued

PS M27/Me0Ad

411.08 .0004 405.79 .()44.9

408.44 .0114 406.16 .0736

406.70 .0242 406.81 .fiJffl

405.79 .CM49

Data are extracted from the original figure in ref.81

Table 5.12 Cross interaction parameters for the system PS/MeOAc as determined from a 6t of

the maximum point in the binodal curve of Kubota, Abbey and Chu [79)

X y

HH 1.0299715 0.99011000

Phase behaviour

5.4 Conclusions

Both SS and HH theories are capable to describe and predict phase behaviour

of the solution PS/CH under atmospheric conditions. However, important

differences between both theories emerge if one is interested in the influence of

pressure. For LCST phase behaviour no detailed experimental information is

available. Both theories predict an increased miscibility with pressure which can

be related to a reduced difference in free volume between both components

upon applying pressure. For UCST phase behaviour, significant differences -

between both theories appear. Particularly the HH theory is very successful in

predicting subtle pressure phenomena observed for UCST phase behaviour. The

SS theory fails to predict these effects. Thus for the first time a theory (HH

theory) is able to predict the complete phase behaviour of the system PS/CH in

a consistent manner.

Inspired by these results, the HH theory is confronted with phase equilibria

of the solution PS/MeOAc. With an adapted value for the segmental polystyrene

size, UCST and LCST demixing under atmospheric conditions can be descnbed.

The pressure influence on both UCST and LCST types of phase behaviour is

described in a satisfactory manner.

The Sanchez-Lacombe theory is not capable in describing UCST type of phase

behaviour for the system PS/CH. '

The Flory-Orwoll-Vrij theory gives a reasonable description of UCST and

LCST of phase behaviour for the system PS/CH. The parameters however have

to be adapted which is clearly a shortcoming of the model. The pressure

influence of phase behaviour is predicted less satisfactory.

96 Chapter 5

Thermodynamic Excess Functions

6. Thermodynamic Excess Functions and

Correlations with Phase Behaviour

6.1 Introduction and Some General Principles

97

In the previous two chapters phase behaviour of polymer solutions was studied

at atmospheric conditions and at elevated pressures. For the solution PS/CH

the HH theory gives a quantitative prediction of the shift of upper critical

solution temperature with pressure. The pressure influence on both UCST as

well as LCST phase behaviour is predicted in a satisfactory manner for the

solution :PS/MeOAc.

The shift of either UCST or LCST critical coordinates with pressure is related

to thermodynamic excess functions of the system according to general principles.

which can be derived as follows [68,83].

For a binary system one may express the molar Gibbs free energy as a function

of the independent variables pressure, temperature and composition :

dG = (8G/8T)p,xdT + (8G/8Ph.xdp + (8G/8x)p,ydx (6.1)

with x a composition variable. Differentiating the left and right hand side of

equation 6.1 twice in respect to composition, keeping p and T constant. one

obtains at the consolute state :

(6.2)

Chapter 6

with V,S and H the molar volume, entropy and enthalpy. Expressing excess

enthalpy and excess volume in the same composition variables as used in

expression 6.2, one obtains :

with VCXI! and JICXC the molar excess volume and molar excess enthalpy. From

eq.6.3 one learns that the shift of the critical temperature with pressure is

related to the second compositional derivative of the excess volume and excess

enthalpy at the consolute state. The relation for the shift of composition with

pressure is obtained by differentiating eq.6.1 three times in respect to

composition which leads ultimately at the critical point to :

(IJx/Bp)<: =

(6.4)

This shift is one of the very rare phenomena which is related to the fourth

derivative of the free energy towards composition. From general thermodynamics

one comes to the conclusion that the sign of ( 82Hexc I ar)p,T at a lower and an

upper critical solution temperature is fixed, which can be derived as follows. One

may write for a point (T ,x) at the spinodal close to the consolute state :

T-Tc =.AT and x-Xc = Ax. We expand the functions T(x) and 82G/8r(T,x) at

the spinodal around the consolute state :

(6.5)

'Thermodynamic Excess Functions

A(/J2G/1Jx2) = (/J3G/1Jx3)Jlx + (B3G/Bx2/JT))T + lh[(a"G/Bx4)~ +

2(/J4G/BilAT))TAx + (/J4G/(1Jr/J~)) A~] + ... = 0 (6.6)

At the critical point (IJT/Bx)c = 0 and (/J3G/Bx\ = 0. Ignoring the case

(a"Gj/Jx4)c = 0, i.e. (/J4G/Bx4)c > 0 (see [83]) and neglecting the latter two and

higher order terms in eq.6.6 one obtains :

(6.7)

Using (a3GjaraT)P = -(a2S/Br)p,T one finds the general relation for the

curvature of the spinodal at the consolute state :

This curvature is negative for upper critical solution temperatures and positive

for lower critical solution temperatures. Because (a"Gj/Jx4)c>O the curvature of

the excess enthalpy is negative at UCST conditions ((/J2H/Br)c < 0) and positive

for a LCST ((/J2H/Br)c > 0). Also for the excess enthalpy these conditions are

fulfilled at UCST resp. LCST. From equation 6.2 it can be concluded that the

shift of the critical temperature with pressure (aT/IJp)c has identical sign as the

term ( a2v-: I Br)c in the case of LCST and opposite sign in the case of UCST.

On the basis of the above theoretical considerations we are in a position to link

the pressure influence on demixing behaviour, as presented in the previous

chapter, to the excess functions. This link is particularly interesting for PS/CH

because of the observed change of sign of (BT/Bp)c in the case of UCST

demixing. In this chapter we will focus on this link for the solutions PS/CH and

PS/MeOAc and relate the predicted values of the excess functions to

experimental data.

100 Chapter()

6.2 The System Polystyrene/Cyclohexane

6.Z.l Link between Excess Volume and Pressure Influence on Phase Behaviour

In the previous chapter the pressure influence on phase behaviour was studied

for the system PS/CH. Concentrating on the upper critical solution temperature,

the HH theory predicts a change of (8T/8p), with increasing molar mass (see

fig5.8) and a change of sign with increasing pressure for a particular solution

(PS(M=600 kg/mole), see fig.5.7}, which are both verified by experiment [72-

73]. According to relation 6.3 this change of sign is related to a change in the

curvature of the excess volume- composition curve. This is illustrated in fig.6.1

where the computed excess volume is presented versus composition for different

molar masses of PS at the critical temperatures. Indeed a change of curvature

is observed in the low PS composition range where the critical compositions are

located. With decreasing molar mass the derivative

• 0 E .... ·e -i

> ... 0 ....

0.00

-0.80

-1.00

-1.10

-2.00

-2.50 c__ _ _,_ _ __,_ __ ..__ _ _.._ _ __,J

0.00 0.20 0.40 0.60 0.80 1.00

Fig.6.1 Predicted excess volume vs. composition for PS/CH solutions at upper critical solution

temperatures. Molar mass PS indicated in kg/mol.

Thermodynamic Excess Functions 101

(a2VCJ(£ lar)p,T changes locally from positive to negative values. With the

endothermic condition for UCST in mind, this corresponds to negative values of

(aT I ap )c for high molar masses of PS and positive values of (aT I ap )c for low .

molar masses. This is in agreement with the data in fig.5.8.

The change of sign of (aTiaP)c.for the PS(M=600 kglmole)ICHsolution is also

analyzed by a study of the path of the corresponding excess volumes. In fig.6.2,

6.3 and 6.4 the total excess volume is plotted for the system at 1, 100 and 300

bar. At the critical composition (wps = 0.06) a change of curvature is observed

with increasing pressure leading to negative values of (aT I ap )c at low pressures,

(aTiaP)c equals zero around 100 bar and beyond 100 bar (aTiap)c becomes

positive in agreement with fig.5.7.

There are two theoretical contributions which are responsible for the total

volume change upon mixing. First of all the total number of vacancies changes

when the two components are mixed. A decrease of this number will cause

volume contraction of the total system whereas an increase favours an expansion

0.3 .----------------,

0.2

0.1

0.0 ' '

-0.1

-0.2

-0.3

-0.4

' ' ' '

'

'

vac

',

-0.5 '-----~--'--~----'-~-..____~_,_~___,

0.0 0.2 0.4 0.6 0.8 1.0

Wpa

Fig.6.2 Computed total excess volume.(tot) vs. composition for PS(M=600 kg/moi)/CH at UCST

at 1 bar. Vacancy (vac) and cell volume (cv) contributions are included.

102

0.3 r--------------,

0.2

0.1

0.0 ' '

-0.1

-0.2

-0.3

-0.4

' ' ' ' ' ' ' ' ' '

'

' ' ' vac'· .•.

tot

'•, ---'

'

'

' ' '

' . . . ' .

-0.1 L..-~-'-~-.l..-~--L-~...1-~---l 0.0 0.2 0.4 0.6 0.8 1.0

Wpa

Chapter 6

F1f1.6.3 Computed total excess volume (tot) vs. composition for PS(M=600 kgjmol)/CH at UCST

at 100 bar. Vacancy (vac) and ceD volume (cv) contributions are included.

0.3 ...-----------------,

0.2

0.1

-0.1

0.0

\~. ________ _/) tot :

-0.2

-0.3 vac

•0.4

'

-.

' ' '

-0.5 L..-~----'--~--'-~-L_~--L-~....J

0.0 0.2 0.4 0.6 0.8 1.0

Wpa

Fig.6.4 Computed total excess volume (tot) vs. composition for PS(M=600 kg/mol)/CH at UCST

at 300 bar. Vacancy (vac) and cell volume (cv) contributions are included.

Thermodynamic Excess Functions 103

upon mixing. A second effect is the change of the cell size relative to the cell

volumes of the pure components. In the case v AB * is. smaller than the average

value of v A* and v8 * there will be a contribution leading to a volume contraction ·

of the total system whereas an increase favours an expansion upon mixing.

These two theoretical contributions (vacancy (VAC) and cell volume (CV)) to

the total excess volume are presented in fig.6.2, 6.3 and 6.4. The cell volume

change leads to a volume expansion upon mixing which is logical from the values

of the volumetric parameters (v A* ,v8 * and v AB *). This effect however is

overruled by the vacancy contribution. The number .of vacancies decreases after

mixing leading to a volume contraction. This effect is larger than the e~ion

caused by the change in cell size and overall a contraction of the system is

predicted. Increasing pressure pas hardly any effect on the cell volume

contribution but the vacancy effect is very sensitive to pressure. The vacancy

contribution becomes less negative with pressure which means that increasing

pressure reduces the. number of vacancies in the mixture in a less pronounced

way relative to the pure components. The sum of the two effects, as described

above, leads to the total excess volume of the system. The ex~ss cell volume

contribution to the excess volume is a convex function (in this study defitled by

a function with a negative second derivative) for the investigated pressure region

whereas the vacancy part is of the concave type (positive second derivative).

Because of the asymmetry of these two types with respect to each other, the sum

of these two contributions does not necessarily lead to a uniformally curved

function over the total composition range. This effect is illustrated by fig.6.2, 6.3

and 6.4. The total excess volume is concave at 1 bar but a change to a convex

form at low polymer concentration is observed with increasing pressure due to

the smaller effect of the vacancy contribution. Because the critical composition

is located in this composition regime, this change leads to a change of sign of

(8T/8p)c with pressure. This is in contrast with the suggestion of Saeki et al [73].

They proposed that the change of sign of (aT I ap )c with molar mass is related to

a change of sign of the value for the excess volume instead of a change of sign

of the curvature of this function.

104 Chapter 6

The interplay between changes in the number of vacancies and cell volume upon

mixing is essential for the SS and HH theories and clearly sets these theories

apart from other equation of state theories. In these other theories only one free

volume mechanism is operational. In the vacancy models only changes in the

number· of vacancies are responsible for volume changes and in the cell models

variations in cell size are responsible for this effect. In general the SS and HH

theories incorporate both effects which makes them powerful in the study of

demixing phenomena.

In the following paragraph detailed experimental excess volumes are presented.

The model predictions concerning the excess volume will be compared to these

experimental data.

'-2.1 Confrontation of 'lbeol'): with Experbnental Exeess Volumes

Extensive dilatometric measurements on the system PS/CH have been

performed by Wolf et al [84] under atmospheric conditions. Wolf used four PS

samples with molar masses 0.6, 37, 110 and 670 kg/mole and measured the

specific volume of the solutions at different temperatures. The corresponding

excess volumes are computed making use of the following relation :

(6.9)

with Xpg and XCH the base mole fraction of PS. and CH respectively and v exc•

vmixt, Vpg and vCH the excess volume, the specific volume of the mixture and of

the pure components expressed in m3 per base mole. In the temperature regime

in which Wolf performed the measurements ( 285-310 K) PS with molar mass

37, 110 and 670 kg/mole is in the glassy state. Thus the equilibrium specific

volume vpg for these samples in this temperature regime is not experimentally

accessible and has to be extrapolated from equilibrium volume information

above Tg. Wolf used a quadratic temperature relation as proposed by Hocker

[75] for this extrapolation procedure. In our computations we do not use this

relation but we extrapolate the equilibrium specific volumes using the equation

Thermodynamic Excess Functions 105

of state according to the HH theory for reasons of consistency and theoretical

reliability. Wolf specifies values for excess volumes and not the measured

specific volumes. From these excess volumes we computed specific volumes using ·

relation 6.9 and the extrapolation procedure of Hocker. These specific volumes

are actually measured by Wolf. Relation 6.9 and vpg, extrapolated according to

the HH theory, serve to compute excess volumes which are to be confronted

with the theory. These excess volumes, together with the theoretically predicted

ones are listed in table 6.1 for PS/CH solutions, differing in molar mass of PS,

at several temperatures. Note that the experimental excess volumes for the

PS(M=0.6 kgjmole)/CH solutions are not obtained by any extrapolation

procedure because PS with such a low molar mass is not in the glassy state at

the indicated temperatures. The theoretical volumes are computed with pure

component parameters and cross interactions parameters equal to those used in

the phase equilibrium computations. It should be noted that for such low molar

masses one may expect end-groups to have appreciable effects. Consequently the

molecular parameters estimated from high molar mass PS are not the best

choise. Let us for the moment focus on the experimental excess volume curves

and especially on their curvatures which are so important for pressure influence 0.00 lf-I .. Jiji;;;:=-----~="

-0.20 0.6 -G)

0 E ..... -0.40 .. E -i

-0.60 > • 0 .,..

-0.80

-1.00 0.00 0.50 1.00 Weight fraction PS

Flg.6.5 Experimental excess volume vs. composition [84] for different PS/CH solutions under

isothermal conditions. Molar mass PS is indicated in kg/mol.

106 Chapter 6

on the phase equilibria. In fig.6.5 experimental excess volumes are displayed at

isothermal conditions. An analysis of the data shows that in the low polymer

composition range the excess volume - composition curve is convex when the PS

molar mass equals 0.6 kg/mole. The curvature of the other molar mass solutions

is hard to access because of the scatter of the data. The results of Saeki [73]

indicate that (8T/8p)c becomes approximately zero for a PS molar mass of

approximately 110 kg/mole. So for this molar mass a change of local curvature

should occur. The local convex curvature for the PS(M=0.6 kg/mole), as

observed by Wolf, is in agreement with the positive value of (aT f ap )c in this low

PS molar mass range, see relation 6.3 and the enthalpic condition for UCST as

described in paragraph 6.1. A change of curvature of the excess volume for

higher molar masses, as is indicated by the theory and by the data of Saeki [73],

can not be decided from the excess volume measurements of Wolf.

So far we have concentrated on the curvature but how does theory predict the

absolute value of the excess volume ? Figs.6.6, 6.7, 6.8 and 6.9 show that the HH

theory generates excess volumes which are approximately a factor ten too small

in comparison with experimental results. Thus having established the cross

parameters from the consolute state at a liquid-liquid demixing curve, the theory

is not capable to generate excess volumes which are in reasonable agreement

with theory. This is clearly a shortcoming of the model. Note that also the effect

of temperature on the excess volume is predicted in an unsatisfactory way.

According to experimental data the excess volume becomes less negative with

increasing temperature whereas the theory suggests an opposite effect. In

studying this effect however we are probing the equation of state behaviour in

a very detailed manner. We are comparing theoretical and experimental

expansion differences in the order of 0.0002 cm3 fgK. It is clear that a subtle

interplay between the expansion coefficients of the pure components and of the

mixture is involved. A detailed study of this temperature effect is hindered

because experimental information about the expansion coefficient of PS in this

temperature region is missing. With the set of mixing parameters determined

from liquid-liquid demixing information, it is clear that also this observed

Thermodynamic Excess Functions

-<D 0 e .... .. e -

II • > • 0 ....

0.00

-0.20

-0.40

-0.60

-0.80

-1.00 0.00 0.10

Weight fraction PS

107

0.20

Fig.ti.ti Experimental ( •) and predicted excess volume according to the SS and HH theories vs.

composition for the system PS(M=37 kg/mol)/CH at 12.47, 21.72 and 28.32 •c.

-<D 0 e .... .. e -

= > • 0 ....

0.20 .----------....., >T S

• ' • • • l I It I i i 1 i i ~ ; \ 1 i ':, : i ~ : : : : : ~ : 0.00 .,.....,_,:,_:.:_.;.;.. __ ,...-_-..,-..,-===___;1_-"=_:::_:::_s:_:::: ___ :::-l

>T HH -0.20

-0.40

-0.60

-0.80

-1.00 0.00 0.10 0.20

Weight fraction PS

Fig.ti.7 Experimental (•) and predicted excess volume according to the SS and HH theories vs.

composition for the system PS(M= 110 kg/mol)/CH at 21.72, 28.32 and 33.303 •c.

108 Chapter 6

0.20 >T

0.00 ··"""'"'n;~,;;;;;;;;;;,,,, ----- --""'"' Q)

0 -0.20 E ..... ..

E - -0.40 E

> • -0.60 0 ...

-0.80

-1.00 0.00 0.10 0.20

Weight fraction PS

Flg..6.8 Experimental ( •) and predicted excess volume acrordiDg to the SS and HH theories vs.

composition for the system PS(M=670 kg/moi)/CH at 28.32, 33.30 and 38.30 "C.

0.30 .------------....,

0.20 ..... -Q) ss 0 E ..... 0.10 .. E - . ..,...,.,..---- ................... HH

l! • 0.00 .,.,., ....................

> • • 0 - -0.10

-0.2 0 .__..__..__..__.....__...._...._........_........__,__.

0.00 0.50 1.00

Weight fraction PS

Fig.6.9 Experimental ( •) and predicted excess volume according to the SS and HH theories vs.

composition for the system PS(M=0.6 kg/mol)/CH at 28.32 °C.

Thennodynamic Excess Functions 109

temperature effect is not predicted in a satisfactory manner.

So far we have confronted the HH theory with experimental excess volumes but

how good is the original SS theory in predicting these volume effects ? Fig.6.6,

6.7, 6.8 and 6.9 show that the SS theory generates positive excess volumes and

thus not even the proper sign is predicted.

General thermodynamics states that for UCST demixing the factor (82H/8x2)p,T

is negative. This condition is indeed fulfilled for the computed excess enthalpies

according to the SS and HH theory. As an example these enthalpies are

presented in fig.6.10 for the system PS (M=37 kg/mole)/CH. It is not possible

to compare these results with experiment because to our knowledge no excess

enthalpies have been measured for this system.

0.05 .-----------..,...,

0.04

1- 0.03 a: ') :J: 0.02

0.01

0.00 ...,__ _ __. __ _..... __ ......_ __ _,

0.00 0.05 0.10 0.15 0.20

Weight fraction PS

Fig.6.10 Predicted excess enthalpy vs. composition according to the SS and HH theories for the

system PS(M=37 kg/mol)/CH at 12.75, 21.72 and 28.32 •c.

110 Chapter 6

Table 6.1 Excess Volumes for PS/Cl{

Weight fraction PS Exp.V exc,H;!l Theor.V exc,HH

in em /base mol

PS(M=37kg/mol)/CH T=285.90K

.2018 -.8845 -.06181

.1475 -.6422 -.04492

.1250 -.5537 -.03791

.1084 -.4825 -.03275

.0869 -.4303 -.02918

.0758 -.3854 -.02610

PS(M=37kg/mol)/CH T=294.87K

.2023 -.5n1 -.08782

.1886 -.5442 -.08211

.1722 -.4948 -.07520

.1521 -.4361 -.06662

.1255 -.3586 -.05513

.osn -.2601 -.03860

PS(M=37kg/mol)/CH T=301.47K

.2018 -.4626 -.10870

.1820 -.4333 -.09860

.1626 -.3n1 -.08864

.1433 -.3333 -.07853

.1253 -.2903 -.06896

.1011 -.2331 -.05592

.0803 -.1843 -.04457

PS(M = 110kg/mol) /CH T = 294.87K

.1598 -.7341 -.07126

.1328 -.6142 -.05943

.1121 -.5192 -.05027

.0959 -.4405 -.04305

.0852 -.3921 -.03826

.0749 -.3427 -.03364

.0646 -.2922 -.02902

PS(M = 110kg/mol)/CH T=301.47K

.1594 -.6121 -.08840

.1389 -.5472 -.07746

.1233 -.4840 -.06902

.1079 -.4235 -.06060

.0901 -.3523 -.05078

.0746 -.2940 -.04215

.0657 -.2587 -.03718

Thermodynamic Excess Functions 111

PS(M=110kg/moi)/CH T=306.45K

.1647 -.5784 -.10570

.1428 -.5135 -.09235

.1288 -.4621 -.08368

.1131 -.4056 -.07383

.1007 -.3610 -.06596

.0848 -.3041 -.05579

.0633 -.2371 -.04381

PS(M =670kg/moi)/CH T=301.47K

.0843 -.7649 -.0479

.0717 -.6523 -.04082

.0631 -.5732 -.03598

.0539 -.4895 -.03077

.0470 -.4259 -.02685

.0419 -.3801 -.02395

PS(M=670kg/moi)/CH T=306.45K

.08689 -.5528 -.05749

.0736 -.4742 -.04886

.0641 -.4129 -.04265

.0609 -.3568 -.04055

.0475 -.3042 -.03172

.0402 -.2601 -.02688

.0333 -.2131 -.02230

PS(M=670kg/moi)/CH T=311.45K

.0845 -.4522 -.06444

.0757 -.4089 -.05789

.0662 -.3563 -.05077

.0583 -.3136 -.04482

.0503 -.2712 -.03876

.0431 -.2313 -.03327

.0361 -.1942 -.02792

PS(M = .6kg/moi)/CH

.9260 -.0280 -.005135

.8382 -.0977 -.003774

.7566 -.1239 .002431

.6762 -.1138 .01123

.6032 -.0945 .02012

.5046 -.0706 .03143

.4579 -.0594 .03587

.4049 -.0464 .03976

.3633 -.0411 .04177

.2637 -.0247 .04194

.2242 -.0165 .03989

.1801 -.011 .03600

.1505 -.010 .03237

.1220 -.007 .02808

.0956 -.004 .02336

.0811 -.004 .02046

112 Chapter 6

6.3 The system PS/MeOAc

In this paragraph the pressure influence on UCST phase behaviour for the

solution polystyrene(PS)fmethylacetate(MeOAc) is related to the predicted

excess volume of the system. As already discussed in chapter 5, pressure

enhances the miscibility in the lower pressure regime for all studied molar

masses of PS. At approximately 300 bar (8T/8p)c becomes zero (see fig.5.17).

In fig.6.11 the predicted total excess volume is presented at 1, 100 and 300 bar

for a PS (M=51 kg/mole)/MeOAc solution. The two theoretical contributions

which are responsable for the total volume change upon mixing are also

incorporated. The volume cross parameter v12 * for PS/MeOAc is smaller than

the hard sphere average of the pure component parameters. This implies that

the cell size decreases upon mixing and a negative excess volume contribution

results, see fig.6.11. This negative contribution is only slightly pressure

dependent. The vacancy effect has a much larger impact on the total excess

volume. The change in the number of vacancies upon mixing leads to a relative

large contraction of the system. Increasing pressure reduces the change in the

vacancy-number but also leads to a different effect. On the low polymer

concentration side the curve representing the vacancy contribution is concave at

1 bar (see fig.6.11). An increase in pressure changes the local curvature into a

convex form which has of course consequences for the total excess volume of the

system. This total excess volume is the sum of the two volume effects. In the low

polymer concentration regime, where the critical concentrations are located, the

total excess volume is concave at 1 and 100 bar. At 300 bar however the concave

form of the cell volume contribution and the convex form of the vacancy effect

compensate each other resulting in an almost straight line for the total excess

volume. Thus the second compositional derivative becomes zero leading to an

invariance of pressure on the critical temperature ((8T/8p)c = 0) at 300 bar

which is completely consistent with the miscibility study in chapter 5.

The interplay between vacancy and cell volume contributions for PS/MeOAc is

of a different type as in the case of the solution PS/CH. In the latter case the

Thermodynamic Excess Functions 113

curvature of the individual contributions did not change upon pressurizing but

only the curvature of the sum of these effects changed. For PS/MeOAc we

observe a change in curvature of the individual vacancy effect which results in a

change in the curvature of the total excess volume.

A direct comparison with experimental excess volumes is not possible because

to our knowledge no excess volumes have been measured for this system.

0.00 ,~

" >p ~ ~.. f -? . .,::,

-0.05 • . ..... ____ Iff?

t) ·. · .. ---0

. . . . . . E

-0.10 ..... • E .e -0.15

2 • > -0.20 • 0 ...

-0.25

-0.3 0 L..-. .................. __. _ ____... _ __.. _ _.~

0.00 0.20 0.40 0.60 0.80 1.00

Weight fraction PS

Fig.6.11 Predicted total excess volume(--) for the system PS(51 kgfmol)/MeOAc at the UCST

at 1, 100 and 300 bar. The vacancy(· • ·) and cell volume (- - -) contributions are

included as well.

114 Chapter 6

6.4 Conclusions

In chapter 5 we have demonstrated that the effect of pressure un UCST phase

behaviour of polymer solutions can be very subtle and complex. The system

PS/CH served to illustrate this. In the original literature, presenting these data

[73] for the above system, these subtle changes were correlated with changes of

sign for the excess volume of mixing.

In this chapter we have presented an alternative and original correlation

between the pressure influence on critical temperature demixing and the excess

volume of mixing for this system. According to the HH theory, these subtle

pressure influences are related with changes in the local curvature of the excess

volume and not with a change of sign. This conclusion is supported by

experimental excess volume data of Wolf [84]. The predicted changes of local

curvature is the result of a delicate interplay between the two theoretical types

of volume effects operational in the HH theory.

The absolute values of the excess volumes for this system are not predicted

very well. The HH theory generates values which are approximately a factor ten

too small whereas the SS theory is not even capable in predicting the proper sign

of the excess volume.

Excess volumes for the solution PS/MeOAc are also presented but are not

experimentally verified because to our knowledge no experimental information

is available.

The Flory-Duggins parameter 115

7. The Flory-Duggins Parameter

7.1 Introduction

It is common practice to interpret the miscibility behaviour of multicomponent

polymer systems in terms of the classical Flory-Huggins theory [6-9]. In this

lattice theory the free energy of mixing for a strictly binary solution reads

with N41 the total number of lattice sites, RT has the usual meaning, ~;represents

the volume fraction of component i, s2 is the number of monomer units per

polymer molecule and X the Flory-Huggins parameter. In the original

formulation of the theory, entropic and enthalpic contributions to the free energy

of mixing are strictly separated. The entropic part consists of combinatorial

factors, represented by the first two terms on the right hand side of equation 7.1.

Volume changes are not considered in this theory, thus only changes in internal

energy contribute to the enthalpic factor, i.e. the last term in the right hand side

of eq. 7.1. The x-parameter is a function of temperature only :

(7.2)

with xh a constant expressed in Kelvin.

A comparison based on eq.7.1 and 7.2 with detailed experimental evidence

points out the inadequacy of the Flory-Huggins theory and inspired the

introduction of additional parameters in eq.7.2, parameters which do not always

have a sound theoretical basis but give an improved agreement between

116 Chapter 7

experiment and theory according to eq. 7.1. Inclusion of an extra constant x.:

(7.3)

is a first step towards improvement of this theory but the strict division of

entropic and enthalpic contributions vanishes. The non-combinatorial entropy

parameter x. was introduced first by Flory [8,9] and was viewed by Guggenheim

[85] as a cooperative free energy correction. The molecular basis however is not

defined very clearly.

In an attempt to overcome remaining discrepancies between experiment and

'theoretical' description, the temperature dependence of x has been extended,

additional concentration functions were coupled to this parameter, segment

areas were incorporated and extra empirical parameters have been added [86].

Consequently the x-parameter looses its original simple meaning expressed by

eq. 7.2 and becomes a complex quantity in which many effects are incorporated.

Nevertheless, many physical properties of polymer multicomponent systems are

expressed in terms of the x-parameter. Frequently the Rayleigh ratios obtained

in scattering experiments are expressed in terms of the x-parameter for

scattering, i.e. Xscat related to the second compositional derivative of the free

energy of mixing.

In this chapter isobaric Xsca1-parameters are presented for the system PS/CH

generated with the SS and the HH theory. The different theoretical factors,

which contribute to this x-parameter, will be discussed in detail. Furthermore the

theoretical x-parameter results for this system will be compared to experimental

Xscacparameters determined by Scholte [36-39].

The Flory-Huggins parameter 117

7.2 Definitions for computation of Xscat·parameters

In paragraph 7.3 theoretical x-parameters for dilute and concentrated PS/CH

solutions are confronted with x-parameters determined by Scholte [36-39] from

scattered light intensities. The intensity of scattered light at zero wave vector is

directly related to the second compositional derivative of the Gibbs free energy

of mixing [87]. The results of Scholte are expressed in terms of the Xsm

parameter which is derived from the second compositional derivative of the free

energy of mixing adopting a Flory-Huggins expression. Scholte does not apply

equation 7.1 but starts from the Flory-Huggins free energy expression in terms

of mass fractions, which for a binary solution reads:

(7.4)

with the combinatorial entropy contribution:

(7.5)

AGw is the Gibbs free energy of mixing of M. grams of solution, RT has the

usual meaning, wi stands for the mass fraction of component i and Mi the molar

mass of species i. In differential form equation 7.4 reads :

(7.6)

From the above it follows :

(7.7)

As derived in chapter 2, the Gibbs free energy of the mixture in the framework

118 Chapter 7

•· of the HH theory is expressed per mole lattice sites and reads :

Gm/(N<S>RT) =

'P A/sA ln'Pa + • 'Pa/ Sa ln'Pa

+ (1-y)/y ln(1-y) + ln (y)/ <s>

- (1-<a>y)/('YY) ln(1-<a>y)

- <c.> ln (v* yV (1-71)3)

+ (1-a)y <c.>[A(yV)4 -2B(yVY21/(2(1-ay)T)

+ 3/2 <cfs> ln (2w<Mo>RT/(N8h)2)

+ pV/(RT)

(7.8)

combinatorial (SHH) term

vacancy (V AC) term

Huggins (HUG) term

cell free volume (FV) term

energetic (EO) term

translational energy (TE) term

compressibility factor (Z) term ·

with all symbols defined in chapter 2. In order to be able to apply eq.7.7 we

have to express the theoretical Gibbs free energy of mixing in eq.7.6 per unit

mass:

(7.9)

with <Mo> the average molar mass per segment. By combining eqs. 7.7, 7.8

and 7.9 we are able to compute theoretical Xscat parameters based on the HH

theory:

= M1a2jaw/ [(SHH- SFH) + VAC +HUG+ FV +EO+ TE + Z]

According to eq.7.10 one is able to systematically investigate the contribution of

the curvature of each individual term to the total curvature of the Gibbs free

The Flory-Huggins parameter 119

energy of mixing with respect to composition. It is this curvature which

determines the miscibility behaviour of the system. As already expressed in eq.

7.3 the x-parameter consists of an enthalpic and a non-combinatorial entropic ·

part. For Xscat these contributions are defined by :

Xsnc,scat = a(Txscat)faT (7.11)

(7.12)

with Xscat = XSnc,scat + XH,scat (7.13)

From eq.7.7

(7.14)

it follows that XH,scat = -1/(2T) 82A"-w/itw/ (7.15)

(7.16)

7.3 x ..... and its contributions

The Xscat parameters and all the theoretical contributions are computed for the

system PS(520 kg/mole)JCH. In fig.7.1 Xscat and these terms, generated by the

HH theory, are presented at the UCST-critical composition as a function of

temperature at atmospheric conditions. All theoretical pure component

parameters and mixing parameters are identical to those used in the previous

chapters. At the spinodal, Xscat takes the following value :

120 Chapter 7

(7.17)

The s~nd derivative of the combinatorial entropy SFH is independent of

temperature and is a constant for a given concentration indicated in fig.7.1 by

the straight line for this particular concentration. In the low and high \' (

temperature range we observe that the value of Xscat exceeds the absolute value

of the combinatorial contribution Whereas at intermediate temperatures the

value of Xscat is smaller. One may conclude that at these intermediate

temperatures the system is in the homogeneous or metastable state (see

paragraph 2.9). In the high and low temperature range the system is in the

heterogeneous state. This conclusion is in agreement with the demixing study in

chapter 5. At low temperatures the system exhibits UCST type of demixing, at

high temperatures the system enters the LCST miscibility gap whereas in

between the system is homogeneous.

The total Xscat parameter is the result of the sum of all individual theoretical

terms. From these terms, the combinatorial (SHH and SFH) and the

translational energy (TE) terms are temperature independent whereas HUG

and Z terms are only slightly temperature dependent (see fig.7.1). The TE term

is negative and thus favours the mixing of the system. the combinatorial and the

HUG terms are positive and stimulate the system to demix. At atmospheric

pressure the Z term is almost zero and has a negligible effect on phase

behaviour. The sum of these four terms is a small negative value practically

temperature independent.

The FV, V AC and EO terms vary strongly with temperature and it are

basically these terms which introduce phase separation in the low and high

temperature regions.

Focussing for the moment on the energetic term, we see its value decreases

and changes sign with increasing temperature. From a model point of view, there

are different effects which determine this observed temperature dependence.

This term represents the balance between pure component interactions and cross

interactions. With increasing temperature the number of the pure components

contacts and cross contacts will change but also the energy corresponding to

The Flory-Duggins parameter 121

·-.s:::. 0

1.00

0.50

0.00

-0.50

FV I

-SFH / /

=---- J, // TOT -----------------?·--~

,/' // ,/ / __ ./ .......... "'

:-... ......... ~---- ... ----_...,... .. .....- ,...,.""""' ~·-- ' ____ ..... ~ ------~----;~--------------:::.......-------- ' .~:-:-:-: .................. :--. ............................. .

' " 1-----------------------,-----" \

\

VAC

8HH

HOG

z

TE

t \ EO

SFH

-1.00 280 360

. 440 520

T (K)

Fig.7.1 X, ... parameter and its theoretical contributions versus temperature at the UCST

composition for the system PS(M=520 kg/mol)/CH according to the HH theory

122 Chapter 7

these contacts. Changes in the cell volume are mainly responsible for this latter

effect whereas changes in the number of vacancies determine the number of

total contacts. These are obvious the effects which cause the decrease of the

energetic contribution with increasing temperature.

' Wh'~:~.t are the influences of the free volume and the vacancy term on Xseat ?

The V AC term represents the contribution of mixing vacancies and segments to

the combinatorial entropy in the SS and HH theories (see chapter 2) and the

free volume (FV) term represents the effect on the curvature of the Gibbs free

energy of mixing from the cell partition function. Both terms are positive in the

whole temperature range and increase quasi-exponentially with temperature (see

fig. 7.1). So one can conclude that free volume arguments are responsible for

LCST demixing. This is consistent with the findings of other free volume theories

which lead to a similar conclusion. A unique feature of this theory is that the

total free volume effect finds its origin in two separate free volume contributions

whereas in other free volume theories only one free volume mechanism causes

LCST demixing.

As discussed before, the Xscat parameter consists of an enthalpic and an

entropic part which are presented in fig.7.2. The total entropic contribution to

the curvature of the Gibbs free energy of mixing also includes the FH

combinatorial entropy term, represented by the thick straight line. The total

entropic term is positive at high temperatures and becomes negative at low

temperatures. So there is one temperature at which the total entropic term

equals zero, in this case at approximately 420K. From the above it is clear that

entropic effects induce LCST~type of demixing.

An opposing effect forms the enthalpic contribution which is positive at low

temperatures and becomes negative at elevated temperatures (see fig.7.2). Thus

it are enthalpic driving forces which cause UCST demixing.

As already discussed in chapter 5, the following conditions have to be fulfilled

(7.18)

LCST: (7.19)

The Flory-Huggins parameter 123

0.50

-1.00 l,..o...o.~~ .................................... ~~ ...........

280 360 440 520

T (K)

Fig.7.2 Enthalpic (H) and entropic (S) contributions to the Xsca, parameter versus temperature at

UCST-composition for the system PS (M=520 kg/moi)/CH system according to the HH

theory. The straight line represents the FH combinatorial entropy term.

From equations 7.13 and 7.14 and fig.7.2 it follows that these conditions are

indeed fulfilled.

In fig.7.3 the computed Xscat parameter is presented as generated by the SS

and HH theory respectively for the PS(520 kg/mole)/CH solution again at the

UCST composition whereas in fig.7.4 the contributions to the SS Xscat are

displayed. The SS and HH Xscat parameters are equal at the UCST (in this case

301.15K). This is logical because it is this critical point that is fitted in order to

quantify the values of the two mixing parameters in both theories. Furthermore

in comparison with HH the SS Xscat function has a smaller temperature slope in

between UCST and LCST but reaches larger values at elevated temperatures.

This implies that LCST phase behaviour is shifted towards lower temperatures

and this is exactly what the phase behaviour computations indicate (see chapter

5). A comparison of the individual contributions to the total Xscat function for the

124 Chapter 7

SS and HH theories learns:

1. The 'energetic (EO) contribution takes lower values in the SS theory.

2. The .free volume (FV) term however has increased in the SS theory.

3. The HUG term vanishes in the SS theory. ' :-.: -

4. All other contributions do not change significantly.

The effects summarized in remarks 1-3 cause the x parameter according to the

SS theory to be less temperature dependent. This will be discussed in

comparison with experimental results in the next paragraph.

0.55 HH -SFH ------------

6 0.50

0.45

0.40 ........ ~ ............................................. ~ ...................

280 360 440 520

T (K)

Fig.7.3 X..,.. parameter versus temperature according to the HH and SS theories at the UCST

composition for tbe system PS(M=520 kg/moi)/CH. Straight line represents the FH

combinatorial entropy.

The Flory-Huggins parameter 125

:c 0

1.00

1-

/ /

-SFH //

FV

0.50 r-------*--~-:._·~· ~TOT ---·- // VAC

0.00

-- / ~-------· / // __ ,..

~ ~~""

-~-~-----------~~~---------- SHH ......... ----....... --,________ ' PV&:

~-----------'~~--------------~ ', HOG

' " lr--------------------~--------'\

'\

TE

-0.50 ~--------------------\~--~ \

-1.00 280

t SFH

I

360

T (K)

I

440

\

\ \ EO

\

520

Fig.7.4 X.,., parameter and its theoretical contributions versus temperature at the UCST·

composition for the system PS.(M=520 kg/mol)/CH according to the SS theory

126 Chapter 7

7.4 Comparison of theoretical x-·values with experiment

Scholte [36-39] performed light scattering experiments on solutions of three

polystyrene samples in cyclohexane in the homogeneous state. These PS samples

are listed in table 7.1 and are the same as used for the miscibility studies. The

studied concentration and temperature ranges are listed in table 7.2 for each

solution. The temperatures in all cases remain lK above the corresponding

UCST.

Table 7.1 Molar mass characteristics of the PS samples

Sample

PSI

PS2

PS3

M,.in kg/mol

51

163

520

M,./M.

1.04

1.06

1.19

For the interpretation of the scattering results Scholte starts from the Flory

Huggins expression for the Gibbs free energy of mixing expressed in terms of

mass fractions, viz. by eq. 7.4. In differential form this Flory-Huggins expression

reads:

(7.20)

with Ap1 the chemical potential of the solvent in solution minus the chemical

potential of pure solvent. The Rayleigh ratios are inversely proportional to

82AGw/8WZ and can be related to 8(Xp.)/8w2• Numerical intergration as a function

of composition gives the desired value for Ap1 and defines according to eq.7.20

the value for Xv.· In our computations we are interested in Xscat which is computed

from the tabulated data for xll by numerical differentiation according to:

The Flory-Huggins parameter 127

(7.21)

Table 7.2 Composition- and temperature ranges of the light scattering studies on PS/CH

Solution T- range inK Composition range in wPS

PS 1/CH 290.55 - 338.15 0.02-0.30

PS2/CH 298.15 - 338.15 0.02-0.20

PS3/CH 301.35 - 338.15 0.02- 0.10 .

These values are plotted in fig.7.5 - 7.10 for the. three PS/CH solutions as a

function of reciprocal temperature. The theoretical SS and HH Xseat values are

represented by full lines in these figures. In the proximity of the respective

critical points computed and experimental Xscat values are in close agreement as

expected. The values of the Xseat parameters at other compositions in the low

temperature range are predicted quite accurately. The prediction of the

temperature dependence of the Xscat values is less satisfactory. Both theories

predict a too large temperature dependence which is most pronounced for the

HH theory. It was already noticed in the previous paragraph that the HH and

SS theories predict a different slope of Xscat versus temperature. These

diiferences are of course also. observed in the comparison with experimental

data. Therefore from the limited temperature range considered in the Xscat data,

one could conclude that the SS theory gives a slightly better prediction.

However, from the phase diagrams it was shown clearly that HH gives a better

prediction of the overall temperature dependencies judged from the location of

LCST relative to UCST phase behaviour. Although the composition dependence

of the Xscat parameter is predicted reasonably, some care has to be exercized.

Especially for the dilute concentrations one should realize that the extraction of

the Xscat parameter from the experimental Rayleigh ratio is in principle not

128 Chapter 7

0.56 0.10

0.08 0.54

0.06

:c 0.04 0 0.52

0.02

0.50

0.48 ...._ _________ ......... ___ __.

2.90 3.10 3.30 3.50

1000/T (1/K)

Flg.7 .5 Experimental X- parameters ( •) and theoretical values (--) acwrdiug to the HH theory

versus temperature for the system PS(M=520 kgfmol)/CH at indicated weight fractions PS ·

0.56 .....------------.

0.54

6 0.52

0.50

0.48 2.90

0.10

0.08

0.06

0.04

0.02

3.10 3.30 3.50

1 000/T (1/K)

Fig.7.6 Experimental X .... parameters ( •) and theoretical values (--) according to the SS theory

versus temperature for the system PS(M=520 kg/mol)/CH at indicated weight fractions PS

The Flory-Duggins parameter 129

0.62

• 0.20 0.60 / 0.15 0.58

0.56 0.10 :c 0.08 ()

0.54

0.52

0.50

0.48 2.90 3.10 3.30 3.50

1000/T (1/K)

Fig.7.7 Experimental X,.,., parameters ( •) and theoretical values(--) according to the HH theory

versus temperature for the system PS(M = 166 kg/mol)/CH at indicated weight fractions PS

0.62

:.c 0

0.60

0.58

0.56

0.54

0.62

0.50

• 0.20 ~

~0.15

0.10

- ~0.08

~~:~: ~0.02

0.48 ...._ ____ ......._ __ __._ __ ___,~

2.90 3.10 3.30 3.50

1 000/T ( 1/K)

Fig.7 .8 Experimental X- parameters ( •) and theoretical values (--) according to the SS theory

versus temperature for the system PS(M = 166 kg/moi)/CH at indicated weight fractions PS

130 . Chapter 7

0.68 .-------------, 0.30

• 0.64

0.60

0.56

0.52

/0.20

~0.1&

~i~i! ~0.02

0.48 ,___.....__.____..._,___.....__.____.____,

2.90 3.10 3.30 3.50 3.70

1 000/T (1/1()

Flc-7.9 Experimental X- parameters ( •) and theoretical values(--) aecordi.ng to the HH theory

versus temperature for the system PS(M=51 kgfmol)/CH at indicated weight fractioos PS ·

o.68 .----=-----~o=-.-=-3-=-o__, •

• 0.64

~ 0.20

0.60

~ 0.15

:c 0

0.10 0.56

~ 0.08 0.06 0.04

0.52 ~ 0.02

0.4 8 '---~----'----'----''--~----'--~---'

2.90 3.10 3.30 3.50 3.70

1 000/T (1/K)

Flg.7.10 Experimental X..,., parameters ( •) and theoretical values according to the SS theory

versus temperature for the system PS(M =51 kg/mol)/CH at indicated weight fractious PS

The Flory-Huggins parameter 131

feasible any more. In this composition regime, excluded volume effects become

important and the simple interpretation in terms of a mean field x parameter

becomes unwarranted. The second virial coefficient and consequently the x parameter are also dependent on the polymer coil dimensions. It has been shown

by the bridging concept [88] that these dilute solution effects can extend to

considerable concentrations. This makes the exact interpretation of the

experimental results impossible because exact relations are unknown.

7.5 Conclusions

X parameters can be computed according to the SS and HH theory. Different

theoretical contributions to these parameters can be studied seperately and for

some contributions molecular backgrounds are suggested. However, the xanalysis does not give new basic results for the interpretation of phase behaviour.

The enthalpic and entropic contributions have been exposed clearly.

Predicted x parameter curves are compared with experimental information for

the system PS/CH. These curves are in reasonable agreement. Care has to be

exerted in the dilute composition regime because of excluded volume effects.

132 Chapter 7

133

Polymer Blend Section

134

Phase Behaviour

8. Phase behaviour : Influence of Pressure,

Temperature, Composition and, Molar Mass

8.1 Introduction

135

For polymer solutions a wealth of experimental information is available

concerning true thermodynamic phase diagrams, pressure influence on these

phase diagrams and pure component equilibrium equation of state data. For high

molar mass polymer mixtures, i.e. polymer blends, the situation is , different.

Unfortunately, most phase diagrams for blends are not true thermodynamic

phase diagrams since they are derived from e.g. DSC-experiments, dynamical

mechanical data etc. Reliable phase diagrams however can be constructed

making use of the neutron scattering technique [89-93). Because of contrast

enhancement a certain amount of protons in either of the polymer constituents

has to be substituted by deuterium. Unfortunately a change of the phase diagram

is to be expected due to this deuterium incorporation. Recently also fluorescence

experiments from which spinodal data can be obtained have been published [94].

In this case the polymer molecules have to be labelled with fluorescent probes.

A low probe concentration suffices but the probe molecules are rather bulky and

also here a shift of the "unlabelled" phase diagram is to be expected.

Studies of the influence of pressure on phase behaviour for polymer blends

are extremely scarce. To our knowledge only two systematic studies have been

devoted to this subject. Suzuki and co-workers studied the pressure dependence

of cloud point curves of the blend poly( ethylacrylate )PEA I poly(vinylidenefluoride) PVDF [95]. They came to the remarkable conclusion

that depending on blend composition pressure either improves or diminishes the

miscibility for this blend. Walsh and Rostami [96] investigated the blend

chlorinated polyethylene- ethylene vinylacetate copolymer. They observed that

136 Chapter 8

miscibility is enhanced with pressure, i.e. the LCST cloud points shift towards

higher temperatures.

From the above it is clear that a detailed study of polymer blends is hindered

by a lack of accurate experimental information. For this reason the SS and HH

theories are in first instance tested for a hypothetical model blend. Furthermore

the HH theory is confronted with phase behaviour of the blend polystyrene(PS)

/ poly(paramethylstyrene) PpMeS [40].

8..2 Model Computations for a Hypothetical Blend

In the following paragraph the miscibility behaviour according to the SS and

HH theory for a hypothetical binary polymer blend is discussed. The pure

component parameters are given realistic values and are shown in table 3.6. The

semi-flexibility rule 3c=s+3 is adopted. The value of the cross segmental

repulsive volume is taken constant and equal to the hard sphere average. The

influence on the phase behaviour of e.g. chain length, temperature, pressure,

composition and molecular cross parameters can be computed now.

For a blend of oligomers in which both components have a molar mass of 5

kg/mole (sa = s., = 100) the spinodal curves for different values of the cross

interaction energy ratio X are shown in fig.8.1. The SS theory predicts UCST

phase behaviour. Upon increase of the parameter X the miscibility improves as

expected. A value larger than unity for the parameter X indicates that the

maximum attraction energy between A-B contacts is more favourable compared

to the pure dispersive interaction of A-A and B-B contacts. If the molar masses

of the pure constituents are increased to 6.5 kg/mole (sA= 5s = 130, see fig.8.2)

the cross interaction parameter X must become larger in order to induce

miscibility in the temperature window considered in this figure. Besides UCST

phase behaviour in the low temperature regime the system also exhibits LCST

phase demixing at higher temperatures. Note that these temperatures are not

·realistic for a real polymer system and only serve to demonstrate a possible

coexistence of UCST and LCST. If the cross interaction becomes less favourable

the UCST and LCST spinodals merge resulting in a hour glass shaped

Phase Behaviour

600 X

T(K)

400

200

0

Fig.8.1 Predicted spinodals for a hypothetical oligomer model blend with molar masses of

both constituents 5 kg/mol. The energetic cross parameter X is indicated.

800

T (K)

500

200

0 0.5

Fig.8.2 Predicted spinodals for a hypothetical oligomer model blend with molar masses of

both constituents 6.5 kg/mol. The energetic cross parameter X is indicated.

137

138

600

T(K)

400

200

0 0.5

1.002 1.000

Chapter 8

Fig.8.3 Predicted spinodals for a hypothetical model blend with molar masses of both constituents

50 kg/mol. The energetic cross parameter X is indicated.

600

T(K)

400

200 0 0.5

Fig.8.4 Predicted spinodals for a hypothetical model blend with molar mass of component 1

50 kg/mol, molar mass of component 2 is indicated. The energetic mixing parameter

equals 1.003.

Phase Behaviour 139

immiscibility region. Upon a further increase of the molar masses of both

components an even larger value of the X-parameter is required to induce

miscibility. Consequently the UCST curve shifts to lower temperatures and

eventually disappears because, from an interactional point of view, the system

is prone to mix. Thus for higher molar mass systems LCST phase behaviour is

more likely to be observed. In fig.8.4 the influence of changing molar mass on

the phase diagrams is depicted at constant cross interaction energy. As expected

an increase in molar mass results in a decreased miscibility. Furthermore an

enhanced asymmetry in the relative chain lengths is reflected in an enhanced

asymmetry of the spinodal curves.

The existence of the LCST demixing curve in fig.8.4 is related to differences

in equation of state properties of the pure components. In the SS theory this

difference can be discussed in terms of differences in lattice free volume. The

influence of pressure on the LCST phase diagram is shown in fig.8.5. Upon

increasing the pressure one can expect to reduce the mismatch between the

600

T (K)

500

L.OO

0 05

Fig.8.S Pressure influence on the spinodal for a hypothetical model blend with molar masses

of the pure constituents 50 kg/mol. The energetic cross parameter X equals 1.003. The

pressure is indicated in bar.

140 Chapter 8

component free volumes and consequently an improved miscibility may be

anticipated. For solutions of PE in n-hexane it has been shown previously that

the pressure dependence of the miscibility is governed by an iso-site free volume

condition at the consolute state. In the absence of cell size changes (Y = 1),

whkh is the case for the computations shown in fig.8.5, an iso-condition is

applicable. In table 8.1 the difference in site free volume at the critical

coordinates is shown as a function of pressure. Covering a substantial pressure

range the difference (y8-yA) remains constant to a very good approximation.

Table 8.1 Free volume difference at LCST-conditions as computed by the SS-theory

p (bar) T (K) 100*(Yo-Y.J

1 425.61 2.406

10 427.58 2.409

50 436.49 2.420

100 447.57 2.434

500 552.57 2.535

Thus critical demixing sets in at a given value of the free volume difference. This

is a clear demonstration that LCST demixing is to a great extend governed by

differences in free volume. The exact value of (y8 -y A) however is not universal

but depends on the specific system and the specific molar mass combination. As

expected the SS theory accounts for the major molecular characteristics which

are now generally accepted to be responsible for the phase behaviour of polymer

systems excluding orientation dependent interactions.

The HH theory produces similar phase behaviour when the same molecular

parameters are adopted. As discussed already in chapter 3, the PVT-behaviour

of the pure components is modelled differently in the concept of the HH theory

in comparison with the SS model. This has consequences for the computed

spinodal curves which are shifted in temperature in the order of 10-50 Kelvin

Phase Behaviour 141

whereas the shift in composition is very small. Because no new effects are

observed the spinodals which are generated by the HH theory are not presented.

A better understanding of more complicated phase behaviour can be obtained

with the SS or the HH theory. For example, the predicted influence of pressure

is not always as simple as shown in fig.8.5. So far, we have assumed that hard

core segmental volume parameters v A*, vB * and v AB * are equal. In fig.8.6 the

calculated LCST using the HH theory is shown as a function of pressure. In this

case it is assumed that the segmental hard core volume v12 * is not equal to the

hard sphere average but is slightly larger (Y = 1.002). Differences arising in the

cell volume can be attributed to differences in packing efficiencies of segments

involved in homo (A-A and B-B) and hetero (A-B) contacts respectively. Here

an essentially new feature can be observed. For the parameters chosen the

miscibility increases at first in accordance with free volume concepts but at high

pressures the miscibility decreases. aearly the pressure dependence of miscibility

407

:.:: .s 406 ~

405

404 ~~~~~~~~~~ 0 50 100 150 200 250

P in bar

Fig.8.6 Lower critical solution temperature versus pressure for a hypothetical model blend. Molar

masses of both constituents equal 50 kg/mol. X= 1.00285, Y = 1.002.

142 Chapter 8

Table S.Z Free volume difference at LCST -conditions as computed by the SS-theory

p (bar) T(K) 100*(y8-y.J

1 404.651 1.849

20 405.183 1.838

40 405.666 1.826

60 406.071 1.813

80 406.395 1.801

100 406.637 1.788

120 406.798 1.775

140 406.874 1.762

160 406.866 1.749

180 406.m 1.735

200 406.594 1.722

220 406.329 1.707

240 405.976 1.692

does not obey the iso-site free volume condition since the free volume difference

of the pure components changes monotonically with pressure. The free volume

difference (y8 -yA) for this system is summarized in table 8.2. With increasing

pressure (y8-yA) systematically becomes smaller indicating that the demixing sets

in at an earlier stage than anticipated from the iso-free volume concept. The iso

free volume concept assumes that the demixing is completely governed by the

site fraction free volume. Just as in the case of the presented polymer solutions,

also changes in the cell volume have their influence on critical demixing

phenomena. In the following chapter on excess functions these two effects, which

both determine the volume change upon mixing, will be studied in more detail

and also the link to phase behaviour will be considered.

We have demonstrated in the previous chapters that such a non-monotonic

pressure dependence on phase behaviour is not uncommon for polymer

solutions. Also for polymer blends there is some evidence that the pressure

Phase Behaviour 143

dependence can be quite complicated. As already presented in paragraph 8.1

Suzuki et al. [95] measured the pressure influence on cloud point curves of the

blend PEA-PVDF. They observed a remarkable tilting effect of these curves with

pressure (see fig.8.7) which means that depending on blend composition

miscibility either improves or decreases.

For the molecular parameters shown in table 3.6 the spinodal curves at two

indicated pressures are drawn in fig.8.8. Oearly the HH but also the SS theories

are able to predict a similar tilting effect of the demixing curves with pressure

as observed by Suzuki et al. One should note however that the computations

indicate a tilting of spinodal curves whereas the experimental information reports

a tilting of cloud point curves. It is not possible to compute the phase behaviour

of the system PEA/PVDF because, to our knowledge, no equilibrium equation

of state data are available for the pure constituents of this blend.

.5

520 r------------,

500

480

460

440

\ \

-....=-., _..-*"

p In bar

600 ..,. ..... __

...... ----- ' ... 400

1

4 2 0 L...-_..___..__ ___ ,_____,,_____J

0.00 0.20 0.40 0.60 0.80 1.00

Weight fraction PVOF

Fig.8.7 Influence of pressure on cloud point curves for the system PEA/PVDF [95].

144 Chapter 8

450

440

::.::: 430

.5 1-

420

410

400 0.1 0.3 0.5 0.7

Weight frection comp.2

Fig.8.8 Computed spinodals at two pressures for a hypothetical model blend. Molar masses of the

pure constituents equal 50 kg/mol. X= 1.00285, Y = 1.002.

8.3 Phase behaviour of the System PS/PpMeS

8.3.1 Introduction

In this paragraph the miscibility behaviour of the blend polystyrene(PS) /

poly(paramethylstyrene )(PpMeS) is studied on an experimental and theoretical

basis (40]. This blend was selected because it can be considered free of specific

interactions and the pure components are easily synthesized anionically with a

narrow molar mass distribution thus excluding polydispersity effects.

Unfortunately however PS and PpMeS are from a physical and chemical point

of view very similar. This complicates the experimental detection of phase

behaviour in this system.

Phase Behaviour 145

8.3.2 Experimental

Materials

PS was obtained from Pressure Chemical Company. PpMeS was synthesized

by anionic polymerization under argon. The distilled and dried monomer was

polymerized in toluene at 60 oc using the initiator n-butyllithium. After two

hours the reaction was terminated by adding 2-propanol to the solution. The

product was precipitated in 2-propanol and dried for 15 hours under vacuum.

Blend Preparation

PS and PpMeS were dissolved in toluene (0.5 wt%) at room temperature.

After stirring the solutions for 15 hours the solvent was evaporated to produce

films with a typical thickness of 80 pm. The films were dried under vacuum for

several days above T g- The molar mass characteristics of the blends are shown

in table 8.3.

Table 8.3 Molar ma5s characteristics of the blend components as measured by GPC calibrated

against PS-standards

Blend . M,_ps(kgfmol) M,.PpMeS(kg/mol)

1 37 133

2 50 133

3 50 44

4 110 44

TGA-measurements

The solvent content of the film was checked by thermo-gravimetric analysis

(Perkin Elmer TGA 7). A maximum weight reduction of 0.3% is observed before

the blend reaches its degradation temperature.

146 Chapter 8

0.70

0.60

- 0.50

~ 0.40

~ 0 ;:: .. 0.30 • 4) %

0.20

0.10

o.oo 370 380 390 400

Temperature IK)

FicJ13 Thermogram of a homogeneous PS/PpMeS blend

0.60

- 0.50 ~ E - 0.40 ~ .2 -- 0.30 • 4) %

0.20

0.10

0.00 L..-__ _.__....._ ........ _.....____.

370 380 390 400

Temperature IK)

Fig.S.lO Thermogram of a heterogeneous PS/PpMeS blend

Phase Behaviour 147

Experimental Determination of Miscibility

The state of miscibility of ihe blends was studied by Differential Scanning ·

Calorimetry (DSC) and Phase Contrast Optical Microscopy.

All Differential Scanning Calorimetry (DSC) measurements were performed

on a Perkin-Elmer DSC-7 system calibrated against Zn and In. Sample sizes

were approximately 5 mg. After annealing at a certain temperature, the samples

were quenched below T g- Subsequently a temperature run was performed with

a typical scan speed of 20 K/min and the blend was annealed at a different

temperature. This cycle was repeated several times varying the annealing

temperature between Tg and the degradation temperature of the blend. This

procedure was applied to PS/PpMeS blends with different compositions and

different molar masses of the pure components. As a criterion of miscibility we

used the appearance of one or two discontinuities in the DCS thermogram after

annealing for several hours at a certain temperature. Figs.8.9 and 8.10 illustrate

examples of thermograms for a homogeneous and a heterogeneous system.

The ·phase contrast optical microscopy technique was used to detect phase

separation because standard optical microscopy was not applicable due to the

small difference in refractive index of the two homopolymers. The temperature

program used in the DSC experiments was used in the microscopy experiments

as well.

8.3.3 Experimental Results

DSC and phase contrast microscopy techniques were used to determine the

state of miscibility of the blends mentioned in table 8.3. For the blends 1 and 2

we clearly observe a reversible transition from a heterogeneous to a

homogeneous phase region with increasing temperature and vice versa. In Figs.

8.11-8.14 the results of the DSC- and microscopy experiments are shown

graphically. The two techniques give consistent results. The results indicate

UCST phase behaviour, which is quite exceptional for high molar mass blends.

This kind of phase behaviour is observed frequently for polymer/solvent or

148 Chapter 8

500 .--------------.

• • • • • • • • • • • g 450 • • • • • • • • G) • • .. • ::I .. • • • .. G) • Q.

E G) 400 1-

3 50 L...-.__L......I.__.__.__.__..___..__ol........l

0.00 0.20 0.40 0.60 0.80 1.00

.. Weight fraction PS

Fig.S.ll Phase diagram for a PS(37 kg/mol)/ PpMeS(133 kg/mol) blend. (•) : homogeneous

(0) : heterogeneous (-- -) : TJine (--) :computed spinodal

g 450 G) .. ::I .. • .. G) Q.

E G) 400 1-

3 50 ~....-.__&...-.__.__,__.__....._...__ ..........

0.00 0.20 0.40 0.60 0.80 1.00

Weight fraction PS

Fig.8.12 Phase diagram for a PS(50 kg/mol)/ PpMeS(133 kg/mol) blend. (e) : homogeneous

(0): heterogeneous (-- -): Tr'ine (--):computed spinodal

Phase Behaviour 149

500 ,...-----------,

• • • - • • • ~ 450 -; • • • .. • • ... • • • • Q.

E • • • 400 • • ~

3 50 I...-..,......JI...-L.....__,....__....__,....__.~ ....... ---...~

0.00 0.20 0.40 0.60 0.80 1.00

Weight fraction PS

Fig.8.13 Phase diagram for a PS(SO kg/mol)/ PpMeS(44 kg/mol) blend. (e): homogeneous

(· • ·) : TJine : computed spinodal

500

• • 0 0 0

g 450

• ... 0 :::J ....

i 0

400 ~

3 50 L-L-....__,__....__,__..___........!.J ........ ........J

0.00 0.20 0.40 0.60 0.80 1.00

Weight fraction PS

Fig.8.14 Phase diagram for a PS(llO kg/mol)/ PpMeS(44 kg/mol) blend. (e) :homogeneous

(0): heterogeneous (-- -): TJine (--):computed spinodal

150 Chapter 8

oligomer/oligomer systems but it is rather extraordinary for polymer/polymer

systems. In fact this is one of the very few homopolymer blends known to exhibit

this kind of phase behaviour [97-99].

8.3.4 Theoretical Study of Phase Behaviour

The pure component parameters are listed in table 3.7. For values of the mixing

parameters X and Y extremely close to one (see table 8.4), the miscibility gap

for the system PS 37 /PpMeS 133 (kg/mol.) is predicted in a quantitative way as

Table 8.4 Mixing parameters of the polymer blend PS/PpMeS according to the HH theory against

PS·standards

X y

1.0001731 1.0005239

shown in fig. 8.11. Here the computed spinodal is compared with the

experimental information. The values of the mixing parameters indicate the

intermolecular interactions are indeed dispersive. Therefore the blend obeys

the restrictions inherent in the derivation of the theory.

In order to predict the phase behaviour of blends with different molar mass we

assume all model parameters constant. The predicted spinodals are presented

in figs. 8.12-8.14. The temperature shift of the UCST with changing molar mass

is slightly underestimated by theory. The discrepancy is most pronounced for the

PS 110/PpMeS 44 (kg/mol.) blend.

The PS/PpMeS system shows no LCST type of demixing behaviour

experimentally and a LCST type of spinodal is not predicted with the HH theory,

even not at extremely high and physically unrealistic temperatures. For systems

without specific interactions LCST phase behaviour is governed by equation of

Phase Behaviour 151

state properties of the constituents. LCST demixing will occur only when the

free volume difference of the pure components exceeds a certain value. This has

been shown before for the Simha-Somcynsky theory [29,31] and is also valid for

the HH theory. In fig. 8.15 the occupied site fraction y (free volume fraction = (1-y}) for both components as a function of temperature is plotted at

atmospheric pressure. The free volume difference for both components is

extremely small and increases only slightly with temperature. Consequently the

blend will not phase separate in the indicated temperature range.

UCST type of demixing is controlled by energetic contributions to the free

energy. At low temperatures the energetic cross interactions are apparently not

large enough to overcome the pure component contacts and from a purely

energetic point of view there is no reason for the system to mix. These energetic

contributions can be replaced by enthalpic contributions because of the relative

small value of the pAY term. These latter effects are investiged in the next

chapter.

1.00 ....------------.

PpMeS

0.95

0.90 PS

0.86 ....... _ ........................ _ ........ _......___.

400 460 500 550

Temperature (K)

Fig.8.15 Site free volumes of the pure constituents of the blend PS/PpMeS versus temperature

152 Chapter 8

The HH theory predicts a monotoneous increase of the UCST with pressure,

visualized in fig.8.16. In the next chapter this pressure effect will be discussed in

terms of the excess function of this system.

600

550

500

450

400 L..-........................................................ ......_. .......... ........J

0 200 400 600 800 1 000

p (bar)

Fig.8.16 Influence of pressure on the UCST for the PS(37 kg/mol) / PpMeS(133 kg/mol) blend

Phase Behaviour 153

8.4 Conclusions

Computations concerning miscibility behaviour of model systems indicate that

the SS and the HH theories are capable in describing the general observed

effects encountered in studies of polymer blend miscibility. These effects include

a transition from UCST to LCST miscibility behaviour with increasing molar

mass of the pure constituents. This is a generally observed phenomena; partial

miscible oligomer blends frequently exhibit UCST type of demixing whereas high

molar mass polymer blends generally demix at elevated temperatures (LCST).

A difference in molar masses of the pure constituents is reflected in an

asymmetry of the spinodal curves, which is another generally observed effect.

Just as in the case of the solution PE/n-hexane (see chapter 3) a site-fraction

free volume principle governs the pressure effect on LCST miscibility. This

principle however is only applicable when the other theoretical volume

mechanism, concerning changes in cell volume upon mixing, is not operational.

One of the very rare studies in literature concerning pressure effects on

miscibility of polymer blends, reveals a complicated pressure effect. Cloud points

of the blend PVDF /PEA show a tilting effect with increasing pressure. A similar

tilting effect can be reproduced with the SS and HH theories for a model blend

when both volume mechanisms are incorporated.

The DSC and phase contrast optical microscopy techniques reveal UCST

miscibility behaviour for the system PS/PpMeS which is quite exceptional for a

high molar mass blend. The HH theory predicts this type of phase behaviour.

This blend does not show phase separation at elevated temperatures (LCST)

because of the similarity of the site free volume fractions of both pure

components.

154 Chapter 8

Excess Functions

9. Thermodynamic Excess Functions and

Correlations with Phase Behaviour

9.1 Introduction

155

In this chapter thermodynamic excess functions of polymer blends are studied

but we are not in a position to verify these functions by experiment. Reason is

the scarcity of reliable experimental excess functions reflecting the difficulty of

such measurements for polymer blends. Prerequisites for excess function

measurements are the equilibrium condition and the requirement of

homogeneity which implies that one is limited to a restricted temperature region.

In general this zone is restricted by the glass transition line of the blend at low

temperatures and by a miscibility gap or degradation region at elevated

temperatures. The difficulty of establishing thermodynamic equilibrium is

another problem one is faced with. The kinetics of the inter-diffusion processes

are extremely slow due to the large values of the viscosity of the individual

phases. This hinders an accurate interpretation of the measured excess functions

one is interested in.

In most cases excess enthalpy measurements are performed via indirect ways.

two main approaches have been attempted in literature. In the first, AHm for low

molar mass analogies of the respective polymers are measured and the results

are extrapolated towards polymer blends [100,101]. This method neglects molar

mass and conformational effects on AHm and is therefore somewhat controversial

to use in detailed studies of excess enthalpies of polymer blends. In a second

indirect way, the heats of solution of the blend and its constituents are measured

in a suitable common solvent [102-104]. The excess enthalpy is determined from .

the appropriate Hess' law cycle, see below.

156 Chapter 9

All. A

polymer A + solvent solution A

+ AHB + . polymer B + solvent solution B

l·"· 1 AH,' AH,AB

polymer A + polymer B solution A + B

Scheme 9.1 Hess' law cycle

From this cycle relation 9.1 follows :

Al-JA + AH 8 = AH + AHAB .. "'s s m s (9.1)

Note that AH." is negligible provided that the solutions are sufficiently dilute. This

method is also not very accurate because AHm is relatively small compared to the

other relevant enthalpies involved which may lead to serious errors in AHm.

Excess volume measurements on polymer blends are scarce in literature. One

of the few systems studied is polystyrene (PS) I polyphenyleneoxide (PPO).

Zoller and Hoehn [105] reported specific volumes for this system at room

temperature indicating large negative excess volumes. However these data are

not completely conclusive since they were obtained for the non-equilibrium

glassy state. In the equilibrium molten state large deviations from the prediction

of linear mixing rules are not observed. Simha and Jain [28] studied the excess

volume of this system in the terms of the Simha-Somcynsky theory. A change of

the mixing parameters as a function of concentration was necessary to describe

these volumes in an accurate way.

Wendorff [106,107] performed excess volume measurements in the molten

state on sandwich-packed and intimately powder-mixed blends of

polymethylmethacrylate (PMMA) I polyvinylidenefluoride (PVDF) and of

Excess Functions 157

polyethylacrylate (PEA) I PVDF. He concluded that these systems are

characterized by positive excess volumes and that the absolute magnitudes

amount to about 0.2 - 0.5%.

Tsujita et al [108, 109] performed specific volume measurements on polystyrene

I polyparachlorostyrene and polyvinylchloride I polymethylmethacrylate blends

and on the corresponding pure constituents. They report negative excess volumes

with a maximum absolute magnitude of 1% relative to the specific volume of the

blends. Both research groups of Wendorff and Tsujita only measured the excess

volumes at a few compositions so it is not possible to generate a detailed excess

volume - composition curve.

We have shown above that excess function measurements for polymer blends

are still in a early stage of development and at the moment there are no

experimental data which are accurate enough to check equation 6.3 which links

the second compositional derivative of excess volume and excess enthalpy to the

pressure influence on phase behaviour. In this chapter we present theoretical

excess functions for a hypothetical model blend and for the system polystyrene

(PS) I polyparamethylstyrene (PpMeS). These functions have a purely predictive

character and may challenge other experimentalists to improve these excess

measurements.

9.2 Hypothetical Model Blend

In the previous chapter we have presented the effect of pressure on LeST

phase behaviour for a hypothetical model blend with the cross interaction

parameters X andY equal to 1.00285 and 1.002 respectively (see fig.8.6). At the

critical composition the miscibility is enhanced in the low pressure regime until

approximately 150 bar and beyond this pressure the LCST shifts towards lower

temperatures. With the aid of equation 6.3 we are in a position now to

rationalize this pressure effect in terms of excess functions for this system. The

excess enthalpies at the lower critical solution temperatures are negative and are

of the concave type (see fig.9.1) which is to be expected from general

158 Chapter 9

0.00

-0.10

1-a: -0.20 ")

• ::r: .. -0.30 0 .,...

-0.40

-o.s o L...-......... ~....--o ......... -___,__.__,__.....~

0.00 0.20 0.40 0.60 0.80 1.00

Weight fraction comp.2 Fig.9.1 Predicted excess enthalpy versus composition at UCST for a hypothetical model blend at

indicated pressures in bar. X=i.0285, Y=Ul02.

G)

0 E ..... • E

.s

= > .. 0 -

-0.60 .___...__...__..___..._........,

0.00 0.20 0.40 0.60 0.80 1.00

Weight fraction comp.2

Fig.9.2 Predicted excess volume(--) versus composition at UCST for a hypothetical model blend

at 1, 150 and 250 bar. Vacancy(···) and cell volume(···) contributions are also

included. X= 1.00285, Y = 1.()()2.

Excess Functions 159

thermodynamics (see chapter 6). Fig.9.2 displays excess volumes at the LCST

at three pressures as a function of the weight fraction polystyrene including the

cell- and the vacancy contribution to the total excess volume. The cell

contribution is only slightly pressure dependent, the major effect stems from

the change in the number of vacancies upon mixing. With increasing pressure

this vacancy effect gives less negative contributions to the total excess volume

(see fig.9.2) and ultimately results in a change of sign of the latter. For this

system the excess volume -composition curve seems uniformally curved for all

pressures which implies that a change of sign of the second compositional

derivative of the excess volume is directly caused by a change of sign of the

excess volume itself. Only under those circumstances where the excess volume

is almost zero local curvatures of the excess volume will appear because the

excess volume will not change sign for all compositions simultaneously. However

the situation for this model blend is thus far less complex as the PS/CH case

where changes of local curvature are responsible for the observed pressure

effect. At low pressures both the excess volume and the excess enthalpy are

convex causing a positive (aTjap)c. Beyond approximately 150 bar the excess

volume curve becomes positive and thus concave resulting in a negative value

for the derivative (aTjap)c.

9.3 The System PS / PpMeS

In the previous chapter we have shown that the HH theory predicts a

monotonous increase of the upper critical solution temperature with increasing

pressure (see fig.8.16) for the blend polystyrene (PS) / polyparamethylstyrene

(PpMeS). In this paragraph we study this uncomplicated influence of pressure

in terms of the predicted excess functions for this system. In fig.9.3 and 9.4 the

predicted excess volume and enthalpy are presented at the critical temperatures.

The excess enthalpy function is of a concave type and is not pressure sensitive.

The excess volume however increases slightly with pressure (see fig.9.3) which

means that the second compositional derivative of this function becomes more

160

-c5 e ....... .. e -I

> • • 0 .....

3.00 .-----------,

100 bar 2.50

2.00

1.50

1.00

0.50

0.00 .___..___.____.___.__-....1 0.00 0.20 0.40 0.60 0.80 1.00

Weight fraction PS

Fig.9.3 Predicted excess volume versus composition at UCST for the blend

PS(37 kg/mol)/PpMeS(133 kg/mol) at indicated pressures in bar.

3.00 r-------------. 1 and 100 bar

2.50

I -I -2.00

1-a: ') 1.50 :1:

• 1.00 .. 0 .....

0.50

0.00 L--_.___.____.___..__-....1 0.00 0.20 0.40 0.60 0.80 1.00

Weight fraction PS

Fig.9.4 Predicted excess enthalpy versus composition at UCST for the blend

PS(37 kg/mol)/PpMeS(133 kg/mol) at indicated pressures in bar.

Chapter 9

Excess Functions 161

negative. From eq.6.3 it follows that this leads to a larger value of (aTjap)c with

increasing pressure which is in agreement with fig.8.16.

9.4 Conclusions

The pressure effect on the LCST critical point of a model blend is analyzed

in terms of thermodynamic excess functions. A change of sign of the excess

volume with pressure is the result of the interplay between the two theoretical

volume mechanisms. The excess enthalpy is negative and becomes less negative

with increasing pressure.

The excess volume and enthalpy are both positive and concave for the system

PS/PpMeS.

162 Chapter 9

References 163

10. References

1. Prigogine 1.; Bellemans A.; Mathot V The Molecular Theory of Solutions;

North Holland Publishing Co.:' Amsterdam, 1957

2. Flory P.J.; Otwoll R.A.; Vrij A J.Am.Chem.Soc. 1964, 86, 3567

3. Flory P .J. J.Am.Chem.Soc. 1965, 87, 1833

4. Eichinger B.E.; Flory P .J. Trans.Faraday Soc. 1%8, 65, 2035

5. Flory P .J. Discuss.Faraday Soc. 1970, 49, 7

6. Huggins M.L.lChem.Phys. 1941, 9, 440

7. Huggins M.L Ann.N.Y.Acad.Sci. 1942, 43, 1

8. Flory P J.lChem.Phys. 1941, 9, 660

9. Flory P .J. J.Chem.Phys. 1942, 10, 51

lO.Dee G.T.; Walsh D.J. Macromolecules 1988,21, 811

11. Dee G.T.; Walsh D.J. Macromolecules 1988, 21, 815

12. Kammer H.W.; Inoue T.; Ougizawa T. Polymer 1989, 30, 888

13. Sanchez I.C.; Lacombe R.U.lPhys.Chem. 1976, 3 80, 2352

14. Sanchez I. C.; Lacombe R.T.).lPolym.Sci. Polym.LettEd. 1976, 15, 17

15. Lacombe R.U.; Sanchez I.C.lPhys.Chem. 1976, 80, 2568

16. Panayiotou C.G. Macromolecules 1987, 20, 861

17. Kleintjens LA.; Komngsveld R.J.lElectrochem.Soc. 1980, 121, 2353

18. Kleintjens LA.; Koningsveld R. Colloid Polym.Sci. 1980, 258, 711

19. NiesE.; van der Haegen R. Macromolecules 1988, 21, 2633

20. Simha R.; Somcynsky T. Macromolecules 1969, 2, 341

21. Olabisi 0.; Simha R. Macromolecules 1975, 8, 211

22. Nanda V.S.; Simha R. J.Am.Chem.Soc. 1964, 86, 197

23. Nanda V.S.; Simha R.lChem.Phys. 1964, 68, 3158

24. Quach A.; Simha R. J.AppLPhys. 1971, 42, 4592

25. Simha R.; Wilson P.S. Olabisi 0, Knll.Z.Z.Pol. 1973, 251, 402

26.Jain R.K.; Simha R. Macromolecules 1980, 13, 1501

27. Simha R.; Jain R.K. Colloid Polym.Sci. 1985, 263, 905

28. Jain R.K.; Simha R. lPolyin.Sci. Polym.Phys.Ed. 1982, 20, 1399

164 Chapter 10

29. Jain R.K.; Simha R. Macromolecules 1984, 17, 2663

30. Nies E.; Stroeks A. Macromolecules 1990, 23, 4088

31.Nies E.; Stroeks A.; Simha R.; Jain R.K. Colloid Polym.Sci. 1990, 268, 731

32. Stroeks A.; NiesE. Polym.Eng.Sci. 1988, 23, 1284

33. Stroeks A.; Nies E. Macromolecules 1990, 23, 4092

34. Nies E.; Stroeks A. in "Integration of Polymer Science and Technology-2",

Lemstra P.J. and Kleintjens L.A. eds., Elsevier Applied Science Pu. 1988

35. Nies E.; Stroeks A. in "Integration of Polymer Science and Technology-3",

Lemstra P .J. and Kleintjens L.A. eds., Elsevier Applied Science Pu. 1989

36. Scholte Th.G.; Eur.PoLJ. 1970, 6, 1063

37.Scholte Th.G.; J.Polym.Sci. Part A2 1970, 8, 841

38. Scholte Th.G.; J.Polym.Sci. Part A2 1971, 9, 1553

39. Scholte Th.G.; J.Polym.Sci. C 1972, 39, 281

40. Stroeks A.; Paquaij R.; Nies E. accepted by Polymer

41. Chandler P. Studies in Statistical Mechanics, Montroll EW and Lebowitz JL

Eds., North-Holland Publishing Co., Amsterdam 1982 Vol.VIII

42. Schweizer K.S.; Curro J.G. Phys.Rev.Lett. 1987, 58, 246

43. Curro J.G~; Schweizer K.S. Macromolecules 1987, 20, 1928

44. Hirschfelder J.O.; Curtiss E:F.; Bird R.B. The Molecular Theory of Gases and

Liquids, Wiley, New York 1954

45.Clayton G.T.; Heaton LeRoy Phys.Rev. 1961,121,649

46. Jones J.E.; Ingham A.B. Proc.R.Soc.London 1925, Al07, 636

47. Flory P.J. J.Chem.Phys. 1944 , 1~11, 425

48. Huggins M.L. J.Phys.Chem. 1942, 46, 151

49. Huggins M.L. Ann.N. Y .A cad. Sci. 1943, 44, 431

50. Freed K.F.; Bawendi M.G. J.Chem.Phys. 1989, 93, 2194

51. Okamoto H. J.Chem.Phys. 1979, 70, 1690

52. Bellemans A.; DeVos E. J.Polym.Sci. C Polym.Symp. 1973, 42, 1195

53. Dickman R.; Hall C.K. J.Chem.Phys. 1986, 85, 3023

54. Irvine P.; Gordon M. Macromolecules 1980, 13, 761

55. Patterson D. J.Polym.Sci. C 1968, 16, 3379

56. Patterson D. Macromolecules 1969, 2, 672

References 1~

57. Patterson D.; Delmas G. Disc. Faraday Soc. 1970, 49, 98

58. Biros J.; Zeman L; Patterson D. Macromolecules 1971, 4, 30

59.Zeman L; Biros J.; Delmas G.; Patterson D.J.Phys.Chem. 1972, 76, 1206

60. Zoller P. in Polymer Handbook Brandrupp J. and lmmergut E.H. eds. Wiley

New York 1989 3ro Ed.

61. Olabisi 0.; Simha R. Macromolecules 1975, 8, 205

62. Walsh D.J. Central Research & Development Dept., E.I. duPont de Nemours

&Co., Wilmington DE private communication

63. Hillegers L T.M.E., The estimation of parameters in functional relationship

models, Dissertation Eindhoven Univ. Technology, The Netherlands 1986

64.Dymond J.H.; Young K.J.; Isdale J.D. J.Chem.Thermodyn. 1979,11, 887

65. Jonas J.; Hasha D.; Huang S.G. J.Phys.Chem 1980, 84, 109

66. Kamagai A.; Iwasaha H. J.Chem.Eng.Data 1978, 23, 193

67. Internal measurement

68. Prigogine I.; Defay R. Chemical Thermodynamics Longmans and Green,

London 1954

69. Sanchez I.C.; Balasz A.C. Macromolecules 1989, 22, 2325

70. Sanchez I. C. in Polymer Blends, Daul D.P. and Newman S. Eds. Academic

Press; New York 1978 Vol.I

71. McMaster LP. Macromolecules 1973, 6, 760

72. Wolf B.A.; Geerissen H. Colloid Polym.Sci. 1981, 259, 1214

73. Saeki S.; Kuwahara N.; Nakata M.; Kaneko M. Polymer 1975, 16, 445

74. Hocker H.; Shih H.; Flory P.J. Trans.Faraday Soc. 1971, 67, 2275

75.Hocker H.; Blake G.J.; Flory P.J. Trans.Faraday Soc. 1971, 67, 2251

76. Sanchez I. C.; Lacombe R.H. Polym.Lett.Ed. 1977, 15, 71

77. Koningsveld R.; Kleintjens LA.; Schultz A.R. J.Polym.Sci. Part A2 1970, 8,

1261

78. Szleifer I. J.Chem.Phys., 1990, 92, 6940

79. Kubota K.; Abbey K.M.; Chu B. Macromolecules 1983, 16, 137

80. van Dijk F.; Wakker A Koninklijke/Shell Lab. Amsterdam, private

communication

81. Myrat C.D.; Rowlinson J.S. Polymer 1965, 6, 645

166 Chapter 10

82. Zeman L.; Patterson D. J.Phys.Chem. 1972, 76, 1214

83. Haase R. Thermodynamik der Mischphasen, Springer Verlag Berlin 1956

84. Wolf B.A. Johannes-Gutenberg UniversiHit, Mainz, FRG, private

communication

85. Guggenheim E.A. Mixtures Clarendon Press, Oxford 1952

86. Koningsveld R. Br.PoLJ. 1975, 7, 435

87. Debeye P. J.Chem.Phys. 1959, 31, 680

88. Koningsveld R.; Stockmayer W.H.; Kennedy J.W.; Kleintjens L.A.

Macromolecules 1974, 7, 73.

89. Kambour R.P.; Bopp R.P.; Maconnachie A.; MacKnight W.J. PoLComm.

1980, 21' 133

90. Shibayama M.; Yang H.; Stein R.S.; Han Ch.C. Macromolecules, 1985, 18,

2179

91. Jelinic J.; Kirste R.G.; Oberthiir R.C.; Schmitt-Strecker S.; Schmitt B.J.

Makromol.Chem. 1984, 185, 129

92. Hadziioannou G.; Stein R.S. Macromolecules 1984, 17, 567

93.Jung W.G.; Fischer E.W. MakromoLChem. MacromoLSymp. 1988, 16, 281

94. Walsh D.J.; Dee G.T.; Halary J.C.;. Uhrich J.M.; Millequant M.; Lesec J.;

Monnerie L. Macromolecules 1989, 22, 3395

95. Suzuki Y.; Miyamoto Y.; Asai K. J.Polym.Sci. PoLLett.Ed. 1982, 20, 563

96. Rostami S.; Walsh D.J. Macromolecules 1984, 17, 315

97. Lin J.L.; Roe R.J. Polymer 1988, 29, 1227

98. Lang S.; Sillescu H. MakromoLChem. 1989, 190, 797

99. Lang S. Dissertation 1986, Johannes-Gutenberg Universitat, Mainz, FRG

100.Cruz C.A.; Paul D.R.; Barlow J.W. JAppl.Polym.Sci. 1979, 23, 589

101.Walsh D.J.; Higgins J.S.; Rostami S.; Weeraperuma K.Macromolecules 1983,

16, 391

102.Tager A.A.; Bessonov YuS Vysok.Soed. 1975, A17, 2383

103.1chihara 1.; Komatsu A.; Hata T Polym.J. 1971, 2, 640

104.Karasz F.E.; MacKnight W.J. Pure AppLChem. 1980, 52, 409

105.Zoller P.; Hoehn H.H. J.Polym.Sci Pol.Phys.Ed. 1982, 20, 1385

106.Li Y.; Wold M.; Wendorff J.H. PoLComm. 1987, 28, 265

References 167

107.Wolf M.; Wendorff J.H. Polymer 1989, 30, 1524

108.Tsujita Y.; Iwakiri K.; :Kiqoshita T.; Takizawa A J.Polym.Sci. Pol.Phys.Ed.

1991, 415

109.Sato T.; Tsujita Y.; Takizawa A; Kinoshita T. Macromolecules 1991, 24, 158

168 Future Outlook

Future Outlook

The hole theories in this thesis are based on the assumptions of random

mixing and of pure dispersive interactions. This limits the application of these

theories because for many polymer systems these conditions are not fulfilled.

Other kinds of interaction might be involved, like hydrogen bonding, dipole

dipole or other charge induced interactions. A theoretical extension in the

combinatoric& and the energetics is desirable to describe equilibrium

thermodynamic properties of these systems. At the moment efforts in this

direction are undertaken by H.Xie and E.Nies at Eindhoven University of

Technology.

Furthermore I hope that this thesis challenges experimentalists to improve

the excess function measurements of especially polymer blends. This is important

for the understanding of miscibility behaviour and its relation with pressure.

Summary

Summary

In this thesis the miscibility behaviour and related properties of polymer

systems in thermodynamic equilibrium are studied in the framework of the so

called hole theories. A representative of these theories is the Simha-Somcynsky

(SS) model which has proven to be very successful in the description of

equilibrium thermodynamic properties of pure polymer components. Therefore

it forms a solid basis for the theoretical study of these properties for polymer

solutions and polymer blends.

In chapter 2 the theoretical background of the SS theory is presented and its

relation with other equation of state models is elucidated. In the SS theory two

volume mechanisms are operational. Macroscopic volume changes of a system

are determined theoretically by a variation in the size of occupied cells and by

a change in the number of vacant sites. This feature distinguishes the SS theory

from other equation of state theories in which only one of these two volume

mechanisms is active. The original Simha-Somcynsky theory is modified by a

replacement of the occupied site fraction by an external contact fraction in the

relevant expressions. This modified version is called the Holes and Huggins

(HH) theory.

Pure components in the SS and HH theories are characterized by four

molecular constants which are quantified by a fit of equilibrium equation of

state data. In comparison with most other equation of state models, the SS and

HH theories give numerically superior fits which is an indication for the validity

of the assumptions underlying these theories. The modified hole theory models

a polymer component differently than the original SS theory. A less dense

structure, i.e. a larger fraction of vacant sites, is suggested (see chapter 3).

Jain and Simha applied the SS hole theory to investigate the miscibility

behaviour of polymer solutions. In this study, the compositional derivatives of the

170 Summary

free energy of mixing, relevant for the description of phase behaviour, were

approximated by polynomial fits to the theoretical free energy. Instead, in this

thesis exact expressions for these derivatives are computed. In chapter 4 the

exact and approximate procedures are compared for the case polyethylene/n

hexane , considered by Jain and Simha. · The LCST (lower critical solution

temperature) demixing behaviour is governed by an iso-free volume principle.

The critical conditions are characterized by an invariant site free volume

difference over a moderate pressure range which is a clear indication that LCST

phase behaviour is governed by free volume. Rather large deviations occur

between "exact" and "approximate" chemical potentials and spinodals which can

be attributed to the earlier mentioned fit in the approximate version.

· The solution polystyrene/cyclohexane is investigated (chapter 5) because a

wealth of experimental information concerning miscibility related properties is

available in literature. Both SS and HH theories are capable in describing and

predicting the UCST (upper critical solution temperature) and LCST miscibility

behaviour under atmospheric conditions. However, important differences

between both theories emerge if one is interested in the influence of pressure.

The HH theory is very successful in predicting these subtle and complex pressure

phenomena observed for UCST phase behaviour. The SS theory fails to predict

these effects. Furthermore in chapter 5 the HH theory is confronted with phase

equilibrium data of the solution polystyrenefmethylacetate. With an adapted

value of the segmental polystyrene size, one is in a position to describe UCST

and LCST type of phase behaviour. The pressure influence on both types of

phase behaviour is predicted in a satisfactory manner.

In chapter 6 we have presented an alternative and original correlation

between pressure effects on phase behaviour and thermodynamic excess

functions for the system polystyrene/cyclohexane. According to the HH theory,

these pressure influences are related with a change in the local curvature of the

excess volume and not with a change of sign as suggested in literature. This

conclusion is supported by experimental excess volume data of Wolf. The

Summary 171

predicted change of local curvature is the result of a delicate interplay between

the two theoretical types of volume mechanisms, i.e. the vacancy free volume

and the cell volume contributions.

Flory Huggins x-parameters are frequently used to express miscibility related

properties of polymer systems. In chapter 7 x-parameters are presented which

are generated with the SS and HH theories. Different theoretical contributions

to these parameters are studied separately. UCST miscibility is mainly motivated

by energetic factors whereas LCST miscibility is induced by free volume aspects.

This outcome does not provide basic new concepts for the interpretation of

polymer phase behaviour because similar conclusions have been drawn in the

past based on other equation of state models. This study however provides more

insight in the balance between the theoretical factors related to phase behaviour.

Theoretically and experimentally determined x-parameters are compared for the

solution polystyrene/ cyclohexane. In the vicinity of the UCST a good agreement

is obtained, at elevated temperatures deviations occur and a too large

temperature dependence is predicted.

Computations presented in chapter 8 concerning miscibility behaviour of a

hypothetical polymer model blend indicate that the SS and HH theories are

capable in describing the general observed effects encountered in studies of

polymer blend miscibility. These effects include a transition from UCST to LCST

miscibility behaviour with increasing molar mass of the constituents. This is a

generally observed phenomena; partial miscible oligomer blends frequently

exhibit UCST type of demixing whereas high molar mass polymer blends

generally demix at elevated temperatures (LCST). A difference in molar masses

of the pure constituents is reflected in an asymmetry of the spinodal curves. Just

as in the case of the solution polyethylene/n-hexane an iso-site free volume

principle governs LCST miscibility. Its application however is limited and only

correct when the other theoretical volume mechanism, i.e. variation in cell size,

is not operational as is the case for the polyethylenejn-hexane system. One of

the very rare studies in literature dealing with pressure effects on miscibility of

172 Summary

polymer blends, reveals a complicated pressure effect. Cloud points of the blend

poly(vinylidenefluoride)/poly(ethylacrylate) exhibit a tilting effect with pressure.

A similar tilting effect for the spinodal is obtained with the SS and HH theories

for a hypothetical model blend when both volume mechanisms are operational.

Miscibility behaviour of the blend polystyrene/poly(paramethylstyrene) is

investigated on an experimental and theoretical basis. The DSC and the phase

contrast optical microscopy techniques reveal UCST miscibility behaviour which

is quite exceptional for high molar mass blends. The HH theory predicts this

type of phase behaviour. This blend does not show phase separation at elevated

temperatures because of the similarity of the site free volume fractions of both

components.

Samenvattlng 173

Samenvatting

In dit onderzoek is bet verschijnsel mengbaarbeid van polymere systemen

bestndeerd en gerelateerd aan tbermodynamiscbe grootheden in bet kader van

de wgenaamde "hole"-tbeorieen. Een vertegenwoordiger van deze theorieen is

bet Simba-Somcynsky model, dat zeer succesvol is in de bescbrijving van

tbermodynamiscbe eigenscbappen onder evenwichtscondities van zuivere

polymeren. Zodoende vormt deze tbeorie een solide basis voor de bestndering

van deze eigenscbappen van polymere multicomponent systemen.

In boofdstuk 2 worden de theoretiscbe acbtergronden van de Simha

Somcynsky roostertheorie gepresenteerd en wordt de relatie met andere

roostermodellen toegelicbt. In de Simba-Somcynsky theorie zijn twee

volumemechanismenoperationeel.Macroscopischevolumeveranderingenvaneen

systeem worden theoretiscb gerealiseerd door middel van een variatie in de

grootte van bezette roosterplaatsen en door een verandering in bet aantal

vacatureplaatsen. Dit feit onderscbeidt de Simba-Somcynsky theorie van de

andere roostermodellen waarin slecbts een volumemecbanisme aktief is. De

originele Simba-Somcynsky tbeorie is gemodificeerd door middel van de

vervanging van de bezette roosterplaatsfractie door een exteme contactfractie in

de relevante uitdrukkingen. Deze gemodificeerde versie wordt aangeduid met de

Holes en Huggins theorie.

Ben zuivere component in de Simha-Somcynsky en Holes and Huggins

theorieen wordt bescbreven door vier moleculaire constanten die bepaald

worden via een bescbrijving van druk-volume-temperatuur data onder

evenwicbtscondities van de desbetreffende component. In vergelijking met

andere modellen genereren de Simba-Somcynsky en Holes and Huggins

theorieen superieure fits, betgeen een indicatie is voor de geldigheid van de

aannamen die ten grondslag liggen aan deze tbeorieen. De gemodificeerde

theorie modelleert een zuiver polymeer anders dan de originele Simba-

174 Samenvatting

Somcynsky versie. Een minder dicbte struktuur wordt gesuggereerd betgeen een

grotere fractie vacatureplaatsen inhoudt.

Jain en Sirnha pasten als eersten de Sirnha-Somcynsky theorie toe op bet

ontmenggedrag van polymere oplossingen. Zij benaderden de

samenstellingsafgeleiden van de Gibbs vrije energie, relevant voor de

bescbrijving van bet fasegedrag, door deze vrije energie te scbrijven als een

polynoom in de samenstelling. In dit proefscbrift daarentegen worden exacte

uitdrukkingen voor deze afgeleiden gebruikt. In boofdstuk 4 worden de exacte

en benaderende procedures met elkaar vergeleken voor de oplossing

polyetbeen/n-bexaan. Het LCST (lower critical solution temperature) type

ontmenggedrag (fasescbeiding optredend bij temperatuurverboging) wordt

bebeerst door een iso-vacature vrij volume principe. De kritische

ontmengcondities worden gekarakteriseerd door een invariant vrij volume

verscbil over een groot docb beperkt drukgebied betgeen een duidelijke

aanwijzing is dat LCST ontmenggedrag vrij volume geinduceerd is. Nogal grote

afwijkingen treden op tussen "exacte" en "benaderde" cbemiscbe potentialen en

spinodalen betgeen is toe te · scbrijven aan bet gebruik van de eerder

polynoomuitdrukking.

Het systeem polystyreen/cyclobexaan is uitvoerig onderzocbt omdat in de

literatuur uitgebreide informatie aanwezig is omtrent bet ontmenggedrag van dit

systeem. Zowel de Simba-Somcynsky als de Holes and Huggins theorie zijn in

staat bet waargenomen LCST ontmenggedrag en UCST (upper critical solution

temperature) type fasegedrag ( fasescheiding bij een temperatuurverlaging) onder

atmosferische condities te beschrijven en te voorspellen. Duidelijke verscbillen

tussen beide modellen manifesteren zich echter als de invloed van druk op bet

fasegedrag bestudeerd wordt. De Holes and Huggins theorie is zeer succesvol in

de voorspelling van deze subtiele en tevens complexe drukinvloed op UCST

ontmenging. De Simha-Somcynsky theorie daarentegen faalt in de voorspelling

van dit effect. Verder wordt in hoofdstuk 5 de Holes and Huggins theorie

geconfronteerd met het ontmenggedrag van de oplossing

SamenvaUing 175

polystyreenjmethylacetaat. Met een aangepaste waarde van de styreen

segmentgrootte kan UCST en LCST type ontmenging beschreven worden.

Verder wordt de drukinvloed op beide vormen van ontmenggedrag redelijk ·

voorspeld.

In boofdstuk 6 is op een altematieve manier de drukinvloed op ontmenging

gecorreleerd aan thermodynamiscbe exces-functies van bet systeem

polystyreen/ cyclobexaan. Volgens bet Holes and Huggins model is de complexe

invloed van druk gerelateerd aan een locale verandering van de kromming van

bet exces-volume van bet desbetreffende systeem en niet aan een

tekenverandering van bet exces-volume, wals in de literatuur is gesuggereerd.

Deze conclusie wordt gesteund door exces-volume metingen volgens Wolf. De

voorspelde krommingsverandering is bet gevolg van bet delicate samenspel

tussen de twee eerder genoemde volumemecbanismen.

Flory Huggins x-parameters worden frequent toegepast om aan ontmenging

gerelateerde grootheden uit te drukken. In boofdstuk 7 zijn x-parameters

gepresenteerd, berekend volgens de Simha-Somcynsky en Holes and Huggins

tbeorieen. Ben studie naar de verscbillende tbeoretiscbe bijdragen leidt tot de

conclusie dat UCST ontmenging grotendeels gemotiveerd wordt door

energetiscbe factoren. LSCT ontmenggedrag daarentegen is vrij volume

geinduceerd. Dit resultaat Ievert geen wezenlijk nieuwe concepten omdat in bet

verleden vergelijkbare conclusies zijn geformuleerd op basis van andere

modellen. Deze studie geeft ecbter wei meer inzicbt in de balans tussen de

verscbillende tbeoretische factoren die van belang zijn voor ontmenging van

polymeersystemen. Theoretiscb en experimenteel bepaalde x-parameters zijn

vergeleken voor bet systeem polystyreenjcyclobexaan. In de nabijbeid van de

UCST wordt een goede overeenstemming bereikt. Bij verboogde temperatuur

treden afwijkingen op en wordt een te grote temperatuurafhankelijkbeid van de

x-parameter voorspeld.

176 SamenvaUing

In boofdstuk 8 wordt aangetoond dat de Simha-Somcynsky en Holes and

Huggins tbeorieen in staat zijn de algemene ontmengeffecten te bescbrijven die

optreden voor polymeermengsels. Zo wordt theoretiscb voor een bypotbetiscbe

modelblend een overgang waargenomen van UCST naar LCST ontmenggedrag

met toenemende molekuulmassa van de zuivere componenten. Dit fenomeen

wordt experimenteel vrij algemeen waargenomen; gedeeltelijk mengbare

oligomeermengsels vertonen vaak UCST type omtmenging terwijl

boogmoleculaire blends meestal ontmengen bij een. verboogde temperatuur

(LCST). Net als in bet geval van polyetheen/n-bexaan wordt in bet geval van

boogmoleculaire mengsels bet LCST ontmenggedrag bebeerst door een iso-vrij

volume principe. Het blijkt dat dit principe aileen toepasbaar is indien bet

andere volume mecbanisme (variatie van de grootte van de roosterplaats) niet

operationeel is. In de litetatuur is weinig bekend over de drukinvloed op de

fasescbeiding van boogmoleculaire mengsels. Ben van de scbaarse studies wijzen

uit dat dit effect zeer gecompliceerd kan zijn. Vlokpuntcurves van de blend

poly(vinylideenfluoride)/poly(etbylacrylaat) vertonen een tilting effect met

toenemende druk. Dit boudt in dat, afhankelijk van de samenstelling, de

mengbaarbeid verbetert of verslecbtert. Ben vergelijkbaar effect voor spinodale

curven wordt voorspeld door de Simha-Somcynsky en Holes and Huggins

theorieen mits beide volumemecbanismen operationeel zijn.

Het ontmenggedrag van de blend polystyreenjpoly(parametbylstyreen) is zowel

theoretiscb als experimenteel onderzocbt. De DSC tecbniek en fase contrast

optiscbe microscopie tonen UCST ontmenggedrag aan, betgeen zeer

uitzonderlijk is voor boogmoleculaire blends. Dit gedrag wordt voorspeld door

de Holes and Huggins tbeorie. Het mengsel ontmengt niet bij verboogde

temperaturen, betgeen wei gebruikelijk is voor partieel mengbare

polymeermengsels. Reden biervoor is bet relatief kleine verscbil in vrij volume

van de zuivere componenten.

Nomenclature 177

Nomenclature

A repulsive energy constant in Lennard-Jones interaction potential

[=1.011]

A : Helmholtz free energy (Jfmol)

~: Helmholtz free energy of mixture (Jfmol)

B attractive energy constant in Lennard-Jones interaction potential

[=1.2049]

Eo: EO:

E(O):

E(r):

Er :

Er :

FV:

f

fi :

fo :

.AG:

o=: ·oi:

Gm:

AGW: g

8r H

constant in van der Waals interaction energy expression

total number of external degrees of freedom per molecule

total number of external degrees of freedom per segment

energy of a system at rest (J /mol)

energetic contribution (see chapter 7)

potential energy of wanderer at the central position in its cell

(Jfmol)

potential energy of wanderer at position r in its cell (Jfmol)

energy of a system in quantum stater (J/mol)

energy of a system in energy level r (J /mol)

cell free volume contribution (see chapter 7)

fraction of occupied sites

fraction of occupied sites of species i

fraction of vacant sites

Gibbs free energy of mixing (Jfmol)

excess Gibbs free energy (Jfmol)

Gibbs free energy of component i

Gibbs free energy of the mixture (Jfmol)

Gibbs free energy of mixing (J/g)

statistical number of arrangements related to the permutations of

vacant and occupied sites

degeneration of energy level r of a system

Enthalpy (J/mol)

178

H:

HUG:

h

h

M: Mo:

~:

m

N:

p :

p*: -p

Hamiltonian (J/mol)

excess enthalpy (Jfmol)

enthalpy of mixing (Jfmol)

enthalpy of solution (Jfmol)

Huggins contributio1,1 (see chapter 7)

free site fraction

Planck constant (Js)

excess free site fraction

derivative in critical condition

derivative in spinodal condition

Boltzmann constant (J/K)

molar mass (kg/mol)

segmental molar mass (kg/mol)

molar mass of species i (kg/mol)

number averaged molar mass (kg/mol)

weight average molar mass (kg/mol)

mass per molecule (kg)

number of molecules in system

Avogadro number (1/mol)

number of vacant cells

total number of lattice sites

pressure (bar)

pressure scaling parameter (bar)

reduced pressure

Nomenclature

Pi momentum corresponding to the centre of mass of the i'th molecule

(kg m/s)

Q auxiliary variable ( = yV /V*)

q contact fraction

q hard core volume correction factor

R gas constant (J/(molK))

r intersegmental or intermolecular distance (m)

r* distance corresponding to minimum in Leonard-Jones curve (m)

Nomenclature 179

s SFH:

SHH:

S; :

S.o • I •

T:

T*:

f: TE:

u v V*:

v: VAC: v-=:

X

XAB:

X;: Xr:

position corresponding to the centre of mass of the i'th molecule (m)

surface area per segment (m2fmol)

Entropy (J/(molK))

Flory Huggins combinatorial entropy contribution (see chapter 7)

combinatorial term in SS and HH theory (see chapter 7)

number of occupied cells per molecule

parameter indicative for quality of pVT-fit

number of occupied· sites per molecule i

number of occupied sites per molecule i in the pure state

absolute temperature (K)

scaling temperature (K)

reduced temperature

translational energy term (see chapter 7)

potential energy of the system (J/mol)

macroscopic volume of system (m3fmol)

macroscopic volumetric scaling parameter (m3/mol)

macroscopic reduced volume

vacancy contribution (see chapter 7)

excess molar volume (m3/mol)

macroscopic volume of mixture (m3/mol)

specific volume of mixture (m3 /mol)

volume corresponding to the minimum in the Lennard-lones

interaction potential (m3fmol)

excess specific volume (m3fbase mol)

cell partition function or cell free volume (m3/mol)

reduced cell free volume

specific volume of component i (m3/mol)

weight fraction of component i

Energetic mixing parameter

Flory Huggins interaction parameter

base mole fraction of component i

site fraction of component i

180

X

y

y

£ :

£* :

P;

aP

aT:

av:

~i :

II'; : .... o • "'• .

Composition variable

volumetric mixing parameter

occupied site fraction

excess occupied site fraction

partition function or sum-over-all-states

Nomenclature

contribution from compressibility factor (see chapter 7)

configurational partition function

translational partition function

coordination number ( = 12)

thermal expansion coefficient (1/K)

auxiliary variable [ = 1(1-1/s)]

thermal pressure coefficient (N/(m2J<:))

auxiliary variable [ =2/z]

configurational partition function directly related to G

pair interaction energy (J /mol)

interaction energy corresponding to the minimum in the Lennard

lones interaction potential (J/mol)

auxiliary variable [ = 2·1/6 (1-a)y(yV /V*)"113)/(1-ay)]

fraction of the surface area for molecules i

auxiliary variable [ = h/((2Dmk:T)1f2)]

chemical potential of component i (J/mol)

standard deviation in pressure (bar)

standard deviation in temperature (K)

standard deviation in volume (m3 /mol)

volume fraction of component i

segment fraction of component i

volume fraction of component i

Flory Huggins interaction parameter

enthalpic part of FH interaction parameter

enthalpic part of "scattering" FH interaction parameter

entropic part of the FH interaction parameter

"scattering" FH interaction parameter

Nomenclature 181

Xsne,-1: non-combinatorial entropic part of the "scattering" FH interaction

parameter

x,. "chemical potential" FH interaction parameter

t reduced cell partition function per three external degrees of freedom

jJ reduced cell partition function per three internal degrees of freedom

w cell volume (m3 /mol) -w reduced cell volume

182 Dankwoord

Dankwoord

Allereerst wil ik Erik Nies bedanken, niet alleen voor zijn deskundige raad

maar tevens voor zijn collegialiteit en zijn nimmer aflatende enthousiasme

waardoor hij anderen steeds weer weet te motiveren. Zonder overdrijving kan

gesteld worden dat zonder zijn inbreng dit proefschrift niet tot stand was

gekomen.

Many thanks to Prof.R.Simha for his wise remarks, critical comments and for

his wide interest, which is not solely restricted to polymers but also includes

personal interest which makes collaboration very pleasant. The work of

Prof.R.Simha forms the inspiration and the basis for this thesis.

Raymond Paquaij wil ik vooral bedanken voor zijn experimentele inbreng,

daar waar bet de blend PS/PpMeS betreft. Na maandenlang stug doormeten

en synthetiseren kregen we uiteindelijk toch vat op bet ontmenggedrag van dit

systeem.

I am grateful to Prof.B.A Wolf for the release of his unpublished excess

volume data on the solution PS/CH.

Dr.A Wakker ben ik erkentelijk voor de ontmenggegevens van bet systeem

PS/MeAc.

Ik dank W.Kingma voor de GPC metingen en P.Piet voor de inwijding in de

anionische synthese.

Verder dank ik aile medewerkers en studenten van de vakgroep

Kunststoftechnologie voor de plezierige sfeer en de prettige samenwerking.

Dit onderzoek werd financieel mogelijk gemaakt door NWO/SON, waarvoor

grote erkentelijkheid.

Curriculum Vitae 183

Curriculum Vitae

De auteur van dit proefschrift werd op 18 september 1963 geboren te Heerlen.

Van 1975 tot 1981 bezocht hij de Stella Maris Scholengemeenschap (Atheneum

IJ) te Meerssen. Aansluitend begon hij in september 1981 de studie Scheikundige

Technologie aan de Technische Universiteit Eindhoven (TUE). Het

propedeutisch diploma werd in juli 1982 behaald en bet kandidaatsexainen in juli

1984. Als "research scholar" was de auteur werkzaam aan de Case Western

Reserve University, Cleveland, Ohio (USA) van december 1985 tot mei 1986. Na

een afstudeerprojek.t, dat gedeeltelijk werd uitgevoerd bij DSM Research te

Geleen en bij de vakgroep Kunststoftechnologie aan de TUE, behaalde hij bet

ingenieursdiploma in april 1987. In mei 1987 startte hij zijn promotieonderzoek

en sindsdien is hij werkzaam als vierjarige assistent in opleiding bij de eerder

genoemde vakgroep. De auteur is winnaar van de Europese Exxon Award 1990.

Per 1 juli 1991 zal hij in dienst treden bij DSM te Geleen.

Stellingen

1. Saeki et al. concluderen op grond van experimentele gegevens dat de afgeleide ( 8T / ap )c onder atmosferische condities van teken verandert met varierende molekuulmassa van bet polymeer in bet systeem polystyreen /cyclobexaan. Hun suggestie dat dit effect gepaard gaat met een tekenverandering van bet exces-volume is onjuist. In boofdstuk 6 van dit proefschrift wordt beschreven dat een verandering van de kromming van bet exces-volume hiermee verband houdt en niet een verandering in bet teken van dit volume.

S.Saeki, N.Ku.wahara, M.Nakata, M.Kaneko; Polymer 197516, 445

2. De wijdverbreide gedachte dat specifieke interaktie, zoals waterstofbrugvorming of dipool-dipool interaktie, noodzakelijk is om een polymeermengsel mengbaar te Iaten zijn, wordt tegengesproken door de modelberekeningen gepresenteerd in hoofdstuk 8 van dit proefschrift.

3. De introduktie door Kammer et al. van de afgeleiden (8p/8T) en (lfP/lJV), zoals gedefinieerd volgens de Flory equation of state theorie, in een aangepaste versie van Prigogine's celmodel maakt deze versie inconsistent.

H. W.Kammer, T.Inoue, T.Ougizawa; Polymer 1989 30,888

4. De conclusie van Kyu et al., gebaseerd op FTIR metingen, dat waterstotbrugvorming optreedt in bet systeem PPTA/nylon is voorba-rig.

T.Kyu, T.I.Chen, H.S.Park, J.L. White; l.Appi.Pol.Sci. 1989 37,201

5. Recente neutronenverstrooiingsmetingen hebben aangetoond dat afzonderlijke polymeerkristallen, bereid via gecontroleerde solutieprecipitatie, na opsmelten binnen 1-2 seconden relaxeren naar de "random-coil" configuratie. Dit spreekt de conclnsie van Rudin et aL tegen die beweren dat deze relaxatie langere tijd in beslag neemt dan de karakteristieke tijden voor verwerking in de smelt.

P J.Barham, D.M.Sadler; Polymer 1991 32, 393 AAjj~ P J.Carreau, H.P.Schreiber, A.Rudin; J.Pol.Sci. Part B 1986 24, 1983

6. Een onderbelicht aspect bij de studie van mengbaarheid van polymeermengsels via intrinsieke excimer fluorescentie is het feit dat excimerformatie de mengbaarheid kan beinvloeden.

Y.Zhao, D.Z.Ma, R.E.Prud'homme; Polymer 199132,791

7. De samenstelling van benzine geeft aanleiding om beschermende maatregelen te treffen ten aanzien van het tanken bij benzinestations.

8. Indien een atletiekwedstrijd aan de binnenkant van de baan met een pistoolschot wordt gestart, is het gezien de snelheid van het geluid niet fair om op een honderdste van een seconde te klokken.

9. De te verwachten levensduur van een promovendus is Ianger dan die van de Nederlander in het algemeen.

Alexander Stroeks, Eindhoven, 21 mei 1991